#------------------------------------------------------------------------------
#$Date: 2025-07-01 14:33:24 +0300 (Tue, 01 Jul 2025) $
#$Revision: 1290 $
#$URL: svn://crystallography.net/testcod/cif/4/10/00/4100021.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4100021
loop_
_publ_author_name
'Tenailleau, Christophe'
'Allix, Mathieu'
'Claridge, John B.'
'Hervieu, Maryvonne'
'Thomas, Michael F.'
'Hirst, James P.'
'Rosseinsky, Matthew J.'
_publ_section_title
;
 Modular Construction of Oxide StructuresCompositional Control of
 Transition Metal Coordination Environments
;
_journal_issue                   24
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7570
_journal_page_last               7583
_journal_paper_doi               10.1021/ja077762f
_journal_volume                  130
_journal_year                    2008
_chemical_formula_sum            'Ba0.81 Ca0.78 Fe2.5 Nd0.91 O6.43'
_chemical_formula_weight         516.38
_space_group_IT_number           74
_space_group_name_Hall           '-I 2b 2'
_space_group_name_H-M_alt        'I m m a'
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_H-M   'I m m a'
_audit_creation_date             2006-07-11T13:11
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2006-07-11T13:11  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            8
_cell_length_a                   5.58392(17)
_cell_length_b                   38.9909(11)
_cell_length_c                   5.61065(18)
_cell_volume                     1221.56(6)
_computing_structure_refinement  GSAS
_diffrn_radiation_probe          neutron
_diffrn_radiation_wavelength     1.59432
_exptl_absorpt_correction_T_max  0.99994
_exptl_absorpt_correction_T_min  0.99994
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 Debye-Scherrer absorption correction
Term (= MU.r/wave) =     0.23465E-04
Correction is not refined.
;
_pd_block_id                     2006-07-11T13:11|FINAL|J_B_Claridge|D2B
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.05
_pd_meas_2theta_range_max        159.9
_pd_meas_2theta_range_min        0.1
_pd_meas_number_of_points        3197
_pd_phase_name
'from C:/Documents and Settings/Titia.LEGOUPILOU/Bureau/John 10L re'
_pd_proc_2theta_range_inc        0.05
_pd_proc_2theta_range_max        160.0385
_pd_proc_2theta_range_min        0.2385
_pd_proc_info_datetime           2006-07-11T13:11:28
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 18 terms.
 Shifted Chebyshev function of 1st kind
      1:    310.382     2:   -52.7215     3:    66.9665     4:   -3.99233    
      5:    10.0767     6:   -3.48285     7:    6.54671     8:   -1.32499    
      9:   -1.24653    10:   -1.66635    11:   -1.04321    12:    3.87201    
     13:    1.39639    14:   -3.20318    15:    7.46634    16:   0.230802    
     17:   -3.89285    18:    4.25531    
;
_pd_proc_ls_peak_cutoff          0.00050
_pd_proc_ls_profile_function
;
 CW Profile function number 2 with  18 terms
 Profile coefficients for Simpson's rule integration of pseudovoigt function
 C.J. Howard (1982). J. Appl. Cryst.,15,615-620.
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 #1(GU)   =   95.187 #2(GV)   = -269.744 #3(GW)   =  263.389
 #4(LX)   =    9.814 #5(LY)   =    0.000 #6(trns) =    0.000
 #7(asym) =  11.3744 #8(shft) =   0.0000 #9(GP)   =    0.000
 #10(stec)=     0.00 #11(ptec)=     0.00 #12(sfec)=     0.00
 #13(L11) =    0.000 #14(L22) =    0.000 #15(L33) =    0.000
 #16(L12) =    0.000 #17(L13) =    0.000 #18(L23) =    0.000
 Peak tails are ignored  where the intensity is below 0.0005 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0382
_pd_proc_ls_prof_wR_expected     0.0169
_pd_proc_ls_prof_wR_factor       0.0539
_pd_proc_number_of_points        3197
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   3.23
_refine_ls_matrix_type           full
_refine_ls_number_parameters     63
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.09473
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        0.822
_reflns_d_resolution_low         6.498
_reflns_limit_h_max              6
_reflns_limit_h_min              0
_reflns_limit_k_max              48
_reflns_limit_k_min              0
_reflns_limit_l_max              6
_reflns_limit_l_min              0
_reflns_number_total             655
_cod_data_source_file            ja077762f-file004.cif
_cod_data_source_block           FINAL_publ
_cod_original_cell_volume        1221.56(5)
_cod_original_formula_sum        'Ba0.81 Ca0.78 Fe2.50 Nd0.91 O6.43'
_cod_database_code               4100021
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000
loop_
_symmetry_equiv_pos_site_id
_symmetry_equiv_pos_as_xyz
1 +x,+y,+z
2 -x,+y,+z
3 +x,-y+1/2,+z
4 -x,-y+1/2,+z
-1 -x,-y,-z
-2 +x,-y,-z
-3 -x,+y+1/2,-z
-4 +x,+y+1/2,-z
101 +x+1/2,+y+1/2,+z+1/2
102 -x+1/2,+y+1/2,+z+1/2
103 +x+1/2,-y,+z+1/2
104 -x+1/2,-y,+z+1/2
-101 -x+1/2,-y+1/2,-z+1/2
-102 +x+1/2,-y+1/2,-z+1/2
-103 -x+1/2,+y,-z+1/2
-104 +x+1/2,+y,-z+1/2
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_thermal_displace_type
_atom_site_U_iso_or_equiv
_atom_site_symmetry_multiplicity
Fe Fe1 0.0 0.05002(19) 0.5049(18) 1.0 Uiso 0.0155(14) 8
O O1 0.25 0.0397(4) 0.25 1.0 Uiso 0.0290(34) 8
O O3 0.25 0.9611(4) 0.25 1.0 Uiso 0.037(4) 8
Ba Ba2 0.0 0.6021(4) 0.007(4) 0.4063 Uiso 0.0305(25) 8
Ba Ba3 0.0 0.69437(32) -0.015(4) 0.4053 Uiso 0.0219(25) 8
Fe Fe2 0.0 0.15159(21) 0.4983(18) 1.0 Uiso 0.0155(14) 8
Fe Fe3 0.0646(26) 0.25 0.5666(25) 0.5 Uiso 0.026(4) 8
O O4 0.25 0.15207(33) 0.25 1.0 Uiso 0.0065(18) 8
O O5 0.25 0.6615(4) 0.25 1.0 Uiso 0.044(4) 8
O O6 0.25 0.25 0.25 0.24(7) Uiso 0.07(5) 4
O O7 0.356(8) 0.25 0.622(8) 0.5 Uiso 0.053(7) 8
O O8 0.0 0.10012(31) 0.5171(32) 1.0 Uiso 0.0145(20) 8
O O9 0.0 0.2062(4) 0.434(4) 0.81(4) Uiso 0.037(6) 8
Nd Nd1 0.0 0.0 0.0 0.7435 Uiso 0.0248(31) 4
Ca Ca1 0.0 0.0 0.0 0.2565 Uiso 0.0248(31) 4
Nd Nd2 0.0 0.6021(4) 0.007(4) 0.37 Uiso 0.0305(25) 8
Ca Ca2 0.0 0.6021(4) 0.007(4) 0.2236 Uiso 0.0305(25) 8
Nd Nd3 0.0 0.69437(32) -0.015(4) 0.1674 Uiso 0.0219(25) 8
Ca Ca3 0.0 0.69437(32) -0.015(4) 0.4272 Uiso 0.0219(25) 8
loop_
_atom_type_symbol
_atom_type_number_in_cell
_atom_type_scat_length_neutron
_atom_type_scat_source
Ba 6.493 0.5070 International_Tables_Vol_C
Fe 20.0 0.9450 International_Tables_Vol_C
O 51.475 0.5803 International_Tables_Vol_C
Nd 7.273 0.7690 International_Tables_Vol_C
Ca 6.232 0.4700 International_Tables_Vol_C
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Fe1 O1 86.5(4) 1_555 . 2_555 N
O1 Fe1 O3 156.1(7) 1_555 . -1_566 N
O1 Fe1 O3 87.81(13) 1_555 . -2_566 N
O1 Fe1 Ba2 132.88(33) 1_555 . -3_445 N
O1 Fe1 Ba2 132.2(7) 1_555 . 101_445 N
O1 Fe1 Ba2 64.2(5) 1_555 . 101_545 N
O1 Fe1 O8 102.8(6) 1_555 . 1_555 N
O1 Fe1 O3 87.81(13) 2_555 . -1_566 N
O1 Fe1 O3 156.1(7) 2_555 . -2_566 N
O1 Fe1 Ba2 132.88(33) 2_555 . -3_445 N
O1 Fe1 Ba2 64.2(5) 2_555 . 101_445 N
O1 Fe1 Ba2 132.2(7) 2_555 . 101_545 N
O1 Fe1 O8 102.8(6) 2_555 . 1_555 N
O3 Fe1 O3 88.1(4) -1_566 . -2_566 N
O3 Fe1 Ba2 65.1(5) -1_566 . -3_445 N
O3 Fe1 Ba2 64.1(5) -1_566 . 101_445 N
O3 Fe1 Ba2 133.4(6) -1_566 . 101_545 N
O3 Fe1 O8 101.1(6) -1_566 . 1_555 N
O3 Fe1 Ba2 65.1(5) -2_566 . -3_445 N
O3 Fe1 Ba2 133.4(6) -2_566 . 101_445 N
O3 Fe1 Ba2 64.1(5) -2_566 . 101_545 N
O3 Fe1 O8 101.1(6) -2_566 . 1_555 N
Ba2 Fe1 Ba2 69.3(5) -3_445 . 101_445 N
Ba2 Fe1 Ba2 69.3(5) -3_445 . 101_545 N
Ba2 Fe1 O8 51.4(5) -3_556 . 1_555 N
Ba2 Fe1 Ba2 107.9(4) 101_445 . 101_545 N
Ba2 Fe1 O8 53.97(22) 101_445 . 1_555 N
Ba2 Fe1 O8 53.97(22) 101_545 . 1_555 N
Fe1 O1 Fe1 157.3(9) 1_555 . -103_545 N
Fe1 O1 Nd1 97.60(28) 1_555 . 1_555 N
Fe1 O1 Nd1 96.32(31) 1_555 . 103_545 N
Fe1 O1 Ca1 97.60(28) 1_555 . 1_555 N
Fe1 O1 Ca1 96.32(31) 1_555 . 103_545 N
Fe1 O1 Nd1 96.32(31) -103_555 . 1_555 N
Fe1 O1 Nd1 97.60(28) -103_555 . 103_545 N
Fe1 O1 Ca1 96.32(31) -103_555 . 1_555 N
Fe1 O1 Ca1 97.60(28) -103_555 . 103_545 N
Nd1 O1 Nd1 103.9(5) 1_555 . 103_545 N
Nd1 O1 Ca1 0.0 1_555 . 1_555 N
Nd1 O1 Ca1 103.9(5) 1_555 . 103_545 N
Nd1 O1 Ca1 103.9(5) 103_545 . 1_555 N
Nd1 O1 Ca1 0.0 103_545 . 103_545 N
Ca1 O1 Ca1 103.9(5) 1_555 . 103_545 N
Fe1 O3 Fe1 155.0(10) -1_566 . 103_544 N
Fe1 O3 Nd1 97.34(28) -1_566 . 1_565 N
Fe1 O3 Nd1 97.79(32) -1_566 . 103_555 N
Fe1 O3 Ca1 97.34(28) -1_566 . 1_565 N
Fe1 O3 Ca1 97.79(32) -1_566 . 103_555 N
Fe1 O3 Nd1 97.79(32) 103_554 . 1_565 N
Fe1 O3 Nd1 97.34(28) 103_554 . 103_555 N
Fe1 O3 Ca1 97.79(32) 103_554 . 1_565 N
Fe1 O3 Ca1 97.34(28) 103_554 . 103_555 N
Nd1 O3 Nd1 105.1(6) 1_565 . 103_555 N
Nd1 O3 Ca1 0.0 1_565 . 1_565 N
Nd1 O3 Ca1 105.1(6) 1_565 . 103_555 N
Nd1 O3 Ca1 105.1(6) 103_555 . 1_565 N
Nd1 O3 Ca1 0.0 103_555 . 103_555 N
Ca1 O3 Ca1 105.1(6) 1_565 . 103_555 N
Fe1 Ba2 Fe1 69.7(4) -3_556 . 101_454 N
Fe1 Ba2 Fe1 69.7(4) -3_556 . 101_554 N
Fe1 Ba2 Ba2 125.25(25) -3_455 . -103_343 N
Fe1 Ba2 Ba2 55.9(5) -3_455 . -103_344 N
Fe1 Ba2 Ba2 125.25(25) -3_455 . -103_443 N
Fe1 Ba2 Ba2 55.9(5) -3_455 . -103_444 N
Fe1 Ba2 Ba3 128.5(7) -3_455 . 1_555 N
Fe1 Ba2 Fe2 177.6(7) -3_455 . -3_454 N
Fe1 Ba2 Fe2 71.4(5) -3_455 . -3_455 N
Fe1 Ba2 Fe2 110.5(5) -3_455 . 101_454 N
Fe1 Ba2 Fe2 110.5(5) -3_455 . 101_554 N
Fe1 Ba2 O4 146.0(5) -3_566 . -3_565 N
Fe1 Ba2 O4 146.0(5) -3_566 . -4_565 N
Fe1 Ba2 O5 95.4(6) -3_566 . 1_555 N
Fe1 Ba2 O5 95.4(6) -3_566 . 2_555 N
Fe1 Ba2 O8 141.9(6) -3_566 . -3_565 N
Fe1 Ba2 O8 34.9(4) -3_566 . -3_566 N
Fe1 Ba2 O8 88.1(6) -3_566 . 101_454 N
Fe1 Ba2 O8 88.1(6) -3_566 . 101_554 N
Fe1 Ba2 Nd1 53.99(27) -3_566 . 3_555 N
Fe1 Ba2 Ca1 53.99(27) -3_566 . 3_555 N
Fe1 Ba2 Nd2 125.25(25) -3_566 . -103_454 N
Fe1 Ba2 Nd2 55.9(5) -3_566 . -103_455 N
Fe1 Ba2 Fe1 107.9(4) 101_454 . 101_554 N
Fe1 Ba2 Ba2 55.61(18) 101_454 . -103_343 N
Fe1 Ba2 Ba2 54.83(19) 101_454 . -103_344 N
Fe1 Ba2 Ba2 124.0(7) 101_454 . -103_443 N
Fe1 Ba2 Ba2 125.5(8) 101_454 . -103_444 N
Fe1 Ba2 Ba3 126.02(23) 101_454 . 1_555 N
Fe1 Ba2 Fe2 109.1(5) 101_454 . -3_454 N
Fe1 Ba2 Fe2 109.8(5) 101_454 . -3_455 N
Fe1 Ba2 Fe2 70.68(15) 101_454 . 101_454 N
Fe1 Ba2 Fe2 178.2(7) 101_454 . 101_554 N
Fe1 Ba2 O4 90.23(29) 101_454 . -3_565 N
Fe1 Ba2 O4 144.2(8) 101_454 . -4_565 N
Fe1 Ba2 O5 145.6(7) 101_454 . 1_555 N
Fe1 Ba2 O5 94.53(29) 101_454 . 2_555 N
Fe1 Ba2 O8 88.9(5) 101_454 . -3_565 N
Fe1 Ba2 O8 89.2(5) 101_454 . -3_566 N
Fe1 Ba2 O8 34.46(30) 101_454 . 101_454 N
Fe1 Ba2 O8 142.3(5) 101_454 . 101_554 N
Fe1 Ba2 Nd1 53.95(22) 101_454 . 3_555 N
Fe1 Ba2 Ca1 53.95(22) 101_454 . 3_555 N
Fe1 Ba2 Nd2 55.61(18) 101_454 . -103_454 N
Fe1 Ba2 Nd2 54.83(19) 101_454 . -103_455 N
Fe1 Ba2 Ba2 124.0(7) 101_554 . -103_343 N
Fe1 Ba2 Ba2 125.5(8) 101_554 . -103_344 N
Fe1 Ba2 Ba2 55.61(18) 101_554 . -103_443 N
Fe1 Ba2 Ba2 54.83(19) 101_554 . -103_444 N
Fe1 Ba2 Ba3 126.02(23) 101_554 . 1_555 N
Fe1 Ba2 Fe2 109.1(5) 101_554 . -3_454 N
Fe1 Ba2 Fe2 109.8(5) 101_554 . -3_455 N
Fe1 Ba2 Fe2 178.2(7) 101_554 . 101_454 N
Fe1 Ba2 Fe2 70.68(15) 101_554 . 101_554 N
Fe1 Ba2 O4 144.2(8) 101_554 . -3_565 N
Fe1 Ba2 O4 90.23(29) 101_554 . -4_565 N
Fe1 Ba2 O5 94.53(29) 101_554 . 1_555 N
Fe1 Ba2 O5 145.6(7) 101_554 . 2_555 N
Fe1 Ba2 O8 88.9(5) 101_554 . -3_565 N
Fe1 Ba2 O8 89.2(5) 101_554 . -3_566 N
Fe1 Ba2 O8 142.3(5) 101_554 . 101_454 N
Fe1 Ba2 O8 34.46(30) 101_554 . 101_554 N
Fe1 Ba2 Nd1 53.95(22) 101_554 . 3_555 N
Fe1 Ba2 Ca1 53.95(22) 101_554 . 3_555 N
Fe1 Ba2 Nd2 124.0(7) 101_554 . -103_454 N
Fe1 Ba2 Nd2 125.5(8) 101_554 . -103_455 N
Ba2 Ba2 Ba2 90.250(30) -103_343 . -103_344 N
Ba2 Ba2 Ba2 88.1(10) -103_343 . -103_443 N
Ba2 Ba2 Ba2 178.3(10) -103_343 . -103_444 N
Ba2 Ba2 Ba3 88.6(4) -103_343 . 1_555 N
Ba2 Ba2 Fe2 53.5(5) -103_343 . -3_454 N
Ba2 Ba2 Fe2 126.17(27) -103_343 . -3_455 N
Ba2 Ba2 Fe2 54.36(20) -103_343 . 101_454 N
Ba2 Ba2 Fe2 124.2(8) -103_343 . 101_554 N
Ba2 Ba2 O4 44.1(4) -103_454 . -3_565 N
Ba2 Ba2 O4 88.6(7) -103_454 . -4_565 N
Ba2 Ba2 O5 130.1(4) -103_454 . 1_555 N
Ba2 Ba2 O5 90.161(20) -103_454 . 2_555 N
Ba2 Ba2 O8 44.1(5) -103_454 . -3_565 N
Ba2 Ba2 O8 135.9(5) -103_454 . -3_566 N
Ba2 Ba2 O8 47.1(4) -103_454 . 101_454 N
Ba2 Ba2 O8 135.2(12) -103_454 . 101_554 N
Ba2 Ba2 Nd1 89.58(26) -103_454 . 3_555 N
Ba2 Ba2 Ca1 89.58(26) -103_454 . 3_555 N
Ba2 Ba2 Nd2 0.0 -103_454 . -103_454 N
Ba2 Ba2 Nd2 90.250(30) -103_454 . -103_455 N
Ba2 Ba2 Ba2 178.3(10) -103_344 . -103_443 N
Ba2 Ba2 Ba2 91.4(10) -103_344 . -103_444 N
Ba2 Ba2 Ba3 91.36(35) -103_344 . 1_555 N
Ba2 Ba2 Fe2 125.28(30) -103_344 . -3_454 N
Ba2 Ba2 Fe2 55.0(5) -103_344 . -3_455 N
Ba2 Ba2 Fe2 54.65(19) -103_344 . 101_454 N
Ba2 Ba2 Fe2 126.8(8) -103_344 . 101_554 N
Ba2 Ba2 O4 90.179(21) -103_455 . -3_565 N
Ba2 Ba2 O4 135.86(35) -103_455 . -4_565 N
Ba2 Ba2 O5 90.9(7) -103_455 . 1_555 N
Ba2 Ba2 O5 49.9(4) -103_455 . 2_555 N
Ba2 Ba2 O8 134.3(5) -103_455 . -3_565 N
Ba2 Ba2 O8 45.7(5) -103_455 . -3_566 N
Ba2 Ba2 O8 43.2(4) -103_455 . 101_454 N
Ba2 Ba2 O8 134.5(12) -103_455 . 101_554 N
Ba2 Ba2 Nd1 90.41(25) -103_455 . 3_555 N
Ba2 Ba2 Ca1 90.41(25) -103_455 . 3_555 N
Ba2 Ba2 Nd2 90.250(30) -103_455 . -103_454 N
Ba2 Ba2 Nd2 0.0 -103_455 . -103_455 N
Ba2 Ba2 Ba2 90.250(30) -103_443 . -103_444 N
Ba2 Ba2 Ba3 88.6(4) -103_443 . 1_555 N
Ba2 Ba2 Fe2 53.5(5) -103_443 . -3_454 N
Ba2 Ba2 Fe2 126.17(27) -103_443 . -3_455 N
Ba2 Ba2 Fe2 124.2(8) -103_443 . 101_454 N
Ba2 Ba2 Fe2 54.36(20) -103_443 . 101_554 N
Ba2 Ba2 O4 88.6(7) -103_554 . -3_565 N
Ba2 Ba2 O4 44.1(4) -103_554 . -4_565 N
Ba2 Ba2 O5 90.161(20) -103_554 . 1_555 N
Ba2 Ba2 O5 130.1(4) -103_554 . 2_555 N
Ba2 Ba2 O8 44.1(5) -103_554 . -3_565 N
Ba2 Ba2 O8 135.9(5) -103_554 . -3_566 N
Ba2 Ba2 O8 135.2(12) -103_554 . 101_454 N
Ba2 Ba2 O8 47.1(4) -103_554 . 101_554 N
Ba2 Ba2 Nd1 89.58(26) -103_554 . 3_555 N
Ba2 Ba2 Ca1 89.58(26) -103_554 . 3_555 N
Ba2 Ba2 Nd2 88.1(10) -103_554 . -103_454 N
Ba2 Ba2 Nd2 178.3(10) -103_554 . -103_455 N
Ba2 Ba2 Ba3 91.36(35) -103_444 . 1_555 N
Ba2 Ba2 Fe2 125.28(30) -103_444 . -3_454 N
Ba2 Ba2 Fe2 55.0(5) -103_444 . -3_455 N
Ba2 Ba2 Fe2 126.8(8) -103_444 . 101_454 N
Ba2 Ba2 Fe2 54.65(19) -103_444 . 101_554 N
Ba2 Ba2 O4 135.86(35) -103_555 . -3_565 N
Ba2 Ba2 O4 90.179(21) -103_555 . -4_565 N
Ba2 Ba2 O5 49.9(4) -103_555 . 1_555 N
Ba2 Ba2 O5 90.9(7) -103_555 . 2_555 N
Ba2 Ba2 O8 134.3(5) -103_555 . -3_565 N
Ba2 Ba2 O8 45.7(5) -103_555 . -3_566 N
Ba2 Ba2 O8 134.5(12) -103_555 . 101_454 N
Ba2 Ba2 O8 43.2(4) -103_555 . 101_554 N
Ba2 Ba2 Nd1 90.41(25) -103_555 . 3_555 N
Ba2 Ba2 Ca1 90.41(25) -103_555 . 3_555 N
Ba2 Ba2 Nd2 178.3(10) -103_555 . -103_454 N
Ba2 Ba2 Nd2 91.4(10) -103_555 . -103_455 N
Ba3 Ba2 Fe2 53.8(5) 1_555 . -3_454 N
Ba3 Ba2 Fe2 57.2(4) 1_555 . -3_455 N
Ba3 Ba2 Fe2 55.37(24) 1_555 . 101_454 N
Ba3 Ba2 Fe2 55.37(24) 1_555 . 101_554 N
Ba3 Ba2 O4 44.51(35) 1_555 . -3_565 N
Ba3 Ba2 O4 44.51(35) 1_555 . -4_565 N
Ba3 Ba2 O5 41.5(4) 1_555 . 1_555 N
Ba3 Ba2 O5 41.5(4) 1_555 . 2_555 N
Ba3 Ba2 O8 89.6(6) 1_555 . -3_565 N
Ba3 Ba2 O8 93.6(7) 1_555 . -3_566 N
Ba3 Ba2 O8 91.7(4) 1_555 . 101_454 N
Ba3 Ba2 O8 91.7(4) 1_555 . 101_554 N
Ba3 Ba2 Nd1 177.5(8) 1_555 . 3_555 N
Ba3 Ba2 Ca1 177.5(8) 1_555 . 3_555 N
Ba3 Ba2 Nd2 88.6(4) 1_555 . -103_454 N
Ba3 Ba2 Nd2 91.36(35) 1_555 . -103_455 N
Fe2 Ba2 Fe2 111.0(5) -3_454 . -3_455 N
Fe2 Ba2 Fe2 70.6(4) -3_454 . 101_454 N
Fe2 Ba2 Fe2 70.6(4) -3_454 . 101_554 N
Fe2 Ba2 O4 35.10(27) -3_565 . -3_565 N
Fe2 Ba2 O4 35.10(27) -3_565 . -4_565 N
Fe2 Ba2 O5 86.7(4) -3_565 . 1_555 N
Fe2 Ba2 O5 86.7(4) -3_565 . 2_555 N
Fe2 Ba2 O8 35.7(4) -3_565 . -3_565 N
Fe2 Ba2 O8 147.5(6) -3_565 . -3_566 N
Fe2 Ba2 O8 91.9(6) -3_565 . 101_454 N
Fe2 Ba2 O8 91.9(6) -3_565 . 101_554 N
Fe2 Ba2 Nd1 123.6(6) -3_565 . 3_555 N
Fe2 Ba2 Ca1 123.6(6) -3_565 . 3_555 N
Fe2 Ba2 Nd2 53.5(5) -3_565 . -103_454 N
Fe2 Ba2 Nd2 125.28(30) -3_565 . -103_455 N
Fe2 Ba2 Fe2 71.8(4) -3_455 . 101_454 N
Fe2 Ba2 Fe2 71.8(4) -3_455 . 101_554 N
Fe2 Ba2 O4 91.5(5) -3_566 . -3_565 N
Fe2 Ba2 O4 91.5(5) -3_566 . -4_565 N
Fe2 Ba2 O5 36.30(27) -3_566 . 1_555 N
Fe2 Ba2 O5 36.30(27) -3_566 . 2_555 N
Fe2 Ba2 O8 146.7(6) -3_566 . -3_565 N
Fe2 Ba2 O8 36.5(4) -3_566 . -3_566 N
Fe2 Ba2 O8 90.0(7) -3_566 . 101_454 N
Fe2 Ba2 O8 90.0(7) -3_566 . 101_554 N
Fe2 Ba2 Nd1 125.4(6) -3_566 . 3_555 N
Fe2 Ba2 Ca1 125.4(6) -3_566 . 3_555 N
Fe2 Ba2 Nd2 126.17(27) -3_566 . -103_454 N
Fe2 Ba2 Nd2 55.0(5) -3_566 . -103_455 N
Fe2 Ba2 Fe2 110.7(5) 101_454 . 101_554 N
Fe2 Ba2 O4 35.53(19) 101_454 . -3_565 N
Fe2 Ba2 O4 90.4(5) 101_454 . -4_565 N
Fe2 Ba2 O5 87.2(5) 101_454 . 1_555 N
Fe2 Ba2 O5 36.17(19) 101_454 . 2_555 N
Fe2 Ba2 O8 90.0(5) 101_454 . -3_565 N
Fe2 Ba2 O8 91.8(5) 101_454 . -3_566 N
Fe2 Ba2 O8 36.30(29) 101_454 . 101_454 N
Fe2 Ba2 O8 147.0(6) 101_454 . 101_554 N
Fe2 Ba2 Nd1 124.61(24) 101_454 . 3_555 N
Fe2 Ba2 Ca1 124.61(24) 101_454 . 3_555 N
Fe2 Ba2 Nd2 54.36(20) 101_454 . -103_454 N
Fe2 Ba2 Nd2 54.65(19) 101_454 . -103_455 N
Fe2 Ba2 O4 90.4(5) 101_554 . -3_565 N
Fe2 Ba2 O4 35.53(19) 101_554 . -4_565 N
Fe2 Ba2 O5 36.17(19) 101_554 . 1_555 N
Fe2 Ba2 O5 87.2(5) 101_554 . 2_555 N
Fe2 Ba2 O8 90.0(5) 101_554 . -3_565 N
Fe2 Ba2 O8 91.8(5) 101_554 . -3_566 N
Fe2 Ba2 O8 147.0(6) 101_554 . 101_454 N
Fe2 Ba2 O8 36.30(29) 101_554 . 101_554 N
Fe2 Ba2 Nd1 124.61(24) 101_554 . 3_555 N
Fe2 Ba2 Ca1 124.61(24) 101_554 . 3_555 N
Fe2 Ba2 Nd2 124.2(8) 101_554 . -103_454 N
Fe2 Ba2 Nd2 126.8(8) 101_554 . -103_455 N
O4 Ba2 O4 59.9(4) -3_565 . -4_565 N
O4 Ba2 O5 86.0(5) -3_565 . 1_555 N
O4 Ba2 O5 57.97(29) -3_565 . 2_555 N
O4 Ba2 O8 60.2(5) -3_565 . -3_565 N
O4 Ba2 O8 122.4(6) -3_565 . -3_566 N
O4 Ba2 O8 62.0(4) -3_565 . 101_454 N
O4 Ba2 O8 121.9(7) -3_565 . 101_554 N
O4 Ba2 Nd1 133.7(6) -3_565 . 3_555 N
O4 Ba2 Ca1 133.7(6) -3_565 . 3_555 N
O4 Ba2 Nd2 44.1(4) -3_565 . -103_454 N
O4 Ba2 Nd2 90.179(21) -3_565 . -103_455 N
O4 Ba2 O5 57.97(29) -4_565 . 1_555 N
O4 Ba2 O5 86.0(5) -4_565 . 2_555 N
O4 Ba2 O8 60.2(5) -4_565 . -3_565 N
O4 Ba2 O8 122.4(6) -4_565 . -3_566 N
O4 Ba2 O8 121.9(7) -4_565 . 101_454 N
O4 Ba2 O8 62.0(4) -4_565 . 101_554 N
O4 Ba2 Nd1 133.7(6) -4_565 . 3_555 N
O4 Ba2 Ca1 133.7(6) -4_565 . 3_555 N
O4 Ba2 Nd2 88.6(7) -4_565 . -103_454 N
O4 Ba2 Nd2 135.86(35) -4_565 . -103_455 N
O5 Ba2 O5 54.9(4) 1_555 . 2_555 N
O5 Ba2 O8 118.1(6) 1_555 . -3_565 N
O5 Ba2 O8 64.7(5) 1_555 . -3_566 N
O5 Ba2 O8 118.3(7) 1_555 . 101_454 N
O5 Ba2 O8 63.4(4) 1_555 . 101_554 N
O5 Ba2 Nd1 140.3(6) 1_555 . 3_555 N
O5 Ba2 Ca1 140.3(6) 1_555 . 3_555 N
O5 Ba2 Nd2 130.1(4) 1_555 . -103_454 N
O5 Ba2 Nd2 90.9(7) 1_555 . -103_455 N
O5 Ba2 O8 118.1(6) 2_555 . -3_565 N
O5 Ba2 O8 64.7(5) 2_555 . -3_566 N
O5 Ba2 O8 63.4(4) 2_555 . 101_454 N
O5 Ba2 O8 118.3(7) 2_555 . 101_554 N
O5 Ba2 Nd1 140.3(6) 2_555 . 3_555 N
O5 Ba2 Ca1 140.3(6) 2_555 . 3_555 N
O5 Ba2 Nd2 90.161(20) 2_555 . -103_454 N
O5 Ba2 Nd2 49.9(4) 2_555 . -103_455 N
O8 Ba2 O8 176.8(8) -3_565 . -3_566 N
O8 Ba2 O8 91.1(8) -3_565 . 101_454 N
O8 Ba2 O8 91.1(8) -3_565 . 101_554 N
O8 Ba2 Nd1 87.9(5) -3_565 . 3_555 N
O8 Ba2 Ca1 87.9(5) -3_565 . 3_555 N
O8 Ba2 Nd2 44.1(5) -3_565 . -103_454 N
O8 Ba2 Nd2 134.3(5) -3_565 . -103_455 N
O8 Ba2 O8 88.8(7) -3_566 . 101_454 N
O8 Ba2 O8 88.8(7) -3_566 . 101_554 N
O8 Ba2 Nd1 88.9(5) -3_566 . 3_555 N
O8 Ba2 Ca1 88.9(5) -3_566 . 3_555 N
O8 Ba2 Nd2 135.9(5) -3_566 . -103_454 N
O8 Ba2 Nd2 45.7(5) -3_566 . -103_455 N
O8 Ba2 O8 176.0(10) 101_454 . 101_554 N
O8 Ba2 Nd1 88.4(4) 101_454 . 3_555 N
O8 Ba2 Ca1 88.4(4) 101_454 . 3_555 N
O8 Ba2 Nd2 47.1(4) 101_454 . -103_454 N
O8 Ba2 Nd2 43.2(4) 101_454 . -103_455 N
O8 Ba2 Nd1 88.4(4) 101_554 . 3_555 N
O8 Ba2 Ca1 88.4(4) 101_554 . 3_555 N
O8 Ba2 Nd2 135.2(12) 101_554 . -103_454 N
O8 Ba2 Nd2 134.5(12) 101_554 . -103_455 N
Nd1 Ba2 Ca1 0.0 3_555 . 3_555 N
Nd1 Ba2 Nd2 89.58(26) 3_555 . -103_454 N
Nd1 Ba2 Nd2 90.41(25) 3_555 . -103_455 N
Ca1 Ba2 Nd2 89.58(26) 3_555 . -103_454 N
Ca1 Ba2 Nd2 90.41(25) 3_555 . -103_455 N
Nd2 Ba2 Nd2 90.250(30) -103_454 . -103_455 N
Ba2 Ba3 Ba3 178.1(5) 1_555 . 3_565 N
Ba2 Ba3 Ba3 91.34(35) 1_555 . -103_343 N
Ba2 Ba3 Ba3 88.6(4) 1_555 . -103_344 N
Ba2 Ba3 Ba3 91.34(35) 1_555 . -103_443 N
Ba2 Ba3 Ba3 88.6(4) 1_555 . -103_444 N
Ba2 Ba3 Fe2 60.4(5) 1_555 . -3_454 N
Ba2 Ba3 Fe2 58.1(5) 1_555 . -3_455 N
Ba2 Ba3 Fe2 59.13(22) 1_555 . 101_454 N
Ba2 Ba3 Fe2 59.13(22) 1_555 . 101_554 N
Ba2 Ba3 Fe3 128.6(7) 1_555 . -1_566 N
Ba2 Ba3 Fe3 128.6(7) 1_555 . -2_566 N
Ba2 Ba3 Fe3 130.87(25) 1_555 . 101_454 N
Ba2 Ba3 Fe3 130.87(25) 1_555 . 102_554 N
Ba2 Ba3 O4 50.7(4) 1_555 . -3_565 N
Ba2 Ba3 O4 50.7(4) 1_555 . -4_565 N
Ba2 Ba3 O5 56.4(5) 1_555 . 1_555 N
Ba2 Ba3 O5 56.4(5) 1_555 . 2_555 N
Ba2 Ba3 O6 139.8(5) 1_555 . -1_565 N
Ba2 Ba3 O6 139.8(5) 1_555 . -2_565 N
Ba2 Ba3 O7 151.5(9) 1_555 . 101_454 N
Ba2 Ba3 O7 151.5(9) 1_555 . 102_554 N
Ba2 Ba3 O9 103.1(8) 1_555 . -3_565 N
Ba2 Ba3 O9 99.6(4) 1_555 . 101_454 N
Ba2 Ba3 O9 99.6(4) 1_555 . 101_554 N
Ba3 Ba3 Ba3 90.0 3_565 . -103_343 N
Ba3 Ba3 Ba3 90.0 3_565 . -103_344 N
Ba3 Ba3 Ba3 90.0 3_565 . -103_443 N
Ba3 Ba3 Ba3 90.0 3_565 . -103_444 N
Ba3 Ba3 Fe2 121.57(28) 3_565 . -3_454 N
Ba3 Ba3 Fe2 119.93(30) 3_565 . -3_455 N
Ba3 Ba3 Fe2 120.84(22) 3_565 . 101_454 N
Ba3 Ba3 Fe2 120.84(22) 3_565 . 101_554 N
Ba3 Ba3 Fe3 49.50(31) 3_565 . -1_566 N
Ba3 Ba3 Fe3 49.50(31) 3_565 . -2_566 N
Ba3 Ba3 Fe3 48.75(22) 3_565 . 101_454 N
Ba3 Ba3 Fe3 48.75(22) 3_565 . 102_554 N
Ba3 Ba3 O4 130.64(34) 3_565 . -3_565 N
Ba3 Ba3 O4 130.64(34) 3_565 . -4_565 N
Ba3 Ba3 O5 122.1(5) 3_565 . 1_555 N
Ba3 Ba3 O5 122.1(5) 3_565 . 2_555 N
Ba3 Ba3 O6 41.54(28) 3_565 . -1_565 N
Ba3 Ba3 O6 41.54(28) 3_565 . -2_565 N
Ba3 Ba3 O7 27.1(8) 3_565 . 101_454 N
Ba3 Ba3 O7 27.1(8) 3_565 . 102_554 N
Ba3 Ba3 O9 78.9(5) 3_565 . -3_565 N
Ba3 Ba3 O9 80.6(4) 3_565 . 101_454 N
Ba3 Ba3 O9 80.6(4) 3_565 . 101_554 N
Ba3 Ba3 Ba3 90.18(5) -103_343 . -103_344 N
Ba3 Ba3 Ba3 93.2(9) -103_343 . -103_443 N
Ba3 Ba3 Ba3 176.7(8) -103_343 . -103_444 N
Ba3 Ba3 Fe2 54.2(4) -103_343 . -3_454 N
Ba3 Ba3 Fe2 126.56(28) -103_343 . -3_455 N
Ba3 Ba3 Fe2 52.54(18) -103_343 . 101_454 N
Ba3 Ba3 Fe2 129.7(7) -103_343 . 101_554 N
Ba3 Ba3 Fe3 116.03(28) -103_454 . -1_566 N
Ba3 Ba3 Fe3 126.57(31) -103_454 . -2_566 N
Ba3 Ba3 Fe3 63.79(23) -103_454 . 101_454 N
Ba3 Ba3 Fe3 129.2(5) -103_454 . 102_554 N
Ba3 Ba3 O4 40.64(34) -103_454 . -3_565 N
Ba3 Ba3 O4 92.4(7) -103_454 . -4_565 N
Ba3 Ba3 O5 147.7(4) -103_454 . 1_555 N
Ba3 Ba3 O5 90.15(4) -103_454 . 2_555 N
Ba3 Ba3 O6 48.46(28) -103_454 . -1_565 N
Ba3 Ba3 O6 92.1(6) -103_454 . -2_565 N
Ba3 Ba3 O7 88.7(12) -103_454 . 101_454 N
Ba3 Ba3 O7 117.1(8) -103_454 . 102_554 N
Ba3 Ba3 O9 47.6(5) -103_454 . -3_565 N
Ba3 Ba3 O9 38.5(4) -103_454 . 101_454 N
Ba3 Ba3 O9 130.0(9) -103_454 . 101_554 N
Ba3 Ba3 Ba3 176.7(8) -103_344 . -103_443 N
Ba3 Ba3 Ba3 86.5(8) -103_344 . -103_444 N
Ba3 Ba3 Fe2 128.36(25) -103_344 . -3_454 N
Ba3 Ba3 Fe2 50.9(4) -103_344 . -3_455 N
Ba3 Ba3 Fe2 52.83(20) -103_344 . 101_454 N
Ba3 Ba3 Fe2 124.9(7) -103_344 . 101_554 N
Ba3 Ba3 Fe3 51.5(4) -103_455 . -1_566 N
Ba3 Ba3 Fe3 61.7(5) -103_455 . -2_566 N
Ba3 Ba3 Fe3 52.62(25) -103_455 . 101_454 N
Ba3 Ba3 Fe3 113.9(6) -103_455 . 102_554 N
Ba3 Ba3 O4 90.13(4) -103_455 . -3_565 N
Ba3 Ba3 O4 139.3(4) -103_455 . -4_565 N
Ba3 Ba3 O5 87.0(7) -103_455 . 1_555 N
Ba3 Ba3 O5 32.1(5) -103_455 . 2_555 N
Ba3 Ba3 O6 90.117(33) -103_455 . -1_565 N
Ba3 Ba3 O6 131.46(32) -103_455 . -2_565 N
Ba3 Ba3 O7 62.9(8) -103_455 . 101_454 N
Ba3 Ba3 O7 89.8(13) -103_455 . 102_554 N
Ba3 Ba3 O9 135.6(4) -103_455 . -3_565 N
Ba3 Ba3 O9 53.3(4) -103_455 . 101_454 N
Ba3 Ba3 O9 138.3(9) -103_455 . 101_554 N
Ba3 Ba3 Ba3 90.18(5) -103_443 . -103_444 N
Ba3 Ba3 Fe2 54.2(4) -103_443 . -3_454 N
Ba3 Ba3 Fe2 126.56(28) -103_443 . -3_455 N
Ba3 Ba3 Fe2 129.7(7) -103_443 . 101_454 N
Ba3 Ba3 Fe2 52.54(18) -103_443 . 101_554 N
Ba3 Ba3 Fe3 126.57(31) -103_554 . -1_566 N
Ba3 Ba3 Fe3 116.03(28) -103_554 . -2_566 N
Ba3 Ba3 Fe3 129.2(5) -103_554 . 101_454 N
Ba3 Ba3 Fe3 63.79(23) -103_554 . 102_554 N
Ba3 Ba3 O4 92.4(7) -103_554 . -3_565 N
Ba3 Ba3 O4 40.64(34) -103_554 . -4_565 N
Ba3 Ba3 O5 90.15(4) -103_554 . 1_555 N
Ba3 Ba3 O5 147.7(4) -103_554 . 2_555 N
Ba3 Ba3 O6 92.1(6) -103_554 . -1_565 N
Ba3 Ba3 O6 48.46(28) -103_554 . -2_565 N
Ba3 Ba3 O7 117.1(8) -103_554 . 101_454 N
Ba3 Ba3 O7 88.7(12) -103_554 . 102_554 N
Ba3 Ba3 O9 47.6(5) -103_554 . -3_565 N
Ba3 Ba3 O9 130.0(9) -103_554 . 101_454 N
Ba3 Ba3 O9 38.5(4) -103_554 . 101_554 N
Ba3 Ba3 Fe2 128.36(25) -103_444 . -3_454 N
Ba3 Ba3 Fe2 50.9(4) -103_444 . -3_455 N
Ba3 Ba3 Fe2 124.9(7) -103_444 . 101_454 N
Ba3 Ba3 Fe2 52.83(20) -103_444 . 101_554 N
Ba3 Ba3 Fe3 61.7(5) -103_555 . -1_566 N
Ba3 Ba3 Fe3 51.5(4) -103_555 . -2_566 N
Ba3 Ba3 Fe3 113.9(6) -103_555 . 101_454 N
Ba3 Ba3 Fe3 52.62(25) -103_555 . 102_554 N
Ba3 Ba3 O4 139.3(4) -103_555 . -3_565 N
Ba3 Ba3 O4 90.13(4) -103_555 . -4_565 N
Ba3 Ba3 O5 32.1(5) -103_555 . 1_555 N
Ba3 Ba3 O5 87.0(7) -103_555 . 2_555 N
Ba3 Ba3 O6 131.46(32) -103_555 . -1_565 N
Ba3 Ba3 O6 90.117(33) -103_555 . -2_565 N
Ba3 Ba3 O7 89.8(13) -103_555 . 101_454 N
Ba3 Ba3 O7 62.9(8) -103_555 . 102_554 N
Ba3 Ba3 O9 135.6(4) -103_555 . -3_565 N
Ba3 Ba3 O9 138.3(9) -103_555 . 101_454 N
Ba3 Ba3 O9 53.3(4) -103_555 . 101_554 N
Fe2 Ba3 Fe2 118.5(4) -3_454 . -3_455 N
Fe2 Ba3 Fe2 75.5(4) -3_454 . 101_454 N
Fe2 Ba3 Fe2 75.5(4) -3_454 . 101_554 N
Fe2 Ba3 Fe3 168.9(5) -3_565 . -1_566 N
Fe2 Ba3 Fe3 168.9(5) -3_565 . -2_566 N
Fe2 Ba3 Fe3 117.6(5) -3_565 . 101_454 N
Fe2 Ba3 Fe3 117.6(5) -3_565 . 102_554 N
Fe2 Ba3 O4 38.25(29) -3_565 . -3_565 N
Fe2 Ba3 O4 38.25(29) -3_565 . -4_565 N
Fe2 Ba3 O5 104.3(5) -3_565 . 1_555 N
Fe2 Ba3 O5 104.3(5) -3_565 . 2_555 N
Fe2 Ba3 O6 90.2(5) -3_565 . -1_565 N
Fe2 Ba3 O6 90.2(5) -3_565 . -2_565 N
Fe2 Ba3 O7 137.2(13) -3_565 . 101_454 N
Fe2 Ba3 O7 137.2(13) -3_565 . 102_554 N
Fe2 Ba3 O9 42.7(5) -3_565 . -3_565 N
Fe2 Ba3 O9 89.9(6) -3_565 . 101_454 N
Fe2 Ba3 O9 89.9(6) -3_565 . 101_554 N
Fe2 Ba3 Fe2 74.0(4) -3_455 . 101_454 N
Fe2 Ba3 Fe2 74.0(4) -3_455 . 101_554 N
Fe2 Ba3 Fe3 70.8(5) -3_566 . -1_566 N
Fe2 Ba3 Fe3 70.8(5) -3_566 . -2_566 N
Fe2 Ba3 Fe3 102.1(5) -3_566 . 101_454 N
Fe2 Ba3 Fe3 102.1(5) -3_566 . 102_554 N
Fe2 Ba3 O4 97.3(4) -3_566 . -3_565 N
Fe2 Ba3 O4 97.3(4) -3_566 . -4_565 N
Fe2 Ba3 O5 36.87(26) -3_566 . 1_555 N
Fe2 Ba3 O5 36.87(26) -3_566 . 2_555 N
Fe2 Ba3 O6 140.2(5) -3_566 . -1_565 N
Fe2 Ba3 O6 140.2(5) -3_566 . -2_565 N
Fe2 Ba3 O7 99.9(11) -3_566 . 101_454 N
Fe2 Ba3 O7 99.9(11) -3_566 . 102_554 N
Fe2 Ba3 O9 161.2(7) -3_566 . -3_565 N
Fe2 Ba3 O9 99.8(5) -3_566 . 101_454 N
Fe2 Ba3 O9 99.8(5) -3_566 . 101_554 N
Fe2 Ba3 Fe2 118.2(4) 101_454 . 101_554 N
Fe2 Ba3 Fe3 102.9(5) 101_454 . -1_566 N
Fe2 Ba3 Fe3 114.1(5) 101_454 . -2_566 N
Fe2 Ba3 Fe3 72.59(22) 101_454 . 101_454 N
Fe2 Ba3 Fe3 165.8(6) 101_454 . 102_554 N
Fe2 Ba3 O4 37.30(19) 101_454 . -3_565 N
Fe2 Ba3 O4 98.7(5) 101_454 . -4_565 N
Fe2 Ba3 O5 102.2(5) 101_454 . 1_555 N
Fe2 Ba3 O5 38.34(19) 101_454 . 2_555 N
Fe2 Ba3 O6 88.88(21) 101_454 . -1_565 N
Fe2 Ba3 O6 143.8(5) 101_454 . -2_565 N
Fe2 Ba3 O7 99.6(9) 101_454 . 101_454 N
Fe2 Ba3 O7 137.1(13) 101_454 . 102_554 N
Fe2 Ba3 O9 96.9(5) 101_454 . -3_565 N
Fe2 Ba3 O9 40.82(34) 101_454 . 101_454 N
Fe2 Ba3 O9 158.1(6) 101_454 . 101_554 N
Fe2 Ba3 Fe3 114.1(5) 101_554 . -1_566 N
Fe2 Ba3 Fe3 102.9(5) 101_554 . -2_566 N
Fe2 Ba3 Fe3 165.8(6) 101_554 . 101_454 N
Fe2 Ba3 Fe3 72.59(22) 101_554 . 102_554 N
Fe2 Ba3 O4 98.7(5) 101_554 . -3_565 N
Fe2 Ba3 O4 37.30(19) 101_554 . -4_565 N
Fe2 Ba3 O5 38.34(19) 101_554 . 1_555 N
Fe2 Ba3 O5 102.2(5) 101_554 . 2_555 N
Fe2 Ba3 O6 143.8(5) 101_554 . -1_565 N
Fe2 Ba3 O6 88.88(21) 101_554 . -2_565 N
Fe2 Ba3 O7 137.1(13) 101_554 . 101_454 N
Fe2 Ba3 O7 99.6(9) 101_554 . 102_554 N
Fe2 Ba3 O9 96.9(5) 101_554 . -3_565 N
Fe2 Ba3 O9 158.1(6) 101_554 . 101_454 N
Fe2 Ba3 O9 40.82(34) 101_554 . 101_554 N
Fe3 Ba3 Fe3 12.4(5) -1_566 . -2_566 N
Fe3 Ba3 Fe3 52.2(4) -1_566 . 101_454 N
Fe3 Ba3 Fe3 63.1(4) -1_566 . 102_554 N
Fe3 Ba3 O4 139.1(4) -1_566 . -3_565 N
Fe3 Ba3 O4 151.1(4) -1_566 . -4_565 N
Fe3 Ba3 O5 86.8(7) -1_566 . 1_555 N
Fe3 Ba3 O5 79.6(6) -1_566 . 2_555 N
Fe3 Ba3 O6 78.75(34) -1_566 . -1_565 N
Fe3 Ba3 O6 84.8(4) -1_566 . -2_565 N
Fe3 Ba3 O7 31.7(11) -1_566 . 101_454 N
Fe3 Ba3 O7 38.8(12) -1_566 . 102_554 N
Fe3 Ba3 O9 127.8(6) -1_566 . -3_565 N
Fe3 Ba3 O9 82.3(5) -1_566 . 101_454 N
Fe3 Ba3 O9 94.4(6) -1_566 . 101_554 N
Fe3 Ba3 Fe3 63.1(4) -2_566 . 101_454 N
Fe3 Ba3 Fe3 52.2(4) -2_566 . 102_554 N
Fe3 Ba3 O4 151.1(4) -2_566 . -3_565 N
Fe3 Ba3 O4 139.1(4) -2_566 . -4_565 N
Fe3 Ba3 O5 79.6(6) -2_566 . 1_555 N
Fe3 Ba3 O5 86.8(7) -2_566 . 2_555 N
Fe3 Ba3 O6 84.8(4) -2_566 . -1_565 N
Fe3 Ba3 O6 78.75(34) -2_566 . -2_565 N
Fe3 Ba3 O7 38.8(12) -2_566 . 101_454 N
Fe3 Ba3 O7 31.7(11) -2_566 . 102_554 N
Fe3 Ba3 O9 127.8(6) -2_566 . -3_565 N
Fe3 Ba3 O9 94.4(6) -2_566 . 101_454 N
Fe3 Ba3 O9 82.3(5) -2_566 . 101_554 N
Fe3 Ba3 Fe3 95.3(5) 101_454 . 102_554 N
Fe3 Ba3 O4 95.41(29) 101_454 . -3_565 N
Fe3 Ba3 O4 155.4(7) 101_454 . -4_565 N
Fe3 Ba3 O5 134.0(8) 101_454 . 1_555 N
Fe3 Ba3 O5 80.6(4) 101_454 . 2_555 N
Fe3 Ba3 O6 38.15(26) 101_454 . -1_565 N
Fe3 Ba3 O6 85.73(35) 101_454 . -2_565 N
Fe3 Ba3 O7 29.1(11) 101_454 . 101_454 N
Fe3 Ba3 O7 67.2(10) 101_454 . 102_554 N
Fe3 Ba3 O9 90.5(5) 101_454 . -3_565 N
Fe3 Ba3 O9 35.1(4) 101_454 . 101_454 N
Fe3 Ba3 O9 129.2(5) 101_454 . 101_554 N
Fe3 Ba3 O4 155.4(7) 102_554 . -3_565 N
Fe3 Ba3 O4 95.41(29) 102_554 . -4_565 N
Fe3 Ba3 O5 80.6(4) 102_554 . 1_555 N
Fe3 Ba3 O5 134.0(8) 102_554 . 2_555 N
Fe3 Ba3 O6 85.73(35) 102_554 . -1_565 N
Fe3 Ba3 O6 38.15(26) 102_554 . -2_565 N
Fe3 Ba3 O7 67.2(10) 102_554 . 101_454 N
Fe3 Ba3 O7 29.1(11) 102_554 . 102_554 N
Fe3 Ba3 O9 90.5(5) 102_554 . -3_565 N
Fe3 Ba3 O9 129.2(5) 102_554 . 101_454 N
Fe3 Ba3 O9 35.1(4) 102_554 . 101_554 N
O4 Ba3 O4 66.9(4) -3_565 . -4_565 N
O4 Ba3 O5 107.1(6) -3_565 . 1_555 N
O4 Ba3 O5 69.84(31) -3_565 . 2_555 N
O4 Ba3 O6 89.1(5) -3_565 . -1_565 N
O4 Ba3 O6 121.0(8) -3_565 . -2_565 N
O4 Ba3 O7 124.2(12) -3_565 . 101_454 N
O4 Ba3 O7 157.7(9) -3_565 . 102_554 N
O4 Ba3 O9 67.3(6) -3_565 . -3_565 N
O4 Ba3 O9 60.8(4) -3_565 . 101_454 N
O4 Ba3 O9 126.4(7) -3_565 . 101_554 N
O4 Ba3 O5 69.84(31) -4_565 . 1_555 N
O4 Ba3 O5 107.1(6) -4_565 . 2_555 N
O4 Ba3 O6 121.0(8) -4_565 . -1_565 N
O4 Ba3 O6 89.1(5) -4_565 . -2_565 N
O4 Ba3 O7 157.7(9) -4_565 . 101_454 N
O4 Ba3 O7 124.2(12) -4_565 . 102_554 N
O4 Ba3 O9 67.3(6) -4_565 . -3_565 N
O4 Ba3 O9 126.4(7) -4_565 . 101_454 N
O4 Ba3 O9 60.8(4) -4_565 . 101_554 N
O5 Ba3 O5 70.9(5) 1_555 . 2_555 N
O5 Ba3 O6 163.5(7) 1_555 . -1_565 N
O5 Ba3 O6 113.58(26) 1_555 . -2_565 N
O5 Ba3 O7 118.1(14) 1_555 . 101_454 N
O5 Ba3 O7 95.1(9) 1_555 . 102_554 N
O5 Ba3 O9 135.1(6) 1_555 . -3_565 N
O5 Ba3 O9 135.9(7) 1_555 . 101_454 N
O5 Ba3 O9 65.2(4) 1_555 . 101_554 N
O5 Ba3 O6 113.58(26) 2_555 . -1_565 N
O5 Ba3 O6 163.5(7) 2_555 . -2_565 N
O5 Ba3 O7 95.1(9) 2_555 . 101_454 N
O5 Ba3 O7 118.1(14) 2_555 . 102_554 N
O5 Ba3 O9 135.1(6) 2_555 . -3_565 N
O5 Ba3 O9 65.2(4) 2_555 . 101_454 N
O5 Ba3 O9 135.9(7) 2_555 . 101_554 N
O6 Ba3 O6 57.59(26) -1_565 . -2_565 N
O6 Ba3 O7 47.0(11) -1_565 . 101_454 N
O6 Ba3 O7 68.7(8) -1_565 . 102_554 N
O6 Ba3 O9 53.7(4) -1_565 . -3_565 N
O6 Ba3 O9 50.14(33) -1_565 . 101_454 N
O6 Ba3 O9 107.7(5) -1_565 . 101_554 N
O6 Ba3 O7 68.7(8) -2_565 . 101_454 N
O6 Ba3 O7 47.0(11) -2_565 . 102_554 N
O6 Ba3 O9 53.7(4) -2_565 . -3_565 N
O6 Ba3 O9 107.7(5) -2_565 . 101_454 N
O6 Ba3 O9 50.14(33) -2_565 . 101_554 N
O7 Ba3 O7 38.5(20) 101_454 . 102_554 N
O7 Ba3 O9 97.9(12) 101_454 . -3_565 N
O7 Ba3 O9 64.1(11) 101_454 . 101_454 N
O7 Ba3 O9 102.2(11) 101_454 . 101_554 N
O7 Ba3 O9 97.9(12) 102_554 . -3_565 N
O7 Ba3 O9 102.2(11) 102_554 . 101_454 N
O7 Ba3 O9 64.1(11) 102_554 . 101_554 N
O9 Ba3 O9 82.4(5) -3_565 . 101_454 N
O9 Ba3 O9 82.4(5) -3_565 . 101_554 N
O9 Ba3 O9 157.9(8) 101_454 . 101_554 N
Ba2 Fe2 Ba2 111.0(5) -3_444 . -3_445 N
Ba2 Fe2 Ba2 72.1(6) -3_444 . 101_445 N
Ba2 Fe2 Ba2 72.1(6) -3_444 . 101_545 N
Ba2 Fe2 Ba3 65.8(4) -3_444 . -3_444 N
Ba2 Fe2 Ba3 175.7(5) -3_444 . -3_445 N
Ba2 Fe2 Ba3 105.7(4) -3_444 . 101_445 N
Ba2 Fe2 Ba3 105.7(4) -3_444 . 101_545 N
Ba2 Fe2 O4 54.6(4) -3_555 . 1_555 N
Ba2 Fe2 O4 54.6(4) -3_555 . 2_555 N
Ba2 Fe2 O5 133.23(34) -3_555 . -3_556 N
Ba2 Fe2 O5 133.23(34) -3_555 . -4_556 N
Ba2 Fe2 O8 58.8(5) -3_555 . 1_555 N
Ba2 Fe2 Ca3 65.8(4) -3_555 . -3_555 N
Ba2 Fe2 Ba2 70.3(5) -3_445 . 101_445 N
Ba2 Fe2 Ba2 70.3(5) -3_445 . 101_545 N
Ba2 Fe2 Ba3 176.8(5) -3_445 . -3_444 N
Ba2 Fe2 Ba3 64.7(4) -3_445 . -3_445 N
Ba2 Fe2 Ba3 108.1(4) -3_445 . 101_445 N
Ba2 Fe2 Ba3 108.1(4) -3_445 . 101_545 N
Ba2 Fe2 O4 125.8(4) -3_556 . 1_555 N
Ba2 Fe2 O4 125.8(4) -3_556 . 2_555 N
Ba2 Fe2 O5 62.4(5) -3_556 . -3_556 N
Ba2 Fe2 O5 62.4(5) -3_556 . -4_556 N
Ba2 Fe2 O8 52.2(5) -3_556 . 1_555 N
Ba2 Fe2 Ca3 176.8(5) -3_556 . -3_555 N
Ba2 Fe2 Ba2 110.7(5) 101_445 . 101_545 N
Ba2 Fe2 Ba3 108.1(5) 101_445 . -3_444 N
Ba2 Fe2 Ba3 105.7(5) 101_445 . -3_445 N
Ba2 Fe2 Ba3 65.51(22) 101_445 . 101_445 N
Ba2 Fe2 Ba3 176.2(4) 101_445 . 101_545 N
Ba2 Fe2 O4 126.7(6) 101_445 . 1_555 N
Ba2 Fe2 O4 55.5(5) 101_445 . 2_555 N
Ba2 Fe2 O5 62.0(5) 101_445 . -3_556 N
Ba2 Fe2 O5 131.8(7) 101_445 . -4_556 N
Ba2 Fe2 O8 55.38(24) 101_445 . 1_555 N
Ba2 Fe2 Ca3 108.1(5) 101_445 . -3_555 N
Ba2 Fe2 Ba3 108.1(5) 101_545 . -3_444 N
Ba2 Fe2 Ba3 105.7(5) 101_545 . -3_445 N
Ba2 Fe2 Ba3 176.2(4) 101_545 . 101_445 N
Ba2 Fe2 Ba3 65.51(22) 101_545 . 101_545 N
Ba2 Fe2 O4 55.5(5) 101_545 . 1_555 N
Ba2 Fe2 O4 126.7(6) 101_545 . 2_555 N
Ba2 Fe2 O5 131.8(7) 101_545 . -3_556 N
Ba2 Fe2 O5 62.0(5) 101_545 . -4_556 N
Ba2 Fe2 O8 55.38(24) 101_545 . 1_555 N
Ba2 Fe2 Ca3 108.1(5) 101_545 . -3_555 N
Ba3 Fe2 Ba3 118.5(4) -3_444 . -3_445 N
Ba3 Fe2 Ba3 73.3(4) -3_444 . 101_445 N
Ba3 Fe2 Ba3 73.3(4) -3_444 . 101_545 N
Ba3 Fe2 O4 52.65(32) -3_555 . 1_555 N
Ba3 Fe2 O4 52.65(32) -3_555 . 2_555 N
Ba3 Fe2 O5 119.6(5) -3_555 . -3_556 N
Ba3 Fe2 O5 119.6(5) -3_555 . -4_556 N
Ba3 Fe2 O8 124.6(6) -3_555 . 1_555 N
Ba3 Fe2 Ca3 0.0 -3_555 . -3_555 N
Ba3 Fe2 Ba3 76.3(5) -3_445 . 101_445 N
Ba3 Fe2 Ba3 76.3(5) -3_445 . 101_545 N
Ba3 Fe2 O4 127.4(4) -3_556 . 1_555 N
Ba3 Fe2 O4 127.4(4) -3_556 . 2_555 N
Ba3 Fe2 O5 45.54(29) -3_556 . -3_556 N
Ba3 Fe2 O5 45.54(29) -3_556 . -4_556 N
Ba3 Fe2 O8 116.9(6) -3_556 . 1_555 N
Ba3 Fe2 Ca3 118.5(4) -3_556 . -3_555 N
Ba3 Fe2 Ba3 118.2(4) 101_445 . 101_545 N
Ba3 Fe2 O4 125.9(5) 101_445 . 1_555 N
Ba3 Fe2 O4 51.1(4) 101_445 . 2_555 N
Ba3 Fe2 O5 47.6(4) 101_445 . -3_556 N
Ba3 Fe2 O5 120.6(6) 101_445 . -4_556 N
Ba3 Fe2 O8 120.87(22) 101_445 . 1_555 N
Ba3 Fe2 Ca3 73.3(4) 101_445 . -3_555 N
Ba3 Fe2 O4 51.1(4) 101_545 . 1_555 N
Ba3 Fe2 O4 125.9(5) 101_545 . 2_555 N
Ba3 Fe2 O5 120.6(6) 101_545 . -3_556 N
Ba3 Fe2 O5 47.6(4) 101_545 . -4_556 N
Ba3 Fe2 O8 120.87(22) 101_545 . 1_555 N
Ba3 Fe2 Ca3 73.3(4) 101_545 . -3_555 N
O4 Fe2 O4 90.1(4) 1_555 . 2_555 N
O4 Fe2 O5 168.4(7) 1_555 . -3_556 N
O4 Fe2 O5 90.16(8) 1_555 . -4_556 N
O4 Fe2 O8 92.7(6) 1_555 . 1_555 N
O4 Fe2 Ca3 52.65(32) 1_555 . -3_555 N
O4 Fe2 O5 90.16(8) 2_555 . -3_556 N
O4 Fe2 O5 168.4(7) 2_555 . -4_556 N
O4 Fe2 O8 92.7(6) 2_555 . 1_555 N
O4 Fe2 Ca3 52.65(32) 2_555 . -3_555 N
O5 Fe2 O5 87.3(4) -3_556 . -4_556 N
O5 Fe2 O8 98.9(6) -3_556 . 1_555 N
O5 Fe2 Ca3 119.6(5) -3_556 . -3_555 N
O5 Fe2 O8 98.9(6) -4_556 . 1_555 N
O5 Fe2 Ca3 119.6(5) -4_556 . -3_555 N
O8 Fe2 Ca3 124.6(6) 1_555 . -3_555 N
Ba3 Fe3 Ba3 81.0(6) -1_566 . -3_445 N
Ba3 Fe3 Ba3 127.8(4) -1_566 . 101_545 N
Ba3 Fe3 Ba3 75.9(5) -1_566 . 103_444 N
Ba3 Fe3 Fe3 83.80(25) -1_566 . 2_555 N
Ba3 Fe3 O6 134.8(4) -1_566 . 1_555 N
Ba3 Fe3 O7 88.0(11) -1_566 . 1_555 N
Ba3 Fe3 O7 45.3(6) -1_566 . -101_556 N
Ba3 Fe3 O7 46.7(5) -1_566 . -102_456 N
Ba3 Fe3 O9 149.3(8) -1_566 . 1_555 N
Ba3 Fe3 O9 72.0(7) -1_566 . 3_555 N
Ba3 Fe3 Ba3 75.9(5) -3_445 . 101_545 N
Ba3 Fe3 Ba3 127.8(4) -3_445 . 103_444 N
Ba3 Fe3 Fe3 83.80(25) -3_556 . 2_555 N
Ba3 Fe3 O6 134.8(4) -3_556 . 1_555 N
Ba3 Fe3 O7 88.0(11) -3_556 . 1_555 N
Ba3 Fe3 O7 45.3(6) -3_556 . -101_556 N
Ba3 Fe3 O7 46.7(5) -3_556 . -102_456 N
Ba3 Fe3 O9 72.0(7) -3_556 . 1_555 N
Ba3 Fe3 O9 149.3(8) -3_556 . 3_555 N
Ba3 Fe3 Ba3 82.5(5) 101_545 . 103_444 N
Ba3 Fe3 Fe3 137.64(23) 101_545 . 2_555 N
Ba3 Fe3 O6 60.6(4) 101_545 . 1_555 N
Ba3 Fe3 O7 45.6(6) 101_545 . 1_555 N
Ba3 Fe3 O7 87.3(11) 101_545 . -101_556 N
Ba3 Fe3 O7 121.7(7) 101_545 . -102_456 N
Ba3 Fe3 O9 59.5(4) 101_545 . 1_555 N
Ba3 Fe3 O9 132.8(8) 101_545 . 3_555 N
Ba3 Fe3 Fe3 137.64(23) 103_555 . 2_555 N
Ba3 Fe3 O6 60.6(4) 103_555 . 1_555 N
Ba3 Fe3 O7 45.6(6) 103_555 . 1_555 N
Ba3 Fe3 O7 87.3(11) 103_555 . -101_556 N
Ba3 Fe3 O7 121.7(7) 103_555 . -102_456 N
Ba3 Fe3 O9 132.8(8) 103_555 . 1_555 N
Ba3 Fe3 O9 59.5(4) 103_555 . 3_555 N
Fe3 Fe3 O6 120.2(4) 2_555 . 1_555 N
Fe3 Fe3 O7 169.2(15) 2_555 . 1_555 N
Fe3 Fe3 O7 104.2(13) 2_555 . -101_556 N
Fe3 Fe3 O7 56.3(10) 2_555 . -102_456 N
Fe3 Fe3 O9 79.0(4) 2_555 . 1_555 N
Fe3 Fe3 O9 79.0(4) 2_555 . 3_555 N
O6 Fe3 O7 70.6(15) 1_555 . 1_555 N
O6 Fe3 O7 135.6(14) 1_555 . -101_556 N
O6 Fe3 O7 176.5(12) 1_555 . -102_456 N
O6 Fe3 O9 75.9(6) 1_555 . 1_555 N
O6 Fe3 O9 75.9(6) 1_555 . 3_555 N
O7 Fe3 O7 64.9(20) 1_555 . -101_556 N
O7 Fe3 O7 112.8(15) 1_555 . -102_456 N
O7 Fe3 O9 105.1(7) 1_555 . 1_555 N
O7 Fe3 O9 105.1(7) 1_555 . 3_555 N
O7 Fe3 O7 47.9(22) -101_556 . -102_456 N
O7 Fe3 O9 115.3(7) -101_556 . 1_555 N
O7 Fe3 O9 115.3(7) -101_556 . 3_555 N
O7 Fe3 O9 102.8(8) -102_456 . 1_555 N
O7 Fe3 O9 102.8(8) -102_456 . 3_555 N
O9 Fe3 O9 128.2(13) 1_555 . 3_555 N
Ba2 O4 Ba2 91.8(7) -3_444 . 101_545 N
Ba2 O4 Ba3 84.8(4) -3_444 . -3_444 N
Ba2 O4 Ba3 176.1(4) -3_444 . 101_545 N
Ba2 O4 Fe2 90.3(5) -3_444 . 1_555 N
Ba2 O4 Fe2 89.0(5) -3_444 . -103_444 N
Ba2 O4 Ca2 0.0 -3_555 . -3_555 N
Ba2 O4 Ca2 91.8(7) -3_555 . 101_545 N
Ba2 O4 Nd3 84.8(4) -3_555 . -3_555 N
Ba2 O4 Nd3 176.1(4) -3_555 . 101_545 N
Ba2 O4 Ca3 84.8(4) -3_555 . -3_555 N
Ba2 O4 Ca3 176.1(4) -3_555 . 101_545 N
Ba2 O4 Ba3 176.1(4) 101_545 . -3_444 N
Ba2 O4 Ba3 84.8(4) 101_545 . 101_545 N
Ba2 O4 Fe2 89.0(5) 101_545 . 1_555 N
Ba2 O4 Fe2 90.3(5) 101_545 . -103_444 N
Ba2 O4 Ca2 91.8(7) 101_545 . -3_555 N
Ba2 O4 Ca2 0.0 101_545 . 101_545 N
Ba2 O4 Nd3 176.1(4) 101_545 . -3_555 N
Ba2 O4 Nd3 84.8(4) 101_545 . 101_545 N
Ba2 O4 Ca3 176.1(4) 101_545 . -3_555 N
Ba2 O4 Ca3 84.8(4) 101_545 . 101_545 N
Ba3 O4 Ba3 98.7(7) -3_444 . 101_545 N
Ba3 O4 Fe2 89.1(5) -3_444 . 1_555 N
Ba3 O4 Fe2 91.6(4) -3_444 . -103_444 N
Ba3 O4 Ca2 84.8(4) -3_555 . -3_555 N
Ba3 O4 Ca2 176.1(4) -3_555 . 101_545 N
Ba3 O4 Nd3 0.0 -3_555 . -3_555 N
Ba3 O4 Nd3 98.7(7) -3_555 . 101_545 N
Ba3 O4 Ca3 0.0 -3_555 . -3_555 N
Ba3 O4 Ca3 98.7(7) -3_555 . 101_545 N
Ba3 O4 Fe2 91.6(4) 101_545 . 1_555 N
Ba3 O4 Fe2 89.1(5) 101_545 . -103_444 N
Ba3 O4 Ca2 176.1(4) 101_545 . -3_555 N
Ba3 O4 Ca2 84.8(4) 101_545 . 101_545 N
Ba3 O4 Nd3 98.7(7) 101_545 . -3_555 N
Ba3 O4 Nd3 0.0 101_545 . 101_545 N
Ba3 O4 Ca3 98.7(7) 101_545 . -3_555 N
Ba3 O4 Ca3 0.0 101_545 . 101_545 N
Fe2 O4 Fe2 178.9(8) 1_555 . -103_444 N
Fe2 O4 Ca2 90.3(5) 1_555 . -3_555 N
Fe2 O4 Ca2 89.0(5) 1_555 . 101_545 N
Fe2 O4 Nd3 89.1(5) 1_555 . -3_555 N
Fe2 O4 Nd3 91.6(4) 1_555 . 101_545 N
Fe2 O4 Ca3 89.1(5) 1_555 . -3_555 N
Fe2 O4 Ca3 91.6(4) 1_555 . 101_545 N
Fe2 O4 Ca2 89.0(5) -103_555 . -3_555 N
Fe2 O4 Ca2 90.3(5) -103_555 . 101_545 N
Fe2 O4 Nd3 91.6(4) -103_555 . -3_555 N
Fe2 O4 Nd3 89.1(5) -103_555 . 101_545 N
Fe2 O4 Ca3 91.6(4) -103_555 . -3_555 N
Fe2 O4 Ca3 89.1(5) -103_555 . 101_545 N
Ca2 O4 Ca2 91.8(7) -3_555 . 101_545 N
Ca2 O4 Nd3 84.8(4) -3_555 . -3_555 N
Ca2 O4 Nd3 176.1(4) -3_555 . 101_545 N
Ca2 O4 Ca3 84.8(4) -3_555 . -3_555 N
Ca2 O4 Ca3 176.1(4) -3_555 . 101_545 N
Ca2 O4 Nd3 176.1(4) 101_545 . -3_555 N
Ca2 O4 Nd3 84.8(4) 101_545 . 101_545 N
Ca2 O4 Ca3 176.1(4) 101_545 . -3_555 N
Ca2 O4 Ca3 84.8(4) 101_545 . 101_545 N
Nd3 O4 Nd3 98.7(7) -3_555 . 101_545 N
Nd3 O4 Ca3 0.0 -3_555 . -3_555 N
Nd3 O4 Ca3 98.7(7) -3_555 . 101_545 N
Nd3 O4 Ca3 98.7(7) 101_545 . -3_555 N
Nd3 O4 Ca3 0.0 101_545 . 101_545 N
Ca3 O4 Ca3 98.7(7) -3_555 . 101_545 N
Ba2 O5 Ba2 80.2(7) 1_555 . -103_444 N
Ba2 O5 Ba3 82.1(4) 1_555 . 1_555 N
Ba2 O5 Ba3 162.2(7) 1_555 . -103_444 N
Ba2 O5 Fe2 81.3(6) 1_555 . -3_455 N
Ba2 O5 Fe2 81.8(5) 1_555 . 101_554 N
Ba2 O5 Nd3 82.1(4) 1_555 . 1_555 N
Ba2 O5 Nd3 162.2(7) 1_555 . -103_555 N
Ba2 O5 Ca3 82.1(4) 1_555 . 1_555 N
Ba2 O5 Ca3 162.2(7) 1_555 . -103_555 N
Ba2 O5 Ba3 162.2(7) -103_444 . 1_555 N
Ba2 O5 Ba3 82.1(4) -103_444 . -103_444 N
Ba2 O5 Fe2 81.8(5) -103_444 . -3_455 N
Ba2 O5 Fe2 81.3(6) -103_444 . 101_554 N
Ba2 O5 Nd3 162.2(7) -103_555 . 1_555 N
Ba2 O5 Nd3 82.1(4) -103_555 . -103_555 N
Ba2 O5 Ca3 162.2(7) -103_555 . 1_555 N
Ba2 O5 Ca3 82.1(4) -103_555 . -103_555 N
Ba3 O5 Ba3 115.7(9) 1_555 . -103_444 N
Ba3 O5 Fe2 97.6(4) 1_555 . -3_455 N
Ba3 O5 Fe2 94.1(5) 1_555 . 101_554 N
Ba3 O5 Nd3 0.0 1_555 . 1_555 N
Ba3 O5 Nd3 115.7(9) 1_555 . -103_555 N
Ba3 O5 Ca3 0.0 1_555 . 1_555 N
Ba3 O5 Ca3 115.7(9) 1_555 . -103_555 N
Ba3 O5 Fe2 94.1(5) -103_444 . -3_455 N
Ba3 O5 Fe2 97.6(4) -103_444 . 101_554 N
Ba3 O5 Nd3 115.7(9) -103_555 . 1_555 N
Ba3 O5 Nd3 0.0 -103_555 . -103_555 N
Ba3 O5 Ca3 115.7(9) -103_555 . 1_555 N
Ba3 O5 Ca3 0.0 -103_555 . -103_555 N
Fe2 O5 Fe2 157.9(10) -3_455 . 101_554 N
Fe2 O5 Nd3 97.6(4) -3_566 . 1_555 N
Fe2 O5 Nd3 94.1(5) -3_566 . -103_555 N
Fe2 O5 Ca3 97.6(4) -3_566 . 1_555 N
Fe2 O5 Ca3 94.1(5) -3_566 . -103_555 N
Fe2 O5 Nd3 94.1(5) 101_554 . 1_555 N
Fe2 O5 Nd3 97.6(4) 101_554 . -103_555 N
Fe2 O5 Ca3 94.1(5) 101_554 . 1_555 N
Fe2 O5 Ca3 97.6(4) 101_554 . -103_555 N
Nd3 O5 Nd3 115.7(9) 1_555 . -103_555 N
Nd3 O5 Ca3 0.0 1_555 . 1_555 N
Nd3 O5 Ca3 115.7(9) 1_555 . -103_555 N
Nd3 O5 Ca3 115.7(9) -103_555 . 1_555 N
Nd3 O5 Ca3 0.0 -103_555 . -103_555 N
Ca3 O5 Ca3 115.7(9) 1_555 . -103_555 N
Ba3 O6 Ba3 96.9(6) -1_565 . -3_444 N
Ba3 O6 Ba3 179.9802 -1_565 . 101_545 N
Ba3 O6 Ba3 83.1(6) -1_565 . 103_444 N
Ba3 O6 Fe3 98.7(4) -1_565 . 1_555 N
Ba3 O6 Fe3 81.3(4) -1_565 . -101_555 N
Ba3 O6 Ba3 83.1(6) -3_444 . 101_545 N
Ba3 O6 Ba3 180.0 -3_444 . 103_444 N
Ba3 O6 Fe3 98.7(4) -3_555 . 1_555 N
Ba3 O6 Fe3 81.3(4) -3_555 . -101_555 N
Ba3 O6 Ba3 96.9(6) 101_545 . 103_444 N
Ba3 O6 Fe3 81.3(4) 101_545 . 1_555 N
Ba3 O6 Fe3 98.7(4) 101_545 . -101_555 N
Ba3 O6 Fe3 81.3(4) 103_555 . 1_555 N
Ba3 O6 Fe3 98.7(4) 103_555 . -101_555 N
Fe3 O6 Fe3 179.9657 1_555 . -101_555 N
Ba3 O7 Ba3 125.8(15) 101_545 . 103_444 N
Ba3 O7 Fe3 105.3(14) 101_545 . 1_555 N
Ba3 O7 Fe3 102.9(15) 101_545 . -101_556 N
Ba3 O7 Fe3 94.5(14) 101_545 . -102_556 N
Ba3 O7 O7 70.8(10) 101_545 . 2_655 N
Ba3 O7 Nd3 0.0 101_545 . 101_545 N
Ba3 O7 Nd3 125.8(15) 101_545 . 103_555 N
Ba3 O7 Ca3 0.0 101_545 . 101_545 N
Ba3 O7 Ca3 125.8(15) 101_545 . 103_555 N
Ba3 O7 Fe3 105.3(14) 103_555 . 1_555 N
Ba3 O7 Fe3 102.9(15) 103_555 . -101_556 N
Ba3 O7 Fe3 94.5(14) 103_555 . -102_556 N
Ba3 O7 O7 70.8(10) 103_555 . 2_655 N
Ba3 O7 Nd3 125.8(15) 103_555 . 101_545 N
Ba3 O7 Nd3 0.0 103_555 . 103_555 N
Ba3 O7 Ca3 125.8(15) 103_555 . 101_545 N
Ba3 O7 Ca3 0.0 103_555 . 103_555 N
Fe3 O7 Fe3 115.1(20) 1_555 . -101_556 N
Fe3 O7 Fe3 134.5(21) 1_555 . -102_556 N
Fe3 O7 O7 169.2(15) 1_555 . 2_655 N
Fe3 O7 Nd3 105.3(14) 1_555 . 101_545 N
Fe3 O7 Nd3 105.3(14) 1_555 . 103_555 N
Fe3 O7 Ca3 105.3(14) 1_555 . 101_545 N
Fe3 O7 Ca3 105.3(14) 1_555 . 103_555 N
Fe3 O7 Fe3 19.5(9) -101_556 . -102_556 N
Fe3 O7 O7 75.8(13) -101_556 . 2_655 N
Fe3 O7 Nd3 102.9(15) -101_556 . 101_545 N
Fe3 O7 Nd3 102.9(15) -101_556 . 103_555 N
Fe3 O7 Ca3 102.9(15) -101_556 . 101_545 N
Fe3 O7 Ca3 102.9(15) -101_556 . 103_555 N
Fe3 O7 O7 56.3(10) -102_556 . 2_655 N
Fe3 O7 Nd3 94.5(14) -102_556 . 101_545 N
Fe3 O7 Nd3 94.5(14) -102_556 . 103_555 N
Fe3 O7 Ca3 94.5(14) -102_556 . 101_545 N
Fe3 O7 Ca3 94.5(14) -102_556 . 103_555 N
O7 O7 Nd3 70.8(10) 2_655 . 101_545 N
O7 O7 Nd3 70.8(10) 2_655 . 103_555 N
O7 O7 Ca3 70.8(10) 2_655 . 101_545 N
O7 O7 Ca3 70.8(10) 2_655 . 103_555 N
Nd3 O7 Nd3 125.8(15) 101_545 . 103_555 N
Nd3 O7 Ca3 0.0 101_545 . 101_545 N
Nd3 O7 Ca3 125.8(15) 101_545 . 103_555 N
Nd3 O7 Ca3 125.8(15) 103_555 . 101_545 N
Nd3 O7 Ca3 0.0 103_555 . 103_555 N
Ca3 O7 Ca3 125.8(15) 101_545 . 103_555 N
Fe1 O8 Ba2 89.5(6) 1_555 . -3_444 N
Fe1 O8 Ba2 93.7(6) 1_555 . -3_445 N
Fe1 O8 Ba2 91.6(4) 1_555 . 101_445 N
Fe1 O8 Ba2 91.6(4) 1_555 . 101_545 N
Fe1 O8 Fe2 175.0(10) 1_555 . 1_555 N
Fe1 O8 Nd2 93.7(6) 1_555 . -3_556 N
Fe1 O8 Ca2 93.7(6) 1_555 . -3_556 N
Fe1 O8 Ca2 91.6(4) 1_555 . 101_445 N
Fe1 O8 Ca2 91.6(4) 1_555 . 101_545 N
Ba2 O8 Ba2 176.8(8) -3_444 . -3_445 N
Ba2 O8 Ba2 88.8(7) -3_444 . 101_445 N
Ba2 O8 Ba2 88.8(7) -3_444 . 101_545 N
Ba2 O8 Fe2 85.4(6) -3_444 . 1_555 N
Ba2 O8 Nd2 176.8(8) -3_555 . -3_556 N
Ba2 O8 Ca2 176.8(8) -3_555 . -3_556 N
Ba2 O8 Ca2 88.8(7) -3_555 . 101_445 N
Ba2 O8 Ca2 88.8(7) -3_555 . 101_545 N
Ba2 O8 Ba2 91.1(8) -3_445 . 101_445 N
Ba2 O8 Ba2 91.1(8) -3_445 . 101_545 N
Ba2 O8 Fe2 91.3(6) -3_445 . 1_555 N
Ba2 O8 Nd2 0.0 -3_556 . -3_556 N
Ba2 O8 Ca2 0.0 -3_556 . -3_556 N
Ba2 O8 Ca2 91.1(8) -3_556 . 101_445 N
Ba2 O8 Ca2 91.1(8) -3_556 . 101_545 N
Ba2 O8 Ba2 176.0(10) 101_445 . 101_545 N
Ba2 O8 Fe2 88.3(4) 101_445 . 1_555 N
Ba2 O8 Nd2 91.1(8) 101_445 . -3_556 N
Ba2 O8 Ca2 91.1(8) 101_445 . -3_556 N
Ba2 O8 Ca2 0.0 101_445 . 101_445 N
Ba2 O8 Ca2 176.0(10) 101_445 . 101_545 N
Ba2 O8 Fe2 88.3(4) 101_545 . 1_555 N
Ba2 O8 Nd2 91.1(8) 101_545 . -3_556 N
Ba2 O8 Ca2 91.1(8) 101_545 . -3_556 N
Ba2 O8 Ca2 176.0(10) 101_545 . 101_445 N
Ba2 O8 Ca2 0.0 101_545 . 101_545 N
Fe2 O8 Nd2 91.3(6) 1_555 . -3_556 N
Fe2 O8 Ca2 91.3(6) 1_555 . -3_556 N
Fe2 O8 Ca2 88.3(4) 1_555 . 101_445 N
Fe2 O8 Ca2 88.3(4) 1_555 . 101_545 N
Nd2 O8 Ca2 0.0 -3_556 . -3_556 N
Nd2 O8 Ca2 91.1(8) -3_556 . 101_445 N
Nd2 O8 Ca2 91.1(8) -3_556 . 101_545 N
Ca2 O8 Ca2 91.1(8) -3_556 . 101_445 N
Ca2 O8 Ca2 91.1(8) -3_556 . 101_545 N
Ca2 O8 Ca2 176.0(10) 101_445 . 101_545 N
Ba3 O9 Ba3 93.9(6) -3_444 . 101_445 N
Ba3 O9 Ba3 93.9(6) -3_444 . 101_545 N
Ba3 O9 Fe3 124.0(9) -3_555 . 1_555 N
Ba3 O9 Fe3 124.0(9) -3_555 . 2_555 N
Ba3 O9 Nd3 0.0 -3_555 . -3_555 N
Ba3 O9 Ca3 0.0 -3_555 . -3_555 N
Ba3 O9 Ca3 93.9(6) -3_555 . 101_445 N
Ba3 O9 Ca3 93.9(6) -3_555 . 101_545 N
Ba3 O9 Ba3 157.9(8) 101_445 . 101_545 N
Ba3 O9 Fe3 107.0(7) 101_445 . 1_555 N
Ba3 O9 Fe3 85.4(6) 101_445 . 2_555 N
Ba3 O9 Nd3 93.9(6) 101_445 . -3_555 N
Ba3 O9 Ca3 93.9(6) 101_445 . -3_555 N
Ba3 O9 Ca3 0.0 101_445 . 101_445 N
Ba3 O9 Ca3 157.9(8) 101_445 . 101_545 N
Ba3 O9 Fe3 85.4(6) 101_545 . 1_555 N
Ba3 O9 Fe3 107.0(7) 101_545 . 2_555 N
Ba3 O9 Nd3 93.9(6) 101_545 . -3_555 N
Ba3 O9 Ca3 93.9(6) 101_545 . -3_555 N
Ba3 O9 Ca3 157.9(8) 101_545 . 101_445 N
Ba3 O9 Ca3 0.0 101_545 . 101_545 N
Fe3 O9 Fe3 21.9(9) 1_555 . 2_555 N
Fe3 O9 Nd3 124.0(9) 1_555 . -3_555 N
Fe3 O9 Ca3 124.0(9) 1_555 . -3_555 N
Fe3 O9 Ca3 107.0(7) 1_555 . 101_445 N
Fe3 O9 Ca3 85.4(6) 1_555 . 101_545 N
Fe3 O9 Nd3 124.0(9) 2_555 . -3_555 N
Fe3 O9 Ca3 124.0(9) 2_555 . -3_555 N
Fe3 O9 Ca3 85.4(6) 2_555 . 101_445 N
Fe3 O9 Ca3 107.0(7) 2_555 . 101_545 N
Nd3 O9 Ca3 0.0 -3_555 . -3_555 N
Nd3 O9 Ca3 93.9(6) -3_555 . 101_445 N
Nd3 O9 Ca3 93.9(6) -3_555 . 101_545 N
Ca3 O9 Ca3 93.9(6) -3_555 . 101_445 N
Ca3 O9 Ca3 93.9(6) -3_555 . 101_545 N
Ca3 O9 Ca3 157.9(8) 101_445 . 101_545 N
O1 Nd1 O1 67.47(27) 1_555 . 2_555 N
O1 Nd1 O1 179.9657 1_555 . -1_555 N
O1 Nd1 O1 112.53(27) 1_555 . -2_555 N
O1 Nd1 O3 75.52(30) 1_555 . 1_545 N
O1 Nd1 O3 111.84(16) 1_555 . 2_545 N
O1 Nd1 O3 104.48(30) 1_555 . -1_565 N
O1 Nd1 O3 68.16(16) 1_555 . -2_565 N
O1 Nd1 Ba2 127.7(4) 1_555 . 3_555 N
O1 Nd1 Ba2 52.3(4) 1_555 . -3_444 N
O1 Nd1 O1 112.53(27) 2_555 . -1_555 N
O1 Nd1 O1 180.0 2_555 . -2_555 N
O1 Nd1 O3 111.84(16) 2_555 . 1_545 N
O1 Nd1 O3 75.52(30) 2_555 . 2_545 N
O1 Nd1 O3 68.16(16) 2_555 . -1_565 N
O1 Nd1 O3 104.48(30) 2_555 . -2_565 N
O1 Nd1 Ba2 127.7(4) 2_555 . 3_555 N
O1 Nd1 Ba2 52.3(4) 2_555 . -3_444 N
O1 Nd1 O1 67.47(27) -1_555 . -2_555 N
O1 Nd1 O3 104.48(30) -1_555 . 1_545 N
O1 Nd1 O3 68.16(16) -1_555 . 2_545 N
O1 Nd1 O3 75.52(30) -1_555 . -1_565 N
O1 Nd1 O3 111.84(16) -1_555 . -2_565 N
O1 Nd1 Ba2 52.3(4) -1_555 . 3_555 N
O1 Nd1 Ba2 127.7(4) -1_555 . -3_444 N
O1 Nd1 O3 68.16(16) -2_555 . 1_545 N
O1 Nd1 O3 104.48(30) -2_555 . 2_545 N
O1 Nd1 O3 111.84(16) -2_555 . -1_565 N
O1 Nd1 O3 75.52(30) -2_555 . -2_565 N
O1 Nd1 Ba2 52.3(4) -2_555 . 3_555 N
O1 Nd1 Ba2 127.7(4) -2_555 . -3_444 N
O3 Nd1 O3 68.11(29) 1_545 . 2_545 N
O3 Nd1 O3 179.972 1_545 . -1_565 N
O3 Nd1 O3 111.89(29) 1_545 . -2_565 N
O3 Nd1 Ba2 52.1(4) 1_545 . 3_555 N
O3 Nd1 Ba2 127.9(4) 1_545 . -3_444 N
O3 Nd1 O3 111.89(29) 2_545 . -1_565 N
O3 Nd1 O3 179.972 2_545 . -2_565 N
O3 Nd1 Ba2 52.1(4) 2_545 . 3_555 N
O3 Nd1 Ba2 127.9(4) 2_545 . -3_444 N
O3 Nd1 O3 68.11(29) -1_565 . -2_565 N
O3 Nd1 Ba2 127.9(4) -1_565 . 3_555 N
O3 Nd1 Ba2 52.1(4) -1_565 . -3_444 N
O3 Nd1 Ba2 127.9(4) -2_565 . 3_555 N
O3 Nd1 Ba2 52.1(4) -2_565 . -3_444 N
Ba2 Nd1 Ba2 180.0 3_555 . -3_444 N
O1 Ca1 O1 67.47(27) 1_555 . 2_555 N
O1 Ca1 O1 179.9657 1_555 . -1_555 N
O1 Ca1 O1 112.53(27) 1_555 . -2_555 N
O1 Ca1 O3 75.52(30) 1_555 . 1_545 N
O1 Ca1 O3 111.84(16) 1_555 . 2_545 N
O1 Ca1 O3 104.48(30) 1_555 . -1_565 N
O1 Ca1 O3 68.16(16) 1_555 . -2_565 N
O1 Ca1 Ba2 127.7(4) 1_555 . 3_555 N
O1 Ca1 Ba2 52.3(4) 1_555 . -3_444 N
O1 Ca1 O1 112.53(27) 2_555 . -1_555 N
O1 Ca1 O1 180.0 2_555 . -2_555 N
O1 Ca1 O3 111.84(16) 2_555 . 1_545 N
O1 Ca1 O3 75.52(30) 2_555 . 2_545 N
O1 Ca1 O3 68.16(16) 2_555 . -1_565 N
O1 Ca1 O3 104.48(30) 2_555 . -2_565 N
O1 Ca1 Ba2 127.7(4) 2_555 . 3_555 N
O1 Ca1 Ba2 52.3(4) 2_555 . -3_444 N
O1 Ca1 O1 67.47(27) -1_555 . -2_555 N
O1 Ca1 O3 104.48(30) -1_555 . 1_545 N
O1 Ca1 O3 68.16(16) -1_555 . 2_545 N
O1 Ca1 O3 75.52(30) -1_555 . -1_565 N
O1 Ca1 O3 111.84(16) -1_555 . -2_565 N
O1 Ca1 Ba2 52.3(4) -1_555 . 3_555 N
O1 Ca1 Ba2 127.7(4) -1_555 . -3_444 N
O1 Ca1 O3 68.16(16) -2_555 . 1_545 N
O1 Ca1 O3 104.48(30) -2_555 . 2_545 N
O1 Ca1 O3 111.84(16) -2_555 . -1_565 N
O1 Ca1 O3 75.52(30) -2_555 . -2_565 N
O1 Ca1 Ba2 52.3(4) -2_555 . 3_555 N
O1 Ca1 Ba2 127.7(4) -2_555 . -3_444 N
O3 Ca1 O3 68.11(29) 1_545 . 2_545 N
O3 Ca1 O3 179.972 1_545 . -1_565 N
O3 Ca1 O3 111.89(29) 1_545 . -2_565 N
O3 Ca1 Ba2 52.1(4) 1_545 . 3_555 N
O3 Ca1 Ba2 127.9(4) 1_545 . -3_444 N
O3 Ca1 O3 111.89(29) 2_545 . -1_565 N
O3 Ca1 O3 179.972 2_545 . -2_565 N
O3 Ca1 Ba2 52.1(4) 2_545 . 3_555 N
O3 Ca1 Ba2 127.9(4) 2_545 . -3_444 N
O3 Ca1 O3 68.11(29) -1_565 . -2_565 N
O3 Ca1 Ba2 127.9(4) -1_565 . 3_555 N
O3 Ca1 Ba2 52.1(4) -1_565 . -3_444 N
O3 Ca1 Ba2 127.9(4) -2_565 . 3_555 N
O3 Ca1 Ba2 52.1(4) -2_565 . -3_444 N
Ba2 Ca1 Ba2 180.0 3_555 . -3_444 N
Ba2 Nd2 Ba2 90.250(30) -103_343 . -103_344 N
Ba2 Nd2 Ba2 88.1(10) -103_343 . -103_443 N
Ba2 Nd2 Ba2 178.3(10) -103_343 . -103_444 N
Ba2 Nd2 Ba3 88.6(4) -103_343 . 1_555 N
Ba2 Nd2 O8 135.9(5) -103_454 . -3_566 N
Ba2 Nd2 Nd3 88.6(4) -103_454 . 1_555 N
Ba2 Nd2 Ca3 88.6(4) -103_454 . 1_555 N
Ba2 Nd2 Ba2 178.3(10) -103_344 . -103_443 N
Ba2 Nd2 Ba2 91.4(10) -103_344 . -103_444 N
Ba2 Nd2 Ba3 91.36(35) -103_344 . 1_555 N
Ba2 Nd2 O8 45.7(5) -103_455 . -3_566 N
Ba2 Nd2 Nd3 91.36(35) -103_455 . 1_555 N
Ba2 Nd2 Ca3 91.36(35) -103_455 . 1_555 N
Ba2 Nd2 Ba2 90.250(30) -103_443 . -103_444 N
Ba2 Nd2 Ba3 88.6(4) -103_443 . 1_555 N
Ba2 Nd2 O8 135.9(5) -103_554 . -3_566 N
Ba2 Nd2 Nd3 88.6(4) -103_554 . 1_555 N
Ba2 Nd2 Ca3 88.6(4) -103_554 . 1_555 N
Ba2 Nd2 Ba3 91.36(35) -103_444 . 1_555 N
Ba2 Nd2 O8 45.7(5) -103_555 . -3_566 N
Ba2 Nd2 Nd3 91.36(35) -103_555 . 1_555 N
Ba2 Nd2 Ca3 91.36(35) -103_555 . 1_555 N
Ba3 Nd2 O8 93.6(7) 1_555 . -3_566 N
Ba3 Nd2 Nd3 0.0 1_555 . 1_555 N
Ba3 Nd2 Ca3 0.0 1_555 . 1_555 N
O8 Nd2 Nd3 93.6(7) -3_566 . 1_555 N
O8 Nd2 Ca3 93.6(7) -3_566 . 1_555 N
Nd3 Nd2 Ca3 0.0 1_555 . 1_555 N
Ba2 Ca2 Ba2 90.250(30) -103_343 . -103_344 N
Ba2 Ca2 Ba2 88.1(10) -103_343 . -103_443 N
Ba2 Ca2 Ba2 178.3(10) -103_343 . -103_444 N
Ba2 Ca2 Ba3 88.6(4) -103_343 . 1_555 N
Ba2 Ca2 O4 44.1(4) -103_454 . -3_565 N
Ba2 Ca2 O4 88.6(7) -103_454 . -4_565 N
Ba2 Ca2 O8 135.9(5) -103_454 . -3_566 N
Ba2 Ca2 O8 47.1(4) -103_454 . 101_454 N
Ba2 Ca2 O8 135.2(12) -103_454 . 101_554 N
Ba2 Ca2 Ca2 90.250(30) -103_454 . -103_455 N
Ba2 Ca2 Ca2 178.3(10) -103_454 . -103_555 N
Ba2 Ca2 Nd3 88.6(4) -103_454 . 1_555 N
Ba2 Ca2 Ca3 88.6(4) -103_454 . 1_555 N
Ba2 Ca2 Ba2 178.3(10) -103_344 . -103_443 N
Ba2 Ca2 Ba2 91.4(10) -103_344 . -103_444 N
Ba2 Ca2 Ba3 91.36(35) -103_344 . 1_555 N
Ba2 Ca2 O4 90.179(21) -103_455 . -3_565 N
Ba2 Ca2 O4 135.86(35) -103_455 . -4_565 N
Ba2 Ca2 O8 45.7(5) -103_455 . -3_566 N
Ba2 Ca2 O8 43.2(4) -103_455 . 101_454 N
Ba2 Ca2 O8 134.5(12) -103_455 . 101_554 N
Ba2 Ca2 Ca2 0.0 -103_455 . -103_455 N
Ba2 Ca2 Ca2 91.4(10) -103_455 . -103_555 N
Ba2 Ca2 Nd3 91.36(35) -103_455 . 1_555 N
Ba2 Ca2 Ca3 91.36(35) -103_455 . 1_555 N
Ba2 Ca2 Ba2 90.250(30) -103_443 . -103_444 N
Ba2 Ca2 Ba3 88.6(4) -103_443 . 1_555 N
Ba2 Ca2 O4 88.6(7) -103_554 . -3_565 N
Ba2 Ca2 O4 44.1(4) -103_554 . -4_565 N
Ba2 Ca2 O8 135.9(5) -103_554 . -3_566 N
Ba2 Ca2 O8 135.2(12) -103_554 . 101_454 N
Ba2 Ca2 O8 47.1(4) -103_554 . 101_554 N
Ba2 Ca2 Ca2 178.3(10) -103_554 . -103_455 N
Ba2 Ca2 Ca2 90.250(30) -103_554 . -103_555 N
Ba2 Ca2 Nd3 88.6(4) -103_554 . 1_555 N
Ba2 Ca2 Ca3 88.6(4) -103_554 . 1_555 N
Ba2 Ca2 Ba3 91.36(35) -103_444 . 1_555 N
Ba2 Ca2 O4 135.86(35) -103_555 . -3_565 N
Ba2 Ca2 O4 90.179(21) -103_555 . -4_565 N
Ba2 Ca2 O8 45.7(5) -103_555 . -3_566 N
Ba2 Ca2 O8 134.5(12) -103_555 . 101_454 N
Ba2 Ca2 O8 43.2(4) -103_555 . 101_554 N
Ba2 Ca2 Ca2 91.4(10) -103_555 . -103_455 N
Ba2 Ca2 Ca2 0.0 -103_555 . -103_555 N
Ba2 Ca2 Nd3 91.36(35) -103_555 . 1_555 N
Ba2 Ca2 Ca3 91.36(35) -103_555 . 1_555 N
Ba3 Ca2 O4 44.51(35) 1_555 . -3_565 N
Ba3 Ca2 O4 44.51(35) 1_555 . -4_565 N
Ba3 Ca2 O8 93.6(7) 1_555 . -3_566 N
Ba3 Ca2 O8 91.7(4) 1_555 . 101_454 N
Ba3 Ca2 O8 91.7(4) 1_555 . 101_554 N
Ba3 Ca2 Ca2 91.36(35) 1_555 . -103_455 N
Ba3 Ca2 Ca2 91.36(35) 1_555 . -103_555 N
Ba3 Ca2 Nd3 0.0 1_555 . 1_555 N
Ba3 Ca2 Ca3 0.0 1_555 . 1_555 N
O4 Ca2 O4 59.9(4) -3_565 . -4_565 N
O4 Ca2 O8 122.4(6) -3_565 . -3_566 N
O4 Ca2 O8 62.0(4) -3_565 . 101_454 N
O4 Ca2 O8 121.9(7) -3_565 . 101_554 N
O4 Ca2 Ca2 90.179(21) -3_565 . -103_455 N
O4 Ca2 Ca2 135.86(35) -3_565 . -103_555 N
O4 Ca2 Nd3 44.51(35) -3_565 . 1_555 N
O4 Ca2 Ca3 44.51(35) -3_565 . 1_555 N
O4 Ca2 O8 122.4(6) -4_565 . -3_566 N
O4 Ca2 O8 121.9(7) -4_565 . 101_454 N
O4 Ca2 O8 62.0(4) -4_565 . 101_554 N
O4 Ca2 Ca2 135.86(35) -4_565 . -103_455 N
O4 Ca2 Ca2 90.179(21) -4_565 . -103_555 N
O4 Ca2 Nd3 44.51(35) -4_565 . 1_555 N
O4 Ca2 Ca3 44.51(35) -4_565 . 1_555 N
O8 Ca2 O8 88.8(7) -3_566 . 101_454 N
O8 Ca2 O8 88.8(7) -3_566 . 101_554 N
O8 Ca2 Ca2 45.7(5) -3_566 . -103_455 N
O8 Ca2 Ca2 45.7(5) -3_566 . -103_555 N
O8 Ca2 Nd3 93.6(7) -3_566 . 1_555 N
O8 Ca2 Ca3 93.6(7) -3_566 . 1_555 N
O8 Ca2 O8 176.0(10) 101_454 . 101_554 N
O8 Ca2 Ca2 43.2(4) 101_454 . -103_455 N
O8 Ca2 Ca2 134.5(12) 101_454 . -103_555 N
O8 Ca2 Nd3 91.7(4) 101_454 . 1_555 N
O8 Ca2 Ca3 91.7(4) 101_454 . 1_555 N
O8 Ca2 Ca2 134.5(12) 101_554 . -103_455 N
O8 Ca2 Ca2 43.2(4) 101_554 . -103_555 N
O8 Ca2 Nd3 91.7(4) 101_554 . 1_555 N
O8 Ca2 Ca3 91.7(4) 101_554 . 1_555 N
Ca2 Ca2 Ca2 91.4(10) -103_455 . -103_555 N
Ca2 Ca2 Nd3 91.36(35) -103_455 . 1_555 N
Ca2 Ca2 Ca3 91.36(35) -103_455 . 1_555 N
Ca2 Ca2 Nd3 91.36(35) -103_555 . 1_555 N
Ca2 Ca2 Ca3 91.36(35) -103_555 . 1_555 N
Nd3 Ca2 Ca3 0.0 1_555 . 1_555 N
Ba2 Nd3 Ba3 91.34(35) 1_555 . -103_343 N
Ba2 Nd3 Ba3 91.34(35) 1_555 . -103_443 N
Ba2 Nd3 O4 50.7(4) 1_555 . -3_565 N
Ba2 Nd3 O4 50.7(4) 1_555 . -4_565 N
Ba2 Nd3 O5 56.4(5) 1_555 . 1_555 N
Ba2 Nd3 O5 56.4(5) 1_555 . 2_555 N
Ba2 Nd3 O7 151.5(9) 1_555 . 101_454 N
Ba2 Nd3 O7 151.5(9) 1_555 . 102_554 N
Ba2 Nd3 O9 103.1(8) 1_555 . -3_565 N
Ba2 Nd3 Nd2 0.0 1_555 . 1_555 N
Ba2 Nd3 Ca2 0.0 1_555 . 1_555 N
Ba3 Nd3 Ba3 93.2(9) -103_343 . -103_443 N
Ba3 Nd3 O4 40.64(34) -103_454 . -3_565 N
Ba3 Nd3 O4 92.4(7) -103_454 . -4_565 N
Ba3 Nd3 O5 147.7(4) -103_454 . 1_555 N
Ba3 Nd3 O5 90.15(4) -103_454 . 2_555 N
Ba3 Nd3 O7 88.7(12) -103_454 . 101_454 N
Ba3 Nd3 O7 117.1(8) -103_454 . 102_554 N
Ba3 Nd3 O9 47.6(5) -103_454 . -3_565 N
Ba3 Nd3 Nd2 91.34(35) -103_454 . 1_555 N
Ba3 Nd3 Ca2 91.34(35) -103_454 . 1_555 N
Ba3 Nd3 O4 92.4(7) -103_554 . -3_565 N
Ba3 Nd3 O4 40.64(34) -103_554 . -4_565 N
Ba3 Nd3 O5 90.15(4) -103_554 . 1_555 N
Ba3 Nd3 O5 147.7(4) -103_554 . 2_555 N
Ba3 Nd3 O7 117.1(8) -103_554 . 101_454 N
Ba3 Nd3 O7 88.7(12) -103_554 . 102_554 N
Ba3 Nd3 O9 47.6(5) -103_554 . -3_565 N
Ba3 Nd3 Nd2 91.34(35) -103_554 . 1_555 N
Ba3 Nd3 Ca2 91.34(35) -103_554 . 1_555 N
O4 Nd3 O4 66.9(4) -3_565 . -4_565 N
O4 Nd3 O5 107.1(6) -3_565 . 1_555 N
O4 Nd3 O5 69.84(31) -3_565 . 2_555 N
O4 Nd3 O7 124.2(12) -3_565 . 101_454 N
O4 Nd3 O7 157.7(9) -3_565 . 102_554 N
O4 Nd3 O9 67.3(6) -3_565 . -3_565 N
O4 Nd3 Nd2 50.7(4) -3_565 . 1_555 N
O4 Nd3 Ca2 50.7(4) -3_565 . 1_555 N
O4 Nd3 O5 69.84(31) -4_565 . 1_555 N
O4 Nd3 O5 107.1(6) -4_565 . 2_555 N
O4 Nd3 O7 157.7(9) -4_565 . 101_454 N
O4 Nd3 O7 124.2(12) -4_565 . 102_554 N
O4 Nd3 O9 67.3(6) -4_565 . -3_565 N
O4 Nd3 Nd2 50.7(4) -4_565 . 1_555 N
O4 Nd3 Ca2 50.7(4) -4_565 . 1_555 N
O5 Nd3 O5 70.9(5) 1_555 . 2_555 N
O5 Nd3 O7 118.1(14) 1_555 . 101_454 N
O5 Nd3 O7 95.1(9) 1_555 . 102_554 N
O5 Nd3 O9 135.1(6) 1_555 . -3_565 N
O5 Nd3 Nd2 56.4(5) 1_555 . 1_555 N
O5 Nd3 Ca2 56.4(5) 1_555 . 1_555 N
O5 Nd3 O7 95.1(9) 2_555 . 101_454 N
O5 Nd3 O7 118.1(14) 2_555 . 102_554 N
O5 Nd3 O9 135.1(6) 2_555 . -3_565 N
O5 Nd3 Nd2 56.4(5) 2_555 . 1_555 N
O5 Nd3 Ca2 56.4(5) 2_555 . 1_555 N
O7 Nd3 O7 38.5(20) 101_454 . 102_554 N
O7 Nd3 O9 97.9(12) 101_454 . -3_565 N
O7 Nd3 Nd2 151.5(9) 101_454 . 1_555 N
O7 Nd3 Ca2 151.5(9) 101_454 . 1_555 N
O7 Nd3 O9 97.9(12) 102_554 . -3_565 N
O7 Nd3 Nd2 151.5(9) 102_554 . 1_555 N
O7 Nd3 Ca2 151.5(9) 102_554 . 1_555 N
O9 Nd3 Nd2 103.1(8) -3_565 . 1_555 N
O9 Nd3 Ca2 103.1(8) -3_565 . 1_555 N
Nd2 Nd3 Ca2 0.0 1_555 . 1_555 N
Ba2 Ca3 Ba3 91.34(35) 1_555 . -103_343 N
Ba2 Ca3 Ba3 88.6(4) 1_555 . -103_344 N
Ba2 Ca3 Ba3 91.34(35) 1_555 . -103_443 N
Ba2 Ca3 Ba3 88.6(4) 1_555 . -103_444 N
Ba2 Ca3 Fe2 60.4(5) 1_555 . -3_454 N
Ba2 Ca3 O4 50.7(4) 1_555 . -3_565 N
Ba2 Ca3 O4 50.7(4) 1_555 . -4_565 N
Ba2 Ca3 O5 56.4(5) 1_555 . 1_555 N
Ba2 Ca3 O5 56.4(5) 1_555 . 2_555 N
Ba2 Ca3 O7 151.5(9) 1_555 . 101_454 N
Ba2 Ca3 O7 151.5(9) 1_555 . 102_554 N
Ba2 Ca3 O9 103.1(8) 1_555 . -3_565 N
Ba2 Ca3 O9 99.6(4) 1_555 . 101_454 N
Ba2 Ca3 O9 99.6(4) 1_555 . 101_554 N
Ba2 Ca3 Nd2 0.0 1_555 . 1_555 N
Ba2 Ca3 Ca2 0.0 1_555 . 1_555 N
Ba2 Ca3 Ca3 91.34(35) 1_555 . -103_454 N
Ba2 Ca3 Ca3 91.34(35) 1_555 . -103_554 N
Ba3 Ca3 Ba3 90.18(5) -103_343 . -103_344 N
Ba3 Ca3 Ba3 93.2(9) -103_343 . -103_443 N
Ba3 Ca3 Ba3 176.7(8) -103_343 . -103_444 N
Ba3 Ca3 Fe2 54.2(4) -103_343 . -3_454 N
Ba3 Ca3 O4 40.64(34) -103_454 . -3_565 N
Ba3 Ca3 O4 92.4(7) -103_454 . -4_565 N
Ba3 Ca3 O5 147.7(4) -103_454 . 1_555 N
Ba3 Ca3 O5 90.15(4) -103_454 . 2_555 N
Ba3 Ca3 O7 88.7(12) -103_454 . 101_454 N
Ba3 Ca3 O7 117.1(8) -103_454 . 102_554 N
Ba3 Ca3 O9 47.6(5) -103_454 . -3_565 N
Ba3 Ca3 O9 38.5(4) -103_454 . 101_454 N
Ba3 Ca3 O9 130.0(9) -103_454 . 101_554 N
Ba3 Ca3 Nd2 91.34(35) -103_454 . 1_555 N
Ba3 Ca3 Ca2 91.34(35) -103_454 . 1_555 N
Ba3 Ca3 Ca3 0.0 -103_454 . -103_454 N
Ba3 Ca3 Ca3 93.2(9) -103_454 . -103_554 N
Ba3 Ca3 Ba3 176.7(8) -103_344 . -103_443 N
Ba3 Ca3 Ba3 86.5(8) -103_344 . -103_444 N
Ba3 Ca3 Fe2 128.36(25) -103_344 . -3_454 N
Ba3 Ca3 O4 90.13(4) -103_455 . -3_565 N
Ba3 Ca3 O4 139.3(4) -103_455 . -4_565 N
Ba3 Ca3 O5 87.0(7) -103_455 . 1_555 N
Ba3 Ca3 O5 32.1(5) -103_455 . 2_555 N
Ba3 Ca3 O7 62.9(8) -103_455 . 101_454 N
Ba3 Ca3 O7 89.8(13) -103_455 . 102_554 N
Ba3 Ca3 O9 135.6(4) -103_455 . -3_565 N
Ba3 Ca3 O9 53.3(4) -103_455 . 101_454 N
Ba3 Ca3 O9 138.3(9) -103_455 . 101_554 N
Ba3 Ca3 Nd2 88.6(4) -103_455 . 1_555 N
Ba3 Ca3 Ca2 88.6(4) -103_455 . 1_555 N
Ba3 Ca3 Ca3 90.18(5) -103_455 . -103_454 N
Ba3 Ca3 Ca3 176.7(8) -103_455 . -103_554 N
Ba3 Ca3 Ba3 90.18(5) -103_443 . -103_444 N
Ba3 Ca3 Fe2 54.2(4) -103_443 . -3_454 N
Ba3 Ca3 O4 92.4(7) -103_554 . -3_565 N
Ba3 Ca3 O4 40.64(34) -103_554 . -4_565 N
Ba3 Ca3 O5 90.15(4) -103_554 . 1_555 N
Ba3 Ca3 O5 147.7(4) -103_554 . 2_555 N
Ba3 Ca3 O7 117.1(8) -103_554 . 101_454 N
Ba3 Ca3 O7 88.7(12) -103_554 . 102_554 N
Ba3 Ca3 O9 47.6(5) -103_554 . -3_565 N
Ba3 Ca3 O9 130.0(9) -103_554 . 101_454 N
Ba3 Ca3 O9 38.5(4) -103_554 . 101_554 N
Ba3 Ca3 Nd2 91.34(35) -103_554 . 1_555 N
Ba3 Ca3 Ca2 91.34(35) -103_554 . 1_555 N
Ba3 Ca3 Ca3 93.2(9) -103_554 . -103_454 N
Ba3 Ca3 Ca3 0.0 -103_554 . -103_554 N
Ba3 Ca3 Fe2 128.36(25) -103_444 . -3_454 N
Ba3 Ca3 O4 139.3(4) -103_555 . -3_565 N
Ba3 Ca3 O4 90.13(4) -103_555 . -4_565 N
Ba3 Ca3 O5 32.1(5) -103_555 . 1_555 N
Ba3 Ca3 O5 87.0(7) -103_555 . 2_555 N
Ba3 Ca3 O7 89.8(13) -103_555 . 101_454 N
Ba3 Ca3 O7 62.9(8) -103_555 . 102_554 N
Ba3 Ca3 O9 135.6(4) -103_555 . -3_565 N
Ba3 Ca3 O9 138.3(9) -103_555 . 101_454 N
Ba3 Ca3 O9 53.3(4) -103_555 . 101_554 N
Ba3 Ca3 Nd2 88.6(4) -103_555 . 1_555 N
Ba3 Ca3 Ca2 88.6(4) -103_555 . 1_555 N
Ba3 Ca3 Ca3 176.7(8) -103_555 . -103_454 N
Ba3 Ca3 Ca3 90.18(5) -103_555 . -103_554 N
Fe2 Ca3 O4 38.25(29) -3_565 . -3_565 N
Fe2 Ca3 O4 38.25(29) -3_565 . -4_565 N
Fe2 Ca3 O5 104.3(5) -3_565 . 1_555 N
Fe2 Ca3 O5 104.3(5) -3_565 . 2_555 N
Fe2 Ca3 O7 137.2(13) -3_565 . 101_454 N
Fe2 Ca3 O7 137.2(13) -3_565 . 102_554 N
Fe2 Ca3 O9 42.7(5) -3_565 . -3_565 N
Fe2 Ca3 O9 89.9(6) -3_565 . 101_454 N
Fe2 Ca3 O9 89.9(6) -3_565 . 101_554 N
Fe2 Ca3 Nd2 60.4(5) -3_565 . 1_555 N
Fe2 Ca3 Ca2 60.4(5) -3_565 . 1_555 N
Fe2 Ca3 Ca3 54.2(4) -3_565 . -103_454 N
Fe2 Ca3 Ca3 54.2(4) -3_565 . -103_554 N
O4 Ca3 O4 66.9(4) -3_565 . -4_565 N
O4 Ca3 O5 107.1(6) -3_565 . 1_555 N
O4 Ca3 O5 69.84(31) -3_565 . 2_555 N
O4 Ca3 O7 124.2(12) -3_565 . 101_454 N
O4 Ca3 O7 157.7(9) -3_565 . 102_554 N
O4 Ca3 O9 67.3(6) -3_565 . -3_565 N
O4 Ca3 O9 60.8(4) -3_565 . 101_454 N
O4 Ca3 O9 126.4(7) -3_565 . 101_554 N
O4 Ca3 Nd2 50.7(4) -3_565 . 1_555 N
O4 Ca3 Ca2 50.7(4) -3_565 . 1_555 N
O4 Ca3 Ca3 40.64(34) -3_565 . -103_454 N
O4 Ca3 Ca3 92.4(7) -3_565 . -103_554 N
O4 Ca3 O5 69.84(31) -4_565 . 1_555 N
O4 Ca3 O5 107.1(6) -4_565 . 2_555 N
O4 Ca3 O7 157.7(9) -4_565 . 101_454 N
O4 Ca3 O7 124.2(12) -4_565 . 102_554 N
O4 Ca3 O9 67.3(6) -4_565 . -3_565 N
O4 Ca3 O9 126.4(7) -4_565 . 101_454 N
O4 Ca3 O9 60.8(4) -4_565 . 101_554 N
O4 Ca3 Nd2 50.7(4) -4_565 . 1_555 N
O4 Ca3 Ca2 50.7(4) -4_565 . 1_555 N
O4 Ca3 Ca3 92.4(7) -4_565 . -103_454 N
O4 Ca3 Ca3 40.64(34) -4_565 . -103_554 N
O5 Ca3 O5 70.9(5) 1_555 . 2_555 N
O5 Ca3 O7 118.1(14) 1_555 . 101_454 N
O5 Ca3 O7 95.1(9) 1_555 . 102_554 N
O5 Ca3 O9 135.1(6) 1_555 . -3_565 N
O5 Ca3 O9 135.9(7) 1_555 . 101_454 N
O5 Ca3 O9 65.2(4) 1_555 . 101_554 N
O5 Ca3 Nd2 56.4(5) 1_555 . 1_555 N
O5 Ca3 Ca2 56.4(5) 1_555 . 1_555 N
O5 Ca3 Ca3 147.7(4) 1_555 . -103_454 N
O5 Ca3 Ca3 90.15(4) 1_555 . -103_554 N
O5 Ca3 O7 95.1(9) 2_555 . 101_454 N
O5 Ca3 O7 118.1(14) 2_555 . 102_554 N
O5 Ca3 O9 135.1(6) 2_555 . -3_565 N
O5 Ca3 O9 65.2(4) 2_555 . 101_454 N
O5 Ca3 O9 135.9(7) 2_555 . 101_554 N
O5 Ca3 Nd2 56.4(5) 2_555 . 1_555 N
O5 Ca3 Ca2 56.4(5) 2_555 . 1_555 N
O5 Ca3 Ca3 90.15(4) 2_555 . -103_454 N
O5 Ca3 Ca3 147.7(4) 2_555 . -103_554 N
O7 Ca3 O7 38.5(20) 101_454 . 102_554 N
O7 Ca3 O9 97.9(12) 101_454 . -3_565 N
O7 Ca3 O9 64.1(11) 101_454 . 101_454 N
O7 Ca3 O9 102.2(11) 101_454 . 101_554 N
O7 Ca3 Nd2 151.5(9) 101_454 . 1_555 N
O7 Ca3 Ca2 151.5(9) 101_454 . 1_555 N
O7 Ca3 Ca3 88.7(12) 101_454 . -103_454 N
O7 Ca3 Ca3 117.1(8) 101_454 . -103_554 N
O7 Ca3 O9 97.9(12) 102_554 . -3_565 N
O7 Ca3 O9 102.2(11) 102_554 . 101_454 N
O7 Ca3 O9 64.1(11) 102_554 . 101_554 N
O7 Ca3 Nd2 151.5(9) 102_554 . 1_555 N
O7 Ca3 Ca2 151.5(9) 102_554 . 1_555 N
O7 Ca3 Ca3 117.1(8) 102_554 . -103_454 N
O7 Ca3 Ca3 88.7(12) 102_554 . -103_554 N
O9 Ca3 O9 82.4(5) -3_565 . 101_454 N
O9 Ca3 O9 82.4(5) -3_565 . 101_554 N
O9 Ca3 Nd2 103.1(8) -3_565 . 1_555 N
O9 Ca3 Ca2 103.1(8) -3_565 . 1_555 N
O9 Ca3 Ca3 47.6(5) -3_565 . -103_454 N
O9 Ca3 Ca3 47.6(5) -3_565 . -103_554 N
O9 Ca3 O9 157.9(8) 101_454 . 101_554 N
O9 Ca3 Nd2 99.6(4) 101_454 . 1_555 N
O9 Ca3 Ca2 99.6(4) 101_454 . 1_555 N
O9 Ca3 Ca3 38.5(4) 101_454 . -103_454 N
O9 Ca3 Ca3 130.0(9) 101_454 . -103_554 N
O9 Ca3 Nd2 99.6(4) 101_554 . 1_555 N
O9 Ca3 Ca2 99.6(4) 101_554 . 1_555 N
O9 Ca3 Ca3 130.0(9) 101_554 . -103_454 N
O9 Ca3 Ca3 38.5(4) 101_554 . -103_554 N
Nd2 Ca3 Ca2 0.0 1_555 . 1_555 N
Nd2 Ca3 Ca3 91.34(35) 1_555 . -103_454 N
Nd2 Ca3 Ca3 91.34(35) 1_555 . -103_554 N
Ca2 Ca3 Ca3 91.34(35) 1_555 . -103_454 N
Ca2 Ca3 Ca3 91.34(35) 1_555 . -103_554 N
Ca3 Ca3 Ca3 93.2(9) -103_454 . -103_554 N
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Fe1 O1 2.038(8) . 1_555 N
Fe1 O1 2.038(8) . 2_555 N
Fe1 O3 2.007(8) . -1_566 N
Fe1 O3 2.007(8) . -2_566 N
Fe1 Ba2 3.519(23) . -3_545 N
Fe1 Ba2 3.409(23) . -3_546 N
Fe1 Ba2 3.453(10) . 101_445 N
Fe1 Ba2 3.453(10) . 101_545 N
Fe1 O8 1.955(15) . 1_555 N
Fe1 Nd1 3.439(10) . 1_555 N
Fe1 Nd1 3.394(9) . 1_556 N
Fe1 Nd1 3.406(4) . 103_455 N
Fe1 Nd1 3.406(4) . 103_555 N
Fe1 Ca1 3.439(10) . 1_555 N
Fe1 Ca1 3.394(9) . 1_556 N
Fe1 Ca1 3.406(4) . 103_455 N
Fe1 Ca1 3.406(4) . 103_555 N
Fe1 Nd2 3.409(23) . -3_546 N
Fe1 Nd2 3.453(10) . 101_445 N
Fe1 Nd2 3.453(10) . 101_545 N
Fe1 Ca2 3.519(23) . -3_545 N
Fe1 Ca2 3.409(23) . -3_546 N
Fe1 Ca2 3.453(10) . 101_445 N
Fe1 Ca2 3.453(10) . 101_545 N
O1 Fe1 2.038(8) . 1_555 N
O1 Fe1 2.038(8) . -103_444 N
O1 Ba2 3.154(21) . -3_545 N
O1 Ba2 3.154(21) . 101_545 N
O1 Nd1 2.514(9) . 1_555 N
O1 Nd1 2.514(9) . 103_555 N
O1 Ca1 2.514(9) . 1_555 N
O1 Ca1 2.514(9) . 103_555 N
O1 Ca2 3.154(21) . -3_545 N
O1 Ca2 3.154(21) . 101_545 N
O3 Fe1 2.007(8) . -1_566 N
O3 Fe1 2.007(8) . 103_564 N
O3 Ba2 3.145(21) . 3_565 N
O3 Ba2 3.145(21) . -101_454 N
O3 Nd1 2.493(9) . 1_565 N
O3 Nd1 2.493(9) . 103_565 N
O3 Ca1 2.493(9) . 1_565 N
O3 Ca1 2.493(9) . 103_565 N
O3 Ca2 3.145(21) . 3_565 N
O3 Ca2 3.145(21) . -101_454 N
Ba2 Fe1 3.519(23) . -3_555 N
Ba2 Fe1 3.409(23) . -3_556 N
Ba2 Fe1 3.453(10) . 101_454 N
Ba2 Fe1 3.453(10) . 101_554 N
Ba2 O1 3.154(21) . -3_555 N
Ba2 O1 3.154(21) . -4_555 N
Ba2 O3 3.145(21) . 3_565 N
Ba2 O3 3.145(21) . 4_565 N
Ba2 Ba2 4.02(4) . -103_343 N
Ba2 Ba2 3.901(35) . -103_344 N
Ba2 Ba2 4.02(4) . -103_443 N
Ba2 Ba2 3.901(35) . -103_444 N
Ba2 Ba3 3.598(15) . 1_555 N
Ba2 Fe2 3.429(23) . -3_555 N
Ba2 Fe2 3.379(24) . -3_556 N
Ba2 Fe2 3.393(10) . 101_454 N
Ba2 Fe2 3.393(10) . 101_554 N
Ba2 O4 2.796(18) . -3_555 N
Ba2 O4 2.796(18) . -4_555 N
Ba2 O5 3.027(22) . 1_555 N
Ba2 O5 3.027(22) . 2_555 N
Ba2 O8 2.943(23) . -3_555 N
Ba2 O8 2.670(23) . -3_556 N
Ba2 O8 2.7936(9) . 101_454 N
Ba2 O8 2.7936(9) . 101_554 N
Ba2 Nd1 3.983(15) . 3_555 N
Ba2 Ca1 3.983(15) . 3_555 N
Ba2 Nd2 4.02(4) . -103_343 N
Ba2 Nd2 3.901(35) . -103_344 N
Ba2 Nd2 4.02(4) . -103_443 N
Ba2 Nd2 3.901(35) . -103_444 N
Ba2 Ca2 4.02(4) . -103_343 N
Ba2 Ca2 3.901(35) . -103_344 N
Ba2 Ca2 4.02(4) . -103_443 N
Ba2 Ca2 3.901(35) . -103_444 N
Ba2 Nd3 3.598(15) . 1_555 N
Ba2 Ca3 3.598(15) . 1_555 N
Ba3 Ba2 3.598(15) . 1_555 N
Ba3 Ba3 4.338(25) . 3_565 N
Ba3 Ba3 3.844(28) . -103_343 N
Ba3 Ba3 4.075(29) . -103_344 N
Ba3 Ba3 3.844(28) . -103_443 N
Ba3 Ba3 4.075(29) . -103_444 N
Ba3 Fe2 3.185(20) . -3_555 N
Ba3 Fe2 3.343(19) . -3_556 N
Ba3 Fe2 3.253(7) . 101_454 N
Ba3 Fe2 3.253(7) . 101_554 N
Ba3 Fe3 3.798(21) . -1_565 N
Ba3 Fe3 3.340(22) . -1_566 N
Ba3 Fe3 3.798(21) . -2_565 N
Ba3 Fe3 3.340(22) . -2_566 N
Ba3 Fe3 3.290(15) . 101_454 N
Ba3 Fe3 3.854(13) . 101_554 N
Ba3 Fe3 3.854(13) . 102_454 N
Ba3 Fe3 3.290(15) . 102_554 N
Ba3 O4 2.533(15) . -3_555 N
Ba3 O4 2.533(15) . -4_555 N
Ba3 O5 2.407(16) . 1_555 N
Ba3 O5 2.407(16) . 2_555 N
Ba3 O6 2.898(12) . -1_565 N
Ba3 O6 2.898(12) . -2_565 N
Ba3 O7 2.437(19) . 101_454 N
Ba3 O7 2.437(19) . 102_554 N
Ba3 O9 2.397(28) . -3_555 N
Ba3 O9 3.292(28) . -3_556 N
Ba3 O9 2.845(4) . 101_454 N
Ba3 O9 2.845(4) . 101_554 N
Ba3 Nd2 3.598(15) . 1_555 N
Ba3 Ca2 3.598(15) . 1_555 N
Ba3 Nd3 4.338(25) . 3_565 N
Ba3 Nd3 3.844(28) . -103_343 N
Ba3 Nd3 4.075(29) . -103_344 N
Ba3 Nd3 3.844(28) . -103_443 N
Ba3 Nd3 4.075(29) . -103_444 N
Ba3 Ca3 4.338(25) . 3_565 N
Ba3 Ca3 3.844(28) . -103_343 N
Ba3 Ca3 4.075(29) . -103_344 N
Ba3 Ca3 3.844(28) . -103_443 N
Ba3 Ca3 4.075(29) . -103_444 N
Fe2 Ba2 3.429(23) . -3_545 N
Fe2 Ba2 3.379(24) . -3_546 N
Fe2 Ba2 3.393(10) . 101_445 N
Fe2 Ba2 3.393(10) . 101_545 N
Fe2 Ba3 3.185(20) . -3_545 N
Fe2 Ba3 3.343(19) . -3_546 N
Fe2 Ba3 3.253(7) . 101_445 N
Fe2 Ba3 3.253(7) . 101_545 N
Fe2 O4 1.972(7) . 1_555 N
Fe2 O4 1.972(7) . 2_555 N
Fe2 O5 2.023(8) . -3_546 N
Fe2 O5 2.023(8) . -4_546 N
Fe2 O8 2.010(15) . 1_555 N
Fe2 O9 2.161(18) . 1_555 N
Fe2 Nd2 3.429(23) . -3_545 N
Fe2 Nd2 3.379(24) . -3_546 N
Fe2 Nd2 3.393(10) . 101_445 N
Fe2 Nd2 3.393(10) . 101_545 N
Fe2 Ca2 3.429(23) . -3_545 N
Fe2 Ca2 3.379(24) . -3_546 N
Fe2 Ca2 3.393(10) . 101_445 N
Fe2 Ca2 3.393(10) . 101_545 N
Fe2 Nd3 3.185(20) . -3_545 N
Fe2 Nd3 3.343(19) . -3_546 N
Fe2 Nd3 3.253(7) . 101_445 N
Fe2 Nd3 3.253(7) . 101_545 N
Fe2 Ca3 3.185(20) . -3_545 N
Fe2 Ca3 3.343(19) . -3_546 N
Fe2 Ca3 3.253(7) . 101_445 N
Fe2 Ca3 3.253(7) . 101_545 N
Fe3 Ba3 3.798(21) . -1_565 N
Fe3 Ba3 3.340(22) . -1_566 N
Fe3 Ba3 3.798(21) . -3_545 N
Fe3 Ba3 3.340(22) . -3_546 N
Fe3 Ba3 3.854(13) . 101_445 N
Fe3 Ba3 3.290(15) . 101_545 N
Fe3 Ba3 3.854(13) . 103_465 N
Fe3 Ba3 3.290(15) . 103_565 N
Fe3 Fe3 0.722(29) . 2_555 N
Fe3 Fe3 2.919(26) . -101_445 N
Fe3 O6 2.056(15) . 1_555 N
Fe3 O6 2.498(13) . 2_555 N
Fe3 O7 1.66(5) . 1_555 N
Fe3 O7 2.37(5) . 2_555 N
Fe3 O7 1.80(5) . -101_445 N
Fe3 O7 2.10(5) . -102_345 N
Fe3 O9 1.897(15) . 1_555 N
Fe3 O9 1.897(15) . 3_555 N
Fe3 Nd3 3.340(22) . -1_566 N
Fe3 Nd3 3.340(22) . -3_546 N
Fe3 Nd3 3.290(15) . 101_545 N
Fe3 Nd3 3.290(15) . 103_565 N
Fe3 Ca3 3.340(22) . -1_566 N
Fe3 Ca3 3.340(22) . -3_546 N
Fe3 Ca3 3.290(15) . 101_545 N
Fe3 Ca3 3.290(15) . 103_565 N
O4 Ba2 2.796(18) . -3_545 N
O4 Ba2 2.796(18) . 101_545 N
O4 Ba3 2.533(15) . -3_545 N
O4 Ba3 2.533(15) . 101_545 N
O4 Fe2 1.972(7) . 1_555 N
O4 Fe2 1.972(7) . -103_444 N
O4 Nd2 2.796(18) . -3_545 N
O4 Nd2 2.796(18) . 101_545 N
O4 Ca2 2.796(18) . -3_545 N
O4 Ca2 2.796(18) . 101_545 N
O4 Nd3 2.533(15) . -3_545 N
O4 Nd3 2.533(15) . 101_545 N
O4 Ca3 2.533(15) . -3_545 N
O4 Ca3 2.533(15) . 101_545 N
O5 Ba2 3.027(22) . 1_555 N
O5 Ba2 3.027(22) . -103_444 N
O5 Ba3 2.407(16) . 1_555 N
O5 Ba3 2.407(16) . -103_444 N
O5 Fe2 2.023(8) . -3_556 N
O5 Fe2 2.023(8) . 101_554 N
O5 Nd2 3.027(22) . 1_555 N
O5 Nd2 3.027(22) . -103_444 N
O5 Ca2 3.027(22) . 1_555 N
O5 Ca2 3.027(22) . -103_444 N
O5 Nd3 2.407(16) . 1_555 N
O5 Nd3 2.407(16) . -103_444 N
O5 Ca3 2.407(16) . 1_555 N
O5 Ca3 2.407(16) . -103_444 N
O6 Ba3 2.898(12) . -1_565 N
O6 Ba3 2.898(12) . -3_545 N
O6 Ba3 2.898(12) . 101_545 N
O6 Ba3 2.898(12) . 103_565 N
O6 Fe3 2.056(15) . 1_555 N
O6 Fe3 2.498(13) . 2_555 N
O6 Fe3 2.056(15) . -101_444 N
O6 Fe3 2.498(13) . -102_444 N
O6 O7 2.17(5) . 1_555 N
O6 O7 2.17(5) . -101_444 N
O6 Nd3 2.898(12) . -1_565 N
O6 Nd3 2.898(12) . -3_545 N
O6 Nd3 2.898(12) . 101_545 N
O6 Nd3 2.898(12) . 103_565 N
O6 Ca3 2.898(12) . -1_565 N
O6 Ca3 2.898(12) . -3_545 N
O6 Ca3 2.898(12) . 101_545 N
O6 Ca3 2.898(12) . 103_565 N
O7 Ba3 2.437(19) . 101_545 N
O7 Ba3 2.437(19) . 103_565 N
O7 Fe3 1.66(5) . 1_555 N
O7 Fe3 2.37(5) . 2_555 N
O7 Fe3 1.80(5) . -101_445 N
O7 Fe3 2.10(5) . -102_445 N
O7 O6 2.17(5) . 1_555 N
O7 O7 1.61(9) . 2_655 N
O7 O7 1.86(7) . -101_445 N
O7 Nd3 2.437(19) . 101_545 N
O7 Nd3 2.437(19) . 103_565 N
O7 Ca3 2.437(19) . 101_545 N
O7 Ca3 2.437(19) . 103_565 N
O8 Fe1 1.955(15) . 1_555 N
O8 Ba2 2.943(23) . -3_545 N
O8 Ba2 2.670(23) . -3_546 N
O8 Ba2 2.7936(9) . 101_445 N
O8 Ba2 2.7936(9) . 101_545 N
O8 Fe2 2.010(15) . 1_555 N
O8 Nd2 2.943(23) . -3_545 N
O8 Nd2 2.670(23) . -3_546 N
O8 Nd2 2.7936(9) . 101_445 N
O8 Nd2 2.7936(9) . 101_545 N
O8 Ca2 2.943(23) . -3_545 N
O8 Ca2 2.670(23) . -3_546 N
O8 Ca2 2.7936(9) . 101_445 N
O8 Ca2 2.7936(9) . 101_545 N
O9 Ba3 2.397(28) . -3_545 N
O9 Ba3 3.292(28) . -3_546 N
O9 Ba3 2.845(4) . 101_445 N
O9 Ba3 2.845(4) . 101_545 N
O9 Fe2 2.161(18) . 1_555 N
O9 Fe3 1.897(15) . 1_555 N
O9 Fe3 1.897(15) . 2_555 N
O9 Nd3 2.397(28) . -3_545 N
O9 Nd3 2.845(4) . 101_445 N
O9 Nd3 2.845(4) . 101_545 N
O9 Ca3 2.397(28) . -3_545 N
O9 Ca3 2.845(4) . 101_445 N
O9 Ca3 2.845(4) . 101_545 N
Nd1 Fe1 3.394(9) . 1_554 N
Nd1 Fe1 3.439(10) . 1_555 N
Nd1 Fe1 3.439(10) . -1_555 N
Nd1 Fe1 3.394(9) . -1_556 N
Nd1 Fe1 3.406(4) . 103_454 N
Nd1 Fe1 3.406(4) . 103_554 N
Nd1 Fe1 3.406(4) . -103_344 N
Nd1 Fe1 3.406(4) . -103_444 N
Nd1 O1 2.514(9) . 1_555 N
Nd1 O1 2.514(9) . 2_555 N
Nd1 O1 2.514(9) . -1_555 N
Nd1 O1 2.514(9) . -2_555 N
Nd1 O3 2.493(9) . 1_545 N
Nd1 O3 2.493(9) . 2_545 N
Nd1 O3 2.493(9) . -1_565 N
Nd1 O3 2.493(9) . -2_565 N
Nd1 Ba2 3.983(15) . 3_555 N
Nd1 Ba2 3.983(15) . -3_545 N
Nd1 Nd1 3.95789(9) . 103_454 N
Nd1 Nd1 3.95789(9) . 103_455 N
Nd1 Nd1 3.95789(9) . 103_554 N
Nd1 Nd1 3.95789(9) . 103_555 N
Nd1 Ca1 3.95789(9) . 103_454 N
Nd1 Ca1 3.95789(9) . 103_455 N
Nd1 Ca1 3.95789(9) . 103_554 N
Nd1 Ca1 3.95789(9) . 103_555 N
Nd1 Nd2 3.983(15) . 3_555 N
Nd1 Nd2 3.983(15) . -3_545 N
Nd1 Ca2 3.983(15) . 3_555 N
Nd1 Ca2 3.983(15) . -3_545 N
Ca1 Fe1 3.394(9) . 1_554 N
Ca1 Fe1 3.439(10) . 1_555 N
Ca1 Fe1 3.439(10) . -1_555 N
Ca1 Fe1 3.394(9) . -1_556 N
Ca1 Fe1 3.406(4) . 103_454 N
Ca1 Fe1 3.406(4) . 103_554 N
Ca1 Fe1 3.406(4) . -103_344 N
Ca1 Fe1 3.406(4) . -103_444 N
Ca1 O1 2.514(9) . 1_555 N
Ca1 O1 2.514(9) . 2_555 N
Ca1 O1 2.514(9) . -1_555 N
Ca1 O1 2.514(9) . -2_555 N
Ca1 O3 2.493(9) . 1_545 N
Ca1 O3 2.493(9) . 2_545 N
Ca1 O3 2.493(9) . -1_565 N
Ca1 O3 2.493(9) . -2_565 N
Ca1 Ba2 3.983(15) . 3_555 N
Ca1 Ba2 3.983(15) . -3_545 N
Ca1 Nd1 3.95789(9) . 103_454 N
Ca1 Nd1 3.95789(9) . 103_455 N
Ca1 Nd1 3.95789(9) . 103_554 N
Ca1 Nd1 3.95789(9) . 103_555 N
Ca1 Ca1 3.95789(9) . 103_454 N
Ca1 Ca1 3.95789(9) . 103_455 N
Ca1 Ca1 3.95789(9) . 103_554 N
Ca1 Ca1 3.95789(9) . 103_555 N
Ca1 Nd2 3.983(15) . 3_555 N
Ca1 Nd2 3.983(15) . -3_545 N
Ca1 Ca2 3.983(15) . 3_555 N
Ca1 Ca2 3.983(15) . -3_545 N
Nd2 Fe1 3.409(23) . -3_556 N
Nd2 Fe1 3.453(10) . 101_454 N
Nd2 Fe1 3.453(10) . 101_554 N
Nd2 Ba2 4.02(4) . -103_343 N
Nd2 Ba2 3.901(35) . -103_344 N
Nd2 Ba2 4.02(4) . -103_443 N
Nd2 Ba2 3.901(35) . -103_444 N
Nd2 Ba3 3.598(15) . 1_555 N
Nd2 Fe2 3.429(23) . -3_555 N
Nd2 Fe2 3.379(24) . -3_556 N
Nd2 Fe2 3.393(10) . 101_454 N
Nd2 Fe2 3.393(10) . 101_554 N
Nd2 O4 2.796(18) . -3_555 N
Nd2 O4 2.796(18) . -4_555 N
Nd2 O5 3.027(22) . 1_555 N
Nd2 O5 3.027(22) . 2_555 N
Nd2 O8 2.943(23) . -3_555 N
Nd2 O8 2.670(23) . -3_556 N
Nd2 O8 2.7936(9) . 101_454 N
Nd2 O8 2.7936(9) . 101_554 N
Nd2 Nd1 3.983(15) . 3_555 N
Nd2 Ca1 3.983(15) . 3_555 N
Nd2 Nd2 4.02(4) . -103_343 N
Nd2 Nd2 3.901(35) . -103_344 N
Nd2 Nd2 4.02(4) . -103_443 N
Nd2 Nd2 3.901(35) . -103_444 N
Nd2 Ca2 4.02(4) . -103_343 N
Nd2 Ca2 3.901(35) . -103_344 N
Nd2 Ca2 4.02(4) . -103_443 N
Nd2 Ca2 3.901(35) . -103_444 N
Nd2 Nd3 3.598(15) . 1_555 N
Nd2 Ca3 3.598(15) . 1_555 N
Ca2 Fe1 3.519(23) . -3_555 N
Ca2 Fe1 3.409(23) . -3_556 N
Ca2 Fe1 3.453(10) . 101_454 N
Ca2 Fe1 3.453(10) . 101_554 N
Ca2 O1 3.154(21) . -3_555 N
Ca2 O1 3.154(21) . -4_555 N
Ca2 O3 3.145(21) . 3_565 N
Ca2 O3 3.145(21) . 4_565 N
Ca2 Ba2 4.02(4) . -103_343 N
Ca2 Ba2 3.901(35) . -103_344 N
Ca2 Ba2 4.02(4) . -103_443 N
Ca2 Ba2 3.901(35) . -103_444 N
Ca2 Ba3 3.598(15) . 1_555 N
Ca2 Fe2 3.429(23) . -3_555 N
Ca2 Fe2 3.379(24) . -3_556 N
Ca2 Fe2 3.393(10) . 101_454 N
Ca2 Fe2 3.393(10) . 101_554 N
Ca2 O4 2.796(18) . -3_555 N
Ca2 O4 2.796(18) . -4_555 N
Ca2 O5 3.027(22) . 1_555 N
Ca2 O5 3.027(22) . 2_555 N
Ca2 O8 2.943(23) . -3_555 N
Ca2 O8 2.670(23) . -3_556 N
Ca2 O8 2.7936(9) . 101_454 N
Ca2 O8 2.7936(9) . 101_554 N
Ca2 Nd1 3.983(15) . 3_555 N
Ca2 Ca1 3.983(15) . 3_555 N
Ca2 Nd2 4.02(4) . -103_343 N
Ca2 Nd2 3.901(35) . -103_344 N
Ca2 Nd2 4.02(4) . -103_443 N
Ca2 Nd2 3.901(35) . -103_444 N
Ca2 Ca2 4.02(4) . -103_343 N
Ca2 Ca2 3.901(35) . -103_344 N
Ca2 Ca2 4.02(4) . -103_443 N
Ca2 Ca2 3.901(35) . -103_444 N
Ca2 Nd3 3.598(15) . 1_555 N
Ca2 Ca3 3.598(15) . 1_555 N
Nd3 Ba2 3.598(15) . 1_555 N
Nd3 Ba3 4.338(25) . 3_565 N
Nd3 Ba3 3.844(28) . -103_343 N
Nd3 Ba3 4.075(29) . -103_344 N
Nd3 Ba3 3.844(28) . -103_443 N
Nd3 Ba3 4.075(29) . -103_444 N
Nd3 Fe2 3.185(20) . -3_555 N
Nd3 Fe2 3.343(19) . -3_556 N
Nd3 Fe2 3.253(7) . 101_454 N
Nd3 Fe2 3.253(7) . 101_554 N
Nd3 Fe3 3.340(22) . -1_566 N
Nd3 Fe3 3.340(22) . -2_566 N
Nd3 Fe3 3.290(15) . 101_454 N
Nd3 Fe3 3.290(15) . 102_554 N
Nd3 O4 2.533(15) . -3_555 N
Nd3 O4 2.533(15) . -4_555 N
Nd3 O5 2.407(16) . 1_555 N
Nd3 O5 2.407(16) . 2_555 N
Nd3 O6 2.898(12) . -1_565 N
Nd3 O6 2.898(12) . -2_565 N
Nd3 O7 2.437(19) . 101_454 N
Nd3 O7 2.437(19) . 102_554 N
Nd3 O9 2.397(28) . -3_555 N
Nd3 O9 2.845(4) . 101_454 N
Nd3 O9 2.845(4) . 101_554 N
Nd3 Nd2 3.598(15) . 1_555 N
Nd3 Ca2 3.598(15) . 1_555 N
Nd3 Nd3 3.844(28) . -103_343 N
Nd3 Nd3 3.844(28) . -103_443 N
Nd3 Ca3 3.844(28) . -103_343 N
Nd3 Ca3 4.075(29) . -103_344 N
Nd3 Ca3 3.844(28) . -103_443 N
Nd3 Ca3 4.075(29) . -103_444 N
Ca3 Ba2 3.598(15) . 1_555 N
Ca3 Ba3 4.338(25) . 3_565 N
Ca3 Ba3 3.844(28) . -103_343 N
Ca3 Ba3 4.075(29) . -103_344 N
Ca3 Ba3 3.844(28) . -103_443 N
Ca3 Ba3 4.075(29) . -103_444 N
Ca3 Fe2 3.185(20) . -3_555 N
Ca3 Fe2 3.343(19) . -3_556 N
Ca3 Fe2 3.253(7) . 101_454 N
Ca3 Fe2 3.253(7) . 101_554 N
Ca3 Fe3 3.340(22) . -1_566 N
Ca3 Fe3 3.340(22) . -2_566 N
Ca3 Fe3 3.290(15) . 101_454 N
Ca3 Fe3 3.290(15) . 102_554 N
Ca3 O4 2.533(15) . -3_555 N
Ca3 O4 2.533(15) . -4_555 N
Ca3 O5 2.407(16) . 1_555 N
Ca3 O5 2.407(16) . 2_555 N
Ca3 O6 2.898(12) . -1_565 N
Ca3 O6 2.898(12) . -2_565 N
Ca3 O7 2.437(19) . 101_454 N
Ca3 O7 2.437(19) . 102_554 N
Ca3 O9 2.397(28) . -3_555 N
Ca3 O9 2.845(4) . 101_454 N
Ca3 O9 2.845(4) . 101_554 N
Ca3 Nd2 3.598(15) . 1_555 N
Ca3 Ca2 3.598(15) . 1_555 N
Ca3 Nd3 3.844(28) . -103_343 N
Ca3 Nd3 4.075(29) . -103_344 N
Ca3 Nd3 3.844(28) . -103_443 N
Ca3 Nd3 4.075(29) . -103_444 N
Ca3 Ca3 4.338(25) . 3_565 N
Ca3 Ca3 3.844(28) . -103_343 N
Ca3 Ca3 4.075(29) . -103_344 N
Ca3 Ca3 3.844(28) . -103_443 N
Ca3 Ca3 4.075(29) . -103_444 N
loop_
_pd_meas_intensity_total
_pd_proc_ls_weight
_pd_proc_intensity_bkg_calc
_pd_calc_intensity_total
69.0(30) 0.0 -16867.46 .
62.0(20) 0.0 -16474.63 .
64.0(30) 0.0 -16089.55 .
69.0(30) 0.0 -15712.08 .
62.0(20) 0.0 -15342.10 .
63.0(30) 0.0 -14979.47 .
71.0(30) 0.0 -14624.07 .
63.0(30) 0.0 -14275.78 .
66.0(30) 0.0 -13934.47 .
71.0(30) 0.0 -13600.01 .
67.0(30) 0.0 -13272.30 .
71.0(30) 0.0 -12951.21 .
73.0(30) 0.0 -12636.63 .
80.0(30) 0.0 -12328.44 .
80.0(30) 0.0 -12026.53 .
83.0(30) 0.0 -11730.80 .
80.0(30) 0.0 -11441.12 .
86.0(30) 0.0 -11157.41 .
90.0(30) 0.0 -10879.53 .
95.0(30) 0.0 -10607.40 .
95.0(30) 0.0 -10340.91 .
95.0(30) 0.0 -10079.97 .
92.0(30) 0.0 -9824.46 .
103.0(30) 0.0 -9574.31 .
102.0(30) 0.0 -9329.39 .
108.0(30) 0.0 -9089.63 .
109.0(30) 0.0 -8854.94 .
110.0(30) 0.0 -8625.20 .
110.0(30) 0.0 -8400.35 .
111.0(30) 0.0 -8180.29 .
106.0(30) 0.0 -7964.92 .
106.0(30) 0.0 -7754.17 .
111.0(30) 0.0 -7547.95 .
107.0(30) 0.0 -7346.17 .
101.0(30) 0.0 -7148.77 .
103.0(30) 0.0 -6955.64 .
108.0(30) 0.0 -6766.71 .
96.0(30) 0.0 -6581.92 .
108.0(30) 0.0 -6401.17 .
121.0(30) 0.0 -6224.39 .
158(4) 0.0 -6051.5 .
203(5) 0.0 -5882.5 .
240(5) 0.0 -5717.2 .
283(5) 0.0 -5555.5 .
315(6) 0.0 -5397.5 .
375(6) 0.0 -5243.1 .
426(7) 0.0 -5092.1 .
457(7) 0.0 -4944.5 .
481(7) 0.0 -4800.2 .
516(7) 0.0 -4659.3 .
572(8) 0.0 -4521.5 .
624(8) 0.0 -4386.9 .
681(8) 0.0 -4255.4 .
704(8) 0.0 -4127.0 .
777(9) 0.0 -4001.5 .
804(9) 0.0 -3878.9 .
858(9) 0.0 -3759.1 .
900(9) 0.0 -3642.2 .
894(9) 0.0 -3528.0 .
934(10) 0.0 -3416.5 .
925(10) 0.0 -3307.7 .
946(10) 0.0 -3201.4 .
951(10) 0.0 -3097.6 .
952(10) 0.0 -2996.4 .
944(10) 0.0 -2897.5 .
959(10) 0.0 -2801.1 .
966(10) 0.0 -2707.0 .
971(10) 0.0 -2615.1 .
971(10) 0.0 -2525.5 .
973(10) 0.0 -2438.1 .
971(10) 0.0 -2352.9 .
946(10) 0.0 -2269.8 .
962(10) 0.0 -2188.7 .
928(10) 0.0 -2109.6 .
917(10) 0.0 -2032.5 .
907(10) 0.0 -1957.4 .
902(9) 0.0 -1884.1 .
899(9) 0.0 -1812.7 .
892(9) 0.0 -1743.1 .
886(9) 0.0 -1675.3 .
854(9) 0.0 -1609.2 .
847(9) 0.0 -1544.8 .
832(9) 0.0 -1482.1 .
819(9) 0.0 -1421.1 .
815(9) 0.0 -1361.6 .
800(9) 0.0 -1303.7 .
819(9) 0.0 -1247.3 .
798(9) 0.0 -1192.4 .
773(9) 0.0 -1138.9 .
766(9) 0.0 -1086.9 .
767(9) 0.0 -1036.3 .
744(9) 0.0 -987.0 .
748(9) 0.0 -939.1 .
718(8) 0.0 -892.5 .
711(8) 0.0 -847.2 .
732(9) 0.0 -803.1 .
718(8) 0.0 -760.2 .
717(8) 0.0 -718.6 .
699(8) 0.0 -678.0 .
688(8) 0.0 -638.7 .
690(8) 0.0 -600.4 .
672(8) 0.0 -563.3 .
684(8) 0.0 -527.2 .
670(8) 0.0 -492.1 .
659(8) 0.0 -458.0 .
649(8) 0.0 -425.0 .
658(8) 0.0 -392.9 .
635(8) 0.0 -361.7 .
629(8) 0.0 -331.5 .
630(8) 0.0 -302.1 .
610(8) 0.0 -273.7 .
611(8) 0.0 -246.1 .
609(8) 0.0 -219.3 .
611(8) 0.0 -193.4 .
615(8) 0.0 -168.2 .
606(8) 0.0 -143.8 .
600(8) 0.0 -120.2 .
581(8) 0.0 -97.4 .
599(8) 0.0 -75.2 .
591(8) 0.0 -53.7 .
575(8) 0.0 -33.0 .
597(8) 0.0 -12.9 .
580(8) 0.0 6.6 .
573(8) 0.0 25.4 .
587(8) 0.0 43.6 .
576(8) 0.0 61.2 .
573(8) 0.0 78.2 .
563(8) 0.0 94.6 .
561(7) 0.0 110.5 .
567(8) 0.0 125.9 .
555(7) 0.0 140.7 .
551(7) 0.0 155.0 .
545(7) 0.0 168.7 .
561(7) 0.0 182.1 .
559(7) 0.0 194.9 .
547(7) 0.0 207.3 .
545(7) 0.0 219.2 .
563(8) 0.0 230.7 .
532(7) 0.0 241.7 .
545(7) 0.0 252.4 .
523(7) 0.0 262.6 .
539(7) 0.0 272.5 .
518(7) 0.0 282.0 .
524(7) 0.0 291.1 .
525(7) 0.0 299.8 .
531(7) 0.0 308.2 .
516(7) 0.0 316.3 .
535(7) 0.0 324.0 .
523(7) 0.0 331.5 .
512(7) 0.0 338.6 .
510(7) 0.0 345.4 .
502(7) 0.0 351.9 .
511(7) 0.0 358.1 .
509(7) 0.0 364.1 .
501(7) 0.0 369.8 .
504(7) 0.0 375.3 .
498(7) 0.0 380.4 .
500(7) 0.0 385.4 .
501(7) 0.0 390.1 .
496(7) 0.0 394.6 .
500(7) 0.0 398.9 .
500(7) 0.0 403.0 .
491(7) 0.0 406.8 .
489(7) 0.0 410.5 .
487(7) 0.0 413.9 .
497(7) 0.0 417.2 .
476(7) 0.0 420.3 .
493(7) 0.0 423.3 .
478(7) 0.0 426.0 .
476(7) 0.0 428.6 .
490(7) 0.0 431.1 .
475(7) 0.0 433.4 .
475(7) 0.0 435.5 .
480(7) 0.0 437.5 .
476(7) 0.0 439.4 .
474(7) 0.0 441.1 .
487(7) 0.0 442.7 .
483(7) 0.0 444.2 .
482(7) 0.0 445.6 .
471(7) 0.0 446.9 .
468(7) 0.0 448.1 .
487(7) 0.0 449.1 .
478(7) 0.0 450.1 .
472(7) 0.0 450.9 .
476(7) 0.0 451.7 .
484(7) 0.0 452.4 .
475(7) 0.0 453.0 .
464(7) 0.0 453.5 .
464(7) 0.0 454.0 .
472(7) 0.0 454.3 .
480(7) 0.0 454.6 .
478(7) 0.0 454.9 .
454(7) 0.0 455.0 .
460(7) 0.0 455.2 .
471(7) 0.0 455.2 .
469(7) 0.0 455.2 .
469(7) 0.0 455.1 .
458(7) 0.0 455.0 .
463(7) 0.0 454.9 .
459(7) 0.02041 454.7 454.8
457(7) 0.02041 454.4 454.5
457(7) 0.02041 454.2 454.2
462(7) 0.02041 453.8 453.9
463(7) 0.02041 453.5 453.6
454(7) 0.02041 453.1 453.2
438(7) 0.02041 452.7 452.7
456(7) 0.02041 452.2 452.3
437(7) 0.02041 451.7 451.8
446(7) 0.02041 451.2 451.3
453(7) 0.02041 450.7 450.8
459(7) 0.02041 450.1 450.2
455(7) 0.02041 449.5 449.6
433(7) 0.02041 448.9 449.0
448(7) 0.02041 448.3 448.4
439(7) 0.02041 447.7 447.8
449(7) 0.02041 447.1 447.1
441(7) 0.02041 446.4 446.5
442(7) 0.02041 445.7 445.8
431(7) 0.02041 445.0 445.1
448(7) 0.02041 444.3 444.4
439(7) 0.02041 443.6 443.7
459(7) 0.02041 442.9 443.0
447(7) 0.02041 442.2 442.3
444(7) 0.02041 441.5 441.6
436(7) 0.02041 440.7 440.9
444(7) 0.02041 440.0 440.1
429(7) 0.02041 439.3 439.4
429(7) 0.02041 438.5 438.7
430(7) 0.02041 437.8 437.9
426(7) 0.02041 437.0 437.2
440(7) 0.02041 436.3 436.4
445(7) 0.02041 435.6 435.7
454(7) 0.02041 434.8 435.0
439(7) 0.02041 434.1 434.2
445(7) 0.02041 433.4 433.5
447(7) 0.02041 432.6 432.8
437(7) 0.02041 431.9 432.1
427(7) 0.02041 431.2 431.4
431(7) 0.02041 430.5 430.7
434(7) 0.02041 429.7 430.0
428(7) 0.02041 429.0 429.3
429(7) 0.02041 428.3 428.6
419(6) 0.02778 427.6 427.9
436(7) 0.02041 427.0 427.2
429(7) 0.02041 426.3 426.6
432(7) 0.02041 425.6 425.9
425(7) 0.02041 424.9 425.3
424(7) 0.02041 424.3 424.7
422(6) 0.02778 423.6 424.0
416(6) 0.02778 423.0 423.4
420(6) 0.02778 422.4 422.8
413(6) 0.02778 421.8 422.3
409(6) 0.02778 421.1 421.7
422(6) 0.02778 420.5 421.1
419(6) 0.02778 420.0 420.6
428(7) 0.02041 419.4 420.1
414(6) 0.02778 418.8 419.6
405(6) 0.02778 418.2 419.2
411(6) 0.02778 417.7 418.8
423(7) 0.02041 417.1 418.5
436(7) 0.02041 416.6 418.3
430(7) 0.02041 416.1 418.4
418(6) 0.02778 415.6 418.8
428(7) 0.02041 415.1 419.5
434(7) 0.02041 414.6 420.9
427(7) 0.02041 414.1 423.0
433(7) 0.02041 413.6 425.8
443(7) 0.02041 413.1 429.6
429(7) 0.02041 412.7 434.1
435(7) 0.02041 412.2 439.2
456(7) 0.02041 411.8 444.8
461(7) 0.02041 411.4 450.4
469(7) 0.02041 411.0 455.3
471(7) 0.02041 410.6 459.0
482(7) 0.02041 410.2 460.9
467(7) 0.02041 409.8 460.8
471(7) 0.02041 409.4 458.3
452(7) 0.02041 409.0 453.4
459(7) 0.02041 408.7 446.6
457(7) 0.02041 408.3 438.8
445(7) 0.02041 408.0 431.2
434(7) 0.02041 407.6 424.4
413(6) 0.02778 407.3 418.9
413(6) 0.02778 407.0 414.8
418(6) 0.02778 406.7 411.8
401(6) 0.02778 406.3 409.8
399(6) 0.02778 406.0 408.5
399(6) 0.02778 405.8 407.6
392(6) 0.02778 405.5 406.9
390(6) 0.02778 405.2 406.4
417(6) 0.02778 404.9 406.0
393(6) 0.02778 404.7 405.6
381(6) 0.02778 404.4 405.2
387(6) 0.02778 404.2 404.9
399(6) 0.02778 403.9 404.6
404(6) 0.02778 403.7 404.3
395(6) 0.02778 403.4 404.0
390(6) 0.02778 403.2 403.7
400(6) 0.02778 403.0 403.5
407(6) 0.02778 402.8 403.2
395(6) 0.02778 402.6 403.0
396(6) 0.02778 402.3 402.8
397(6) 0.02778 402.1 402.6
384(6) 0.02778 401.9 402.3
383(6) 0.02778 401.7 402.1
401(6) 0.02778 401.6 401.9
394(6) 0.02778 401.4 401.7
390(6) 0.02778 401.2 401.6
400(6) 0.02778 401.0 401.4
400(6) 0.02778 400.8 401.2
393(6) 0.02778 400.6 401.1
406(6) 0.02778 400.5 401.0
392(6) 0.02778 400.3 400.9
407(6) 0.02778 400.1 400.9
403(6) 0.02778 400.0 401.0
402(6) 0.02778 399.8 401.2
406(6) 0.02778 399.6 401.5
396(6) 0.02778 399.5 401.9
406(6) 0.02778 399.3 402.3
412(6) 0.02778 399.2 402.9
413(6) 0.02778 399.0 403.4
430(7) 0.02041 398.9 403.8
431(7) 0.02041 398.7 404.1
432(7) 0.02041 398.6 404.1
411(6) 0.02778 398.4 403.9
425(7) 0.02041 398.3 403.3
423(7) 0.02041 398.1 402.5
426(7) 0.02041 397.9 401.6
397(6) 0.02778 397.8 400.7
408(6) 0.02778 397.6 399.8
405(6) 0.02778 397.5 399.0
401(6) 0.02778 397.3 398.5
399(6) 0.02778 397.2 398.0
384(6) 0.02778 397.0 397.7
400(6) 0.02778 396.9 397.4
388(6) 0.02778 396.7 397.2
385(6) 0.02778 396.6 397.1
381(6) 0.02778 396.4 397.0
387(6) 0.02778 396.2 396.9
396(6) 0.02778 396.1 396.9
383(6) 0.02778 395.9 397.0
399(6) 0.02778 395.7 397.2
393(6) 0.02778 395.6 397.5
402(6) 0.02778 395.4 397.9
413(6) 0.02778 395.2 398.4
412(6) 0.02778 395.0 399.0
402(6) 0.02778 394.9 399.6
400(6) 0.02778 394.7 400.3
408(6) 0.02778 394.5 400.9
396(7) 0.02041 394.3 401.2
391(6) 0.02778 394.1 401.0
400(6) 0.02778 393.9 400.4
395(6) 0.02778 393.7 399.3
402(6) 0.02778 393.6 398.1
376(6) 0.02778 393.4 396.9
384(6) 0.02778 393.1 395.7
379(6) 0.02778 392.9 394.8
391(6) 0.02778 392.7 394.1
395(6) 0.02778 392.5 393.6
401(6) 0.02778 392.3 393.2
390(6) 0.02778 392.1 393.0
399(6) 0.02778 391.9 392.9
392(6) 0.02778 391.6 392.9
402(6) 0.02778 391.4 393.2
394(6) 0.02778 391.2 393.4
407(6) 0.02778 390.9 393.6
408(6) 0.02778 390.7 393.9
427(7) 0.02041 390.4 394.2
425(7) 0.02041 390.2 394.5
425(7) 0.02041 389.9 394.7
410(6) 0.02778 389.7 394.8
411(6) 0.02778 389.4 394.4
406(6) 0.02778 389.2 393.7
409(6) 0.02778 388.9 392.8
410(6) 0.02778 388.6 391.9
406(6) 0.02778 388.4 390.9
386(6) 0.02778 388.1 390.1
387(6) 0.02778 387.8 389.4
379(6) 0.02778 387.5 388.9
372(6) 0.02778 387.2 388.4
398(6) 0.02778 386.9 388.1
391(6) 0.02778 386.6 387.8
388(6) 0.02778 386.3 387.5
398(6) 0.02778 386.0 387.3
396(6) 0.02778 385.7 387.2
397(6) 0.02778 385.4 387.2
385(6) 0.02778 385.1 387.4
387(6) 0.02778 384.7 387.9
397(6) 0.02778 384.4 388.7
379(6) 0.02778 384.1 389.8
384(6) 0.02778 383.8 391.5
388(6) 0.02778 383.4 393.6
393(6) 0.02778 383.1 396.2
391(6) 0.02778 382.7 399.0
401(6) 0.02778 382.4 401.9
409(6) 0.02778 382.0 404.6
396(6) 0.02778 381.7 406.4
398(6) 0.02778 381.3 406.6
394(6) 0.02778 381.0 405.1
387(6) 0.02778 380.6 401.9
380(6) 0.02778 380.2 397.9
396(6) 0.02778 379.9 393.6
388(6) 0.02778 379.5 389.6
372(6) 0.02778 379.1 386.4
374(6) 0.02778 378.7 383.9
372(6) 0.02778 378.3 382.0
368(6) 0.02778 378.0 380.8
367(6) 0.02778 377.6 379.9
370(6) 0.02778 377.2 379.2
390(6) 0.02778 376.8 378.6
374(6) 0.02778 376.4 378.2
367(6) 0.02778 376.0 377.7
381(6) 0.02778 375.6 377.3
368(6) 0.02778 375.2 376.9
375(6) 0.02778 374.8 376.5
363(6) 0.02778 374.3 376.1
369(6) 0.02778 373.9 375.7
364(6) 0.02778 373.5 375.4
366(6) 0.02778 373.1 375.0
374(6) 0.02778 372.7 374.6
368(6) 0.02778 372.3 374.3
374(6) 0.02778 371.8 373.9
373(6) 0.02778 371.4 373.6
368(6) 0.02778 371.0 373.3
364(6) 0.02778 370.5 372.9
367(6) 0.02778 370.1 372.6
356(6) 0.02778 369.7 372.3
361(6) 0.02778 369.2 372.0
359(6) 0.02778 368.8 371.7
372(6) 0.02778 368.4 371.5
363(6) 0.02778 367.9 371.2
358(6) 0.02778 367.5 371.0
362(6) 0.02778 367.0 370.8
361(6) 0.02778 366.6 370.6
361(6) 0.02778 366.1 370.5
371(6) 0.02778 365.7 370.3
367(6) 0.02778 365.2 370.3
375(6) 0.02778 364.8 370.3
358(6) 0.02778 364.3 370.3
364(6) 0.02778 363.9 370.4
368(6) 0.02778 363.4 370.6
371(6) 0.02778 363.0 370.9
371(6) 0.02778 362.5 371.4
365(6) 0.02778 362.1 372.1
376(6) 0.02778 361.6 373.1
389(6) 0.02778 361.2 374.8
383(6) 0.02778 360.7 377.5
380(6) 0.02778 360.3 381.9
387(6) 0.02778 359.8 389.2
393(6) 0.02778 359.4 400.6
399(6) 0.02778 358.9 418.0
420(6) 0.02778 358.5 443.3
464(7) 0.02041 358.0 478.2
519(7) 0.02041 357.6 523.7
576(8) 0.01563 357.1 579.0
654(8) 0.01563 356.7 641.2
725(9) 0.01235 356.2 706.1
770(9) 0.01235 355.8 767.2
817(9) 0.01235 355.3 815.7
839(9) 0.01235 354.9 843.0
834(9) 0.01235 354.4 846.3
826(9) 0.01235 354.0 832.0
811(9) 0.01235 353.5 810.0
763(9) 0.01235 353.1 788.2
743(9) 0.01235 352.7 769.4
727(9) 0.01235 352.2 750.0
697(8) 0.01563 351.8 722.6
673(8) 0.01563 351.3 681.8
620(8) 0.01563 350.9 629.4
581(8) 0.01563 350.5 571.8
541(7) 0.02041 350.0 516.4
475(7) 0.02041 349.6 468.7
450(7) 0.02041 349.2 431.2
419(6) 0.02778 348.8 404.1
408(6) 0.02778 348.3 385.9
402(6) 0.02778 347.9 374.4
394(6) 0.02778 347.5 367.2
377(6) 0.02778 347.1 362.7
372(6) 0.02778 346.7 359.7
374(6) 0.02778 346.2 357.6
373(6) 0.02778 345.8 356.0
374(6) 0.02778 345.4 354.6
373(6) 0.02778 345.0 353.5
369(6) 0.02778 344.6 352.5
357(6) 0.02778 344.2 351.8
349(6) 0.02778 343.8 351.3
355(6) 0.02778 343.4 351.2
360(6) 0.02778 343.0 351.6
355(6) 0.02778 342.6 352.7
346(6) 0.02778 342.3 354.7
353(6) 0.02778 341.9 357.7
367(6) 0.02778 341.5 361.7
361(6) 0.02778 341.1 366.6
364(6) 0.02778 340.7 371.7
370(6) 0.02778 340.4 376.6
380(6) 0.02778 340.0 380.1
382(6) 0.02778 339.6 381.3
383(6) 0.02778 339.3 379.5
381(6) 0.02778 338.9 374.9
375(6) 0.02778 338.6 368.4
378(6) 0.02778 338.2 361.5
364(6) 0.02778 337.9 355.1
349(6) 0.02778 337.5 349.8
339(6) 0.02778 337.2 345.8
342(6) 0.02778 336.9 343.0
349(6) 0.02778 336.5 341.1
338(6) 0.02778 336.2 339.8
353(6) 0.02778 335.9 338.9
349(6) 0.02778 335.5 338.2
345(6) 0.02778 335.2 337.6
347(6) 0.02778 334.9 337.2
346(6) 0.02778 334.6 336.7
347(6) 0.02778 334.3 336.3
352(6) 0.02778 334.0 335.9
351(6) 0.02778 333.7 335.5
350(6) 0.02778 333.4 335.2
343(6) 0.02778 333.1 334.8
354(6) 0.02778 332.8 334.5
344(6) 0.02778 332.6 334.2
353(6) 0.02778 332.3 333.9
340(6) 0.02778 332.0 333.6
336(6) 0.02778 331.7 333.4
326(6) 0.02778 331.5 333.2
337(6) 0.02778 331.2 333.1
339(6) 0.02778 331.0 333.1
329(6) 0.02778 330.7 333.1
340(6) 0.02778 330.5 333.4
346(6) 0.02778 330.2 333.8
348(6) 0.02778 330.0 334.3
347(6) 0.02778 329.8 335.0
345(6) 0.02778 329.5 335.9
349(6) 0.02778 329.3 336.9
352(6) 0.02778 329.1 338.2
349(6) 0.02778 328.9 339.8
351(6) 0.02778 328.7 341.9
364(6) 0.02778 328.5 344.6
358(6) 0.02778 328.3 347.8
354(6) 0.02778 328.1 351.2
346(6) 0.02778 327.9 354.0
357(6) 0.02778 327.7 355.7
368(6) 0.02778 327.5 355.5
366(6) 0.02778 327.3 353.1
349(6) 0.02778 327.1 349.1
350(6) 0.02778 327.0 344.4
346(6) 0.02778 326.8 339.8
334(6) 0.02778 326.6 335.8
330(6) 0.02778 326.5 332.8
336(6) 0.02778 326.3 330.6
332(6) 0.02778 326.2 329.1
340(6) 0.02778 326.0 328.2
324(6) 0.02778 325.9 327.6
323(6) 0.02778 325.8 327.1
326(6) 0.02778 325.6 326.8
324(6) 0.02778 325.5 326.6
326(6) 0.02778 325.4 326.2
325(6) 0.02778 325.3 326.0
330(6) 0.02778 325.1 325.9
327(6) 0.02778 325.0 325.7
329(6) 0.02778 324.9 325.6
326(5) 0.0400 324.8 325.5
332(6) 0.02778 324.7 325.4
312(5) 0.0400 324.6 325.1
335(6) 0.02778 324.6 325.1
324(6) 0.02778 324.5 325.0
328(6) 0.02778 324.4 325.0
324(5) 0.0400 324.3 324.9
323(6) 0.02778 324.3 325.3
325(5) 0.0400 324.2 325.2
332(6) 0.02778 324.1 325.2
328(5) 0.0400 324.1 325.1
334(6) 0.02778 324.0 325.1
324(6) 0.02778 324.0 325.1
333(6) 0.02778 323.9 325.0
327(6) 0.02778 323.9 325.0
328(6) 0.02778 323.8 325.0
323(6) 0.02778 323.8 325.0
320(6) 0.02778 323.8 325.1
329(6) 0.02778 323.7 325.1
325(6) 0.02778 323.7 325.1
329(6) 0.02778 323.7 325.2
323(6) 0.02778 323.7 325.2
312(6) 0.02778 323.7 325.3
323(6) 0.02778 323.7 325.4
317(6) 0.02778 323.7 325.6
332(6) 0.02778 323.7 325.8
325(6) 0.02778 323.7 326.2
324(6) 0.02778 323.7 326.8
313(6) 0.02778 323.7 327.8
324(6) 0.02778 323.7 329.3
325(6) 0.02778 323.7 331.6
330(6) 0.02778 323.7 334.8
318(6) 0.02778 323.8 338.9
324(6) 0.02778 323.8 343.7
331(6) 0.02778 323.8 348.5
333(6) 0.02778 323.8 352.7
331(6) 0.02778 323.9 355.4
339(6) 0.02778 323.9 355.8
322(6) 0.02778 324.0 353.6
334(6) 0.02778 324.0 349.5
320(6) 0.02778 324.1 344.5
320(6) 0.02778 324.1 339.9
324(6) 0.02778 324.2 336.0
321(5) 0.0400 324.2 333.3
318(6) 0.02778 324.3 331.9
308(5) 0.0400 324.3 331.6
313(6) 0.02778 324.4 332.4
325(6) 0.02778 324.5 334.1
334(6) 0.02778 324.6 336.5
344(6) 0.02778 324.6 339.2
332(6) 0.02778 324.7 342.0
321(6) 0.02778 324.8 344.2
330(5) 0.0400 324.9 345.3
335(6) 0.02778 324.9 344.9
345(6) 0.02778 325.0 343.2
331(6) 0.02778 325.1 340.6
326(5) 0.0400 325.2 337.8
325(6) 0.02778 325.3 335.3
323(5) 0.0400 325.4 333.3
315(6) 0.02778 325.5 331.9
311(5) 0.0400 325.6 331.1
341(6) 0.02778 325.7 330.8
333(6) 0.02778 325.8 330.7
321(6) 0.02778 325.9 330.8
339(6) 0.02778 326.0 331.0
341(6) 0.02778 326.1 331.2
340(6) 0.02778 326.2 331.5
339(6) 0.02778 326.3 331.9
332(6) 0.02778 326.5 332.3
315(6) 0.02778 326.6 332.7
312(6) 0.02778 326.7 333.2
318(6) 0.02778 326.8 333.7
308(6) 0.02778 326.9 334.2
318(6) 0.02778 327.0 334.8
310(6) 0.02778 327.2 335.5
313(6) 0.02778 327.3 336.3
314(6) 0.02778 327.4 337.1
304(6) 0.02778 327.5 338.0
311(6) 0.02778 327.7 339.0
308(6) 0.02778 327.8 340.2
308(6) 0.02778 327.9 341.6
311(6) 0.02778 328.1 343.2
322(6) 0.02778 328.2 345.0
320(6) 0.02778 328.3 347.3
319(6) 0.02778 328.4 350.1
322(6) 0.02778 328.6 354.0
327(6) 0.02778 328.7 359.7
329(6) 0.02778 328.8 368.1
356(6) 0.02778 329.0 380.9
370(6) 0.02778 329.1 400.2
408(6) 0.02778 329.2 428.5
453(7) 0.02041 329.4 468.5
515(7) 0.02041 329.5 522.4
582(8) 0.01563 329.7 591.8
664(8) 0.01563 329.8 677.8
774(9) 0.01235 329.9 780.9
888(9) 0.01235 330.1 899.9
994(10) 0.01000 330.2 1033.5
1150(11) 0.00826 330.3 1177.7
1305(11) 0.00826 330.5 1321.6
1389(11) 0.00826 330.6 1444.9
1462(13) 0.00592 330.7 1524.0
1490(12) 0.00694 330.9 1535.7
1425(12) 0.00694 331.0 1464.7
1313(11) 0.00826 331.2 1318.5
1135(11) 0.00826 331.3 1128.9
945(9) 0.01235 331.4 933.1
771(9) 0.01235 331.6 758.9
657(8) 0.01563 331.7 620.6
529(8) 0.01563 331.8 521.0
475(7) 0.02041 332.0 455.1
454(7) 0.02041 332.1 414.5
456(7) 0.02041 332.2 390.6
426(7) 0.02041 332.4 376.8
422(6) 0.02778 332.5 368.6
427(7) 0.02041 332.6 363.6
412(6) 0.02778 332.7 360.5
408(6) 0.02778 332.9 358.6
396(6) 0.02778 333.0 357.8
382(6) 0.02778 333.1 358.0
369(6) 0.02778 333.2 359.1
362(6) 0.02778 333.4 360.6
387(6) 0.02778 333.5 362.5
387(6) 0.02778 333.6 364.0
407(6) 0.02778 333.7 364.9
442(7) 0.02041 333.8 364.8
457(7) 0.02041 334.0 363.8
473(7) 0.02041 334.1 362.1
479(7) 0.02041 334.2 360.4
467(7) 0.02041 334.3 359.5
456(7) 0.02041 334.4 360.2
440(7) 0.02041 334.5 363.3
418(6) 0.02778 334.6 369.2
392(6) 0.02778 334.7 377.4
389(6) 0.02778 334.8 387.0
385(6) 0.02778 334.9 396.2
386(6) 0.02778 335.1 402.7
392(6) 0.02778 335.2 404.6
378(6) 0.02778 335.2 400.7
370(6) 0.02778 335.3 392.3
361(6) 0.02778 335.4 381.6
349(6) 0.02778 335.5 371.0
344(6) 0.02778 335.6 362.0
324(6) 0.02778 335.7 355.3
323(6) 0.02778 335.8 350.8
350(6) 0.02778 335.9 348.4
349(6) 0.02778 336.0 347.5
355(6) 0.02778 336.0 348.1
364(6) 0.02778 336.1 350.1
371(6) 0.02778 336.2 354.1
386(6) 0.02778 336.3 360.8
403(6) 0.02778 336.3 371.1
408(6) 0.02778 336.4 385.4
429(7) 0.02041 336.5 403.8
433(7) 0.02041 336.5 425.0
454(7) 0.02041 336.6 446.6
471(7) 0.02041 336.7 465.3
479(7) 0.02041 336.7 477.1
489(7) 0.02041 336.8 479.8
485(7) 0.02041 336.8 473.2
473(7) 0.02041 336.9 458.6
455(7) 0.02041 336.9 438.4
421(6) 0.02778 337.0 416.3
388(6) 0.02778 337.0 395.7
355(6) 0.02778 337.0 378.6
354(6) 0.02778 337.1 366.0
347(6) 0.02778 337.1 357.5
338(6) 0.02778 337.2 352.4
319(5) 0.0400 337.2 350.1
325(6) 0.02778 337.2 349.9
331(6) 0.02778 337.2 351.5
331(6) 0.02778 337.2 354.4
340(6) 0.02778 337.3 358.4
363(6) 0.02778 337.3 362.8
372(6) 0.02778 337.3 366.7
362(6) 0.02778 337.3 369.2
370(6) 0.02778 337.3 369.2
369(6) 0.02778 337.3 366.8
362(6) 0.02778 337.3 362.5
345(6) 0.02778 337.3 357.6
332(6) 0.02778 337.3 352.9
325(6) 0.02778 337.3 349.1
308(6) 0.02778 337.3 346.3
322(6) 0.02778 337.3 344.6
323(6) 0.02778 337.3 343.7
321(6) 0.02778 337.2 343.4
322(6) 0.02778 337.2 343.7
316(6) 0.02778 337.2 344.5
321(6) 0.02778 337.2 345.8
330(6) 0.02778 337.1 347.8
340(6) 0.02778 337.1 350.5
338(6) 0.02778 337.1 354.2
347(6) 0.02778 337.0 359.5
359(6) 0.02778 337.0 366.8
372(6) 0.02778 336.9 376.4
410(6) 0.02778 336.9 388.6
419(6) 0.02778 336.8 402.6
421(6) 0.02778 336.8 416.4
442(7) 0.02041 336.7 426.7
438(7) 0.02041 336.6 431.2
437(7) 0.02041 336.6 427.5
425(7) 0.02041 336.5 416.3
424(7) 0.02041 336.4 401.0
423(7) 0.02041 336.4 384.9
415(6) 0.02778 336.3 370.7
432(7) 0.02041 336.2 359.6
430(7) 0.02041 336.1 351.7
438(7) 0.02041 336.0 346.7
422(6) 0.02778 335.9 343.7
405(6) 0.02778 335.9 342.0
392(6) 0.02778 335.8 341.2
356(6) 0.02778 335.7 340.8
353(6) 0.02778 335.6 340.9
337(6) 0.02778 335.4 341.1
334(6) 0.02778 335.3 341.4
325(6) 0.02778 335.2 341.8
314(6) 0.02778 335.1 342.1
318(6) 0.02778 335.0 342.4
314(5) 0.0400 334.9 343.0
319(6) 0.02778 334.8 344.1
326(6) 0.02778 334.6 346.1
330(6) 0.02778 334.5 349.1
342(6) 0.02778 334.4 353.0
365(6) 0.02778 334.2 357.4
385(6) 0.02778 334.1 361.3
418(6) 0.02778 333.9 363.6
434(7) 0.02041 333.8 363.6
444(7) 0.02041 333.7 361.0
471(7) 0.02041 333.5 356.7
449(7) 0.02041 333.3 351.8
420(6) 0.02778 333.2 347.2
388(6) 0.02778 333.0 343.5
360(6) 0.02778 332.9 340.9
343(6) 0.02778 332.7 339.2
332(6) 0.02778 332.5 338.2
312(6) 0.02778 332.4 337.7
319(6) 0.02778 332.2 337.5
318(6) 0.02778 332.0 337.6
307(5) 0.0400 331.8 337.7
308(6) 0.02778 331.6 338.0
305(6) 0.02778 331.5 338.4
316(6) 0.02778 331.3 339.0
308(6) 0.02778 331.1 339.8
308(6) 0.02778 330.9 340.9
310(6) 0.02778 330.7 342.8
308(6) 0.02778 330.5 345.7
316(6) 0.02778 330.3 350.6
321(6) 0.02778 330.1 358.9
339(6) 0.02778 329.9 372.6
353(6) 0.02778 329.7 394.2
389(6) 0.02778 329.5 426.1
452(7) 0.02041 329.2 469.4
501(7) 0.02041 329.0 523.4
571(8) 0.01563 328.8 583.6
645(8) 0.01563 328.6 642.1
693(8) 0.01563 328.4 688.3
719(8) 0.01563 328.1 712.4
732(9) 0.01235 327.9 709.3
688(8) 0.01563 327.7 679.2
642(8) 0.01563 327.4 627.5
615(8) 0.01563 327.2 564.6
543(7) 0.02041 327.0 502.3
521(7) 0.02041 326.7 448.8
509(7) 0.02041 326.5 407.7
486(7) 0.02041 326.2 378.9
466(7) 0.02041 326.0 360.2
442(7) 0.02041 325.7 348.9
418(6) 0.02778 325.5 342.2
377(6) 0.02778 325.2 338.1
350(6) 0.02778 325.0 335.5
336(6) 0.02778 324.7 333.7
328(6) 0.02778 324.4 332.3
314(6) 0.02778 324.2 331.1
309(6) 0.02778 323.9 330.1
307(6) 0.02778 323.7 329.2
304(6) 0.02778 323.4 328.5
304(6) 0.02778 323.1 327.8
304(6) 0.02778 322.8 327.1
306(5) 0.0400 322.6 326.6
295(6) 0.02778 322.3 326.0
305(6) 0.02778 322.0 325.5
305(6) 0.02778 321.7 325.0
307(6) 0.02778 321.4 324.6
300(5) 0.0400 321.2 324.2
303(6) 0.02778 320.9 323.8
294(5) 0.0400 320.6 323.5
300(5) 0.0400 320.3 323.2
291(5) 0.0400 320.0 322.9
299(5) 0.0400 319.7 322.7
303(6) 0.02778 319.4 322.7
305(6) 0.02778 319.1 323.5
289(5) 0.0400 318.8 324.2
296(5) 0.0400 318.5 325.4
294(5) 0.0400 318.2 327.7
292(5) 0.0400 317.9 331.1
307(6) 0.02778 317.6 335.7
305(6) 0.02778 317.3 341.3
301(5) 0.0400 317.0 347.1
322(6) 0.02778 316.7 351.8
320(6) 0.02778 316.4 354.2
341(6) 0.02778 316.1 353.2
337(6) 0.02778 315.8 349.1
340(6) 0.02778 315.5 343.0
322(6) 0.02778 315.2 336.3
326(6) 0.02778 314.8 330.3
332(6) 0.02778 314.5 325.7
325(6) 0.02778 314.2 322.2
344(6) 0.02778 313.9 319.9
330(6) 0.02778 313.6 318.5
318(6) 0.02778 313.3 317.6
311(6) 0.02778 312.9 317.0
308(6) 0.02778 312.6 316.7
306(6) 0.02778 312.3 316.5
295(5) 0.0400 312.0 316.5
309(6) 0.02778 311.7 316.7
310(6) 0.02778 311.3 316.9
311(6) 0.02778 311.0 317.0
319(6) 0.02778 310.7 317.1
320(6) 0.02778 310.4 316.8
325(6) 0.02778 310.0 316.4
318(6) 0.02778 309.7 315.7
315(6) 0.02778 309.4 315.0
314(6) 0.02778 309.1 314.4
321(6) 0.02778 308.7 313.9
326(6) 0.02778 308.4 313.6
322(6) 0.02778 308.1 313.4
336(6) 0.02778 307.8 313.4
353(6) 0.02778 307.4 313.5
376(6) 0.02778 307.1 313.9
398(6) 0.02778 306.8 314.6
421(6) 0.02778 306.4 316.1
414(6) 0.02778 306.1 319.0
418(6) 0.02778 305.8 324.1
422(6) 0.02778 305.5 332.7
430(7) 0.02041 305.1 345.7
429(7) 0.02041 304.8 363.5
445(7) 0.02041 304.5 385.0
439(7) 0.02041 304.1 407.0
464(7) 0.02041 303.8 424.9
452(7) 0.02041 303.5 433.1
460(7) 0.02041 303.1 428.4
429(7) 0.02041 302.8 412.3
395(6) 0.02778 302.5 390.2
391(6) 0.02778 302.2 367.7
373(6) 0.02778 301.8 348.5
348(6) 0.02778 301.5 334.3
344(6) 0.02778 301.2 325.2
328(6) 0.02778 300.9 320.4
324(6) 0.02778 300.5 318.9
322(6) 0.02778 300.2 319.6
318(6) 0.02778 299.9 321.6
306(6) 0.02778 299.5 324.2
326(5) 0.0400 299.2 326.5
323(6) 0.02778 298.9 327.5
305(6) 0.02778 298.6 327.0
309(6) 0.02778 298.3 324.9
309(6) 0.02778 297.9 321.8
309(6) 0.02778 297.6 318.5
307(5) 0.0400 297.3 315.5
278(6) 0.02778 297.0 313.2
300(5) 0.0400 296.7 311.8
301(5) 0.0400 296.3 311.0
295(5) 0.0400 296.0 310.9
284(5) 0.0400 295.7 311.1
285(5) 0.0400 295.4 311.7
287(5) 0.0400 295.1 312.5
277(5) 0.0400 294.8 313.6
284(5) 0.0400 294.4 315.0
277(5) 0.0400 294.1 316.6
285(5) 0.0400 293.8 318.7
294(5) 0.0400 293.5 321.1
299(5) 0.0400 293.2 324.2
294(5) 0.0400 292.9 328.0
312(6) 0.02778 292.6 332.8
316(6) 0.02778 292.3 339.4
330(6) 0.02778 292.0 349.1
365(6) 0.02778 291.7 364.9
398(6) 0.02778 291.4 392.3
460(7) 0.02041 291.1 440.8
545(8) 0.01563 290.8 524.2
689(8) 0.01563 290.5 658.1
932(10) 0.01000 290.2 854.8
1231(11) 0.00826 289.9 1113.6
1496(12) 0.00694 289.6 1411.7
1758(14) 0.00510 289.3 1698.8
1922(14) 0.00510 289.0 1903.1
1954(14) 0.00510 288.7 1956.2
1793(13) 0.00592 288.4 1836.2
1487(12) 0.00694 288.2 1590.5
1269(11) 0.00826 287.9 1297.7
947(10) 0.01000 287.6 1022.1
735(9) 0.01235 287.3 799.5
590(8) 0.01563 287.0 641.3
516(7) 0.02041 286.7 544.2
481(7) 0.02041 286.5 499.6
482(7) 0.02041 286.2 499.3
526(7) 0.02041 285.9 537.6
610(8) 0.01563 285.7 608.9
716(8) 0.01563 285.4 703.2
823(9) 0.01235 285.1 802.8
916(10) 0.01000 284.9 881.7
905(10) 0.01000 284.6 913.1
859(9) 0.01235 284.3 883.3
758(9) 0.01235 284.1 804.0
657(8) 0.01563 283.8 702.3
541(7) 0.02041 283.6 602.4
463(7) 0.02041 283.3 518.0
403(6) 0.02778 283.0 453.2
365(6) 0.02778 282.8 406.6
353(6) 0.02778 282.5 375.0
340(6) 0.02778 282.3 354.6
339(6) 0.02778 282.1 342.0
336(6) 0.02778 281.8 334.7
342(6) 0.02778 281.6 330.3
329(6) 0.02778 281.3 327.1
329(6) 0.02778 281.1 323.4
331(6) 0.02778 280.9 318.9
308(6) 0.02778 280.6 313.7
303(6) 0.02778 280.4 308.6
302(5) 0.0400 280.2 304.1
284(5) 0.0400 280.0 300.7
285(5) 0.0400 279.7 298.6
296(5) 0.0400 279.5 297.8
289(5) 0.0400 279.3 298.5
299(5) 0.0400 279.1 301.0
317(5) 0.0400 278.9 305.8
316(6) 0.02778 278.7 313.0
335(6) 0.02778 278.4 323.1
358(6) 0.02778 278.2 335.6
373(6) 0.02778 278.0 349.2
382(7) 0.02041 277.8 361.5
387(6) 0.02778 277.6 369.4
391(6) 0.02778 277.4 369.5
380(6) 0.02778 277.2 361.1
349(6) 0.02778 277.0 346.7
326(5) 0.0400 276.8 330.5
304(6) 0.02778 276.7 315.7
299(5) 0.0400 276.5 303.9
276(5) 0.0400 276.3 295.7
285(5) 0.0400 276.1 290.5
270(5) 0.0400 275.9 287.6
272(5) 0.0400 275.7 286.2
274(5) 0.0400 275.6 285.7
266(5) 0.0400 275.4 285.8
265(5) 0.0400 275.2 286.1
255(5) 0.0400 275.1 286.4
264(5) 0.0400 274.9 286.3
269(5) 0.0400 274.7 285.8
272(5) 0.0400 274.6 284.9
271(5) 0.0400 274.4 283.8
267(5) 0.0400 274.3 282.9
264(5) 0.0400 274.1 282.3
262(5) 0.0400 274.0 282.0
264(5) 0.0400 273.8 282.2
268(5) 0.0400 273.7 282.9
266(5) 0.0400 273.5 284.4
272(5) 0.0400 273.4 287.3
278(5) 0.0400 273.2 292.1
294(5) 0.0400 273.1 299.8
312(6) 0.02778 273.0 311.0
328(6) 0.02778 272.8 325.6
341(6) 0.02778 272.7 342.5
374(6) 0.02778 272.6 359.2
384(6) 0.02778 272.5 372.2
386(6) 0.02778 272.3 378.6
384(6) 0.02778 272.2 377.1
377(6) 0.02778 272.1 368.0
353(6) 0.02778 272.0 353.3
343(6) 0.02778 271.9 336.3
322(6) 0.02778 271.8 320.2
303(6) 0.02778 271.7 307.2
302(5) 0.0400 271.6 298.3
290(5) 0.0400 271.5 293.1
289(5) 0.0400 271.4 290.8
286(5) 0.0400 271.3 290.1
299(5) 0.0400 271.2 290.0
310(6) 0.02778 271.1 289.3
318(6) 0.02778 271.0 288.0
325(6) 0.02778 270.9 286.5
333(6) 0.02778 270.8 285.3
337(6) 0.02778 270.7 285.0
320(6) 0.02778 270.6 285.0
323(6) 0.02778 270.6 286.4
316(6) 0.02778 270.5 288.0
305(6) 0.02778 270.4 288.9
290(5) 0.0400 270.4 288.7
287(5) 0.0400 270.3 287.2
286(5) 0.0400 270.2 285.0
276(6) 0.02778 270.2 282.8
293(5) 0.0400 270.1 281.0
285(5) 0.0400 270.0 279.8
293(5) 0.0400 270.0 279.2
281(5) 0.0400 269.9 279.2
296(5) 0.0400 269.9 279.7
286(5) 0.0400 269.8 280.7
293(5) 0.0400 269.8 282.3
304(6) 0.02778 269.7 285.1
301(5) 0.0400 269.7 289.4
305(6) 0.02778 269.7 297.1
330(6) 0.02778 269.6 309.2
342(6) 0.02778 269.6 327.0
361(6) 0.02778 269.5 351.2
382(6) 0.02778 269.5 381.2
399(6) 0.02778 269.5 415.4
437(7) 0.02041 269.5 450.7
486(7) 0.02041 269.4 485.1
517(7) 0.02041 269.4 518.5
564(8) 0.01563 269.4 551.0
589(8) 0.01563 269.4 577.7
588(8) 0.01563 269.4 589.0
598(8) 0.01563 269.3 576.5
549(7) 0.02041 269.3 540.3
501(7) 0.02041 269.3 490.6
445(7) 0.02041 269.3 441.4
389(6) 0.02778 269.3 403.9
373(6) 0.02778 269.3 384.4
377(6) 0.02778 269.3 384.4
376(6) 0.02778 269.3 401.6
418(6) 0.02778 269.3 429.6
438(7) 0.02041 269.3 458.8
461(7) 0.02041 269.3 477.8
469(7) 0.02041 269.3 477.7
439(7) 0.02041 269.3 458.2
420(6) 0.02778 269.3 426.7
395(6) 0.02778 269.4 392.3
369(6) 0.02778 269.4 361.1
367(6) 0.02778 269.4 336.5
357(6) 0.02778 269.4 318.9
353(6) 0.02778 269.4 306.8
349(6) 0.02778 269.5 298.2
355(6) 0.02778 269.5 292.1
358(6) 0.02778 269.5 287.6
344(6) 0.02778 269.5 284.5
332(6) 0.02778 269.6 282.5
305(6) 0.02778 269.6 281.8
303(6) 0.02778 269.6 282.5
297(5) 0.0400 269.7 284.7
292(5) 0.0400 269.7 289.0
286(5) 0.0400 269.8 295.8
296(5) 0.0400 269.8 304.8
299(5) 0.0400 269.8 315.4
309(6) 0.02778 269.9 325.5
308(6) 0.02778 269.9 332.6
305(6) 0.02778 270.0 334.7
317(6) 0.02778 270.0 331.8
323(6) 0.02778 270.1 325.7
330(6) 0.02778 270.1 318.1
351(6) 0.02778 270.2 310.4
371(6) 0.02778 270.2 303.6
378(6) 0.02778 270.3 298.1
368(6) 0.02778 270.4 293.8
363(6) 0.02778 270.4 290.4
341(6) 0.02778 270.5 287.2
313(6) 0.02778 270.5 284.3
297(5) 0.0400 270.6 282.0
280(5) 0.0400 270.7 280.3
282(5) 0.0400 270.7 279.6
270(5) 0.0400 270.8 279.7
277(5) 0.0400 270.9 280.5
272(5) 0.0400 270.9 281.7
277(5) 0.0400 271.0 282.9
268(5) 0.0400 271.1 283.4
273(5) 0.0400 271.1 283.1
264(5) 0.0400 271.2 281.9
273(5) 0.0400 271.3 280.3
256(5) 0.0400 271.4 278.8
257(5) 0.0400 271.5 277.5
276(5) 0.0400 271.5 276.6
271(5) 0.0400 271.6 276.1
252(5) 0.0400 271.7 275.9
266(5) 0.0400 271.8 275.8
267(5) 0.0400 271.9 276.0
258(5) 0.0400 271.9 276.3
269(5) 0.0400 272.0 276.8
269(5) 0.0400 272.1 277.6
266(5) 0.0400 272.2 278.7
276(5) 0.0400 272.3 280.1
282(5) 0.0400 272.4 281.8
304(6) 0.02778 272.5 283.5
305(6) 0.02778 272.6 285.2
329(6) 0.02778 272.6 286.8
329(6) 0.02778 272.7 288.5
339(6) 0.02778 272.8 290.5
337(6) 0.02778 272.9 293.1
343(6) 0.02778 273.0 296.3
327(6) 0.02778 273.1 300.2
320(6) 0.02778 273.2 304.5
327(6) 0.02778 273.3 308.3
316(6) 0.02778 273.4 310.0
312(6) 0.02778 273.5 308.4
308(6) 0.02778 273.6 304.1
305(6) 0.02778 273.7 298.6
292(5) 0.0400 273.8 293.3
276(5) 0.0400 273.9 289.0
275(5) 0.0400 274.0 286.0
283(5) 0.0400 274.1 284.4
281(5) 0.0400 274.2 283.6
274(5) 0.0400 274.3 283.5
272(5) 0.0400 274.4 283.8
276(5) 0.0400 274.5 284.3
277(5) 0.0400 274.6 284.9
281(5) 0.0400 274.7 285.7
279(5) 0.0400 274.8 286.7
275(5) 0.0400 274.9 288.0
288(6) 0.02778 275.0 289.6
296(5) 0.0400 275.1 291.6
318(6) 0.02778 275.2 294.4
310(6) 0.02778 275.3 298.2
314(6) 0.02778 275.4 303.1
318(6) 0.02778 275.5 309.4
324(6) 0.02778 275.6 317.4
320(6) 0.02778 275.7 327.9
319(6) 0.02778 275.8 342.8
347(6) 0.02778 275.9 366.1
368(6) 0.02778 276.0 403.1
426(7) 0.02041 276.1 459.6
523(7) 0.02041 276.2 537.8
609(8) 0.01563 276.3 634.6
724(9) 0.01235 276.4 738.0
821(9) 0.01235 276.5 828.5
895(9) 0.01235 276.6 886.4
935(10) 0.01000 276.7 906.2
926(10) 0.01000 276.8 897.0
879(9) 0.01235 276.9 866.4
821(9) 0.01235 277.1 816.6
749(9) 0.01235 277.2 757.1
706(8) 0.01563 277.3 708.4
696(8) 0.01563 277.4 688.9
738(9) 0.01235 277.5 704.9
786(9) 0.01235 277.6 747.3
885(9) 0.01235 277.7 794.0
891(9) 0.01235 277.8 817.9
868(9) 0.01235 277.9 801.2
805(9) 0.01235 278.0 742.2
691(8) 0.01563 278.1 654.5
587(8) 0.01563 278.2 560.5
491(7) 0.02041 278.2 478.4
442(7) 0.02041 278.3 417.0
396(6) 0.02778 278.4 377.5
384(6) 0.02778 278.5 356.1
383(6) 0.02778 278.6 347.0
370(6) 0.02778 278.7 344.2
373(6) 0.02778 278.8 342.4
348(6) 0.02778 278.9 338.0
329(6) 0.02778 279.0 330.4
319(6) 0.02778 279.1 321.2
319(6) 0.02778 279.2 312.2
304(6) 0.02778 279.3 304.7
290(5) 0.0400 279.4 299.0
284(5) 0.0400 279.5 295.2
285(5) 0.0400 279.6 292.7
289(5) 0.0400 279.6 291.1
298(5) 0.0400 279.7 290.0
291(5) 0.0400 279.8 289.2
298(6) 0.02778 279.9 288.6
289(5) 0.0400 280.0 288.2
297(5) 0.0400 280.1 287.8
295(5) 0.0400 280.2 287.5
301(5) 0.0400 280.2 287.3
292(5) 0.0400 280.3 287.2
283(5) 0.0400 280.4 287.1
285(5) 0.0400 280.5 287.2
275(5) 0.0400 280.6 287.4
277(5) 0.0400 280.6 287.8
282(5) 0.0400 280.7 288.6
280(5) 0.0400 280.8 289.7
281(5) 0.0400 280.9 291.2
284(5) 0.0400 280.9 293.1
287(5) 0.0400 281.0 295.3
291(5) 0.0400 281.1 297.6
298(5) 0.0400 281.1 299.8
298(5) 0.0400 281.2 301.5
295(5) 0.0400 281.3 302.2
294(6) 0.02778 281.3 301.6
294(5) 0.0400 281.4 300.3
295(5) 0.0400 281.5 298.9
286(5) 0.0400 281.5 298.3
280(5) 0.0400 281.6 299.0
282(5) 0.0400 281.7 301.9
288(5) 0.0400 281.7 308.2
290(5) 0.0400 281.8 319.6
306(6) 0.02778 281.8 338.4
332(6) 0.02778 281.9 366.6
369(6) 0.02778 281.9 403.7
416(6) 0.02778 282.0 445.6
449(7) 0.02041 282.1 482.6
460(7) 0.02041 282.1 501.8
452(7) 0.02041 282.2 493.7
419(6) 0.02778 282.2 462.3
392(6) 0.02778 282.2 420.3
352(6) 0.02778 282.3 379.7
329(6) 0.02778 282.3 347.1
319(6) 0.02778 282.4 324.6
304(6) 0.02778 282.4 311.2
293(5) 0.0400 282.5 304.6
302(5) 0.0400 282.5 302.2
296(5) 0.0400 282.5 302.1
300(5) 0.0400 282.6 302.8
309(6) 0.02778 282.6 303.4
320(6) 0.02778 282.6 303.3
314(6) 0.02778 282.7 302.7
310(6) 0.02778 282.7 301.6
303(6) 0.02778 282.7 300.1
291(5) 0.0400 282.8 298.2
288(6) 0.02778 282.8 296.0
285(5) 0.0400 282.8 293.8
286(5) 0.0400 282.8 291.8
286(5) 0.0400 282.8 290.3
272(5) 0.0400 282.9 289.3
269(5) 0.0400 282.9 288.8
276(5) 0.0400 282.9 289.0
276(5) 0.0400 282.9 289.8
272(5) 0.0400 282.9 291.5
268(5) 0.0400 282.9 294.5
282(5) 0.0400 282.9 298.9
277(5) 0.0400 282.9 304.6
288(5) 0.0400 283.0 311.6
300(5) 0.0400 283.0 318.6
296(5) 0.0400 283.0 324.7
302(5) 0.0400 283.0 328.9
305(6) 0.02778 283.0 331.2
308(6) 0.02778 283.0 331.2
307(6) 0.02778 283.0 329.0
313(6) 0.02778 283.0 325.1
314(6) 0.02778 282.9 320.0
303(6) 0.02778 282.9 314.5
293(5) 0.0400 282.9 309.2
289(5) 0.0400 282.9 304.5
297(5) 0.0400 282.9 300.5
273(5) 0.0400 282.9 297.2
275(5) 0.0400 282.9 294.3
287(5) 0.0400 282.9 291.8
278(5) 0.0400 282.8 289.6
279(5) 0.0400 282.8 288.1
283(5) 0.0400 282.8 286.9
285(5) 0.0400 282.8 286.1
296(5) 0.0400 282.7 285.6
301(5) 0.0400 282.7 285.3
304(6) 0.02778 282.7 285.0
309(6) 0.02778 282.7 284.9
290(5) 0.0400 282.6 284.8
289(5) 0.0400 282.6 284.7
290(5) 0.0400 282.5 285.0
278(5) 0.0400 282.5 285.0
284(5) 0.0400 282.5 284.9
288(5) 0.0400 282.4 284.9
293(5) 0.0400 282.4 285.0
303(6) 0.02778 282.3 285.0
321(6) 0.02778 282.3 285.1
323(6) 0.02778 282.2 285.3
335(6) 0.02778 282.2 285.6
346(6) 0.02778 282.1 286.1
342(6) 0.02778 282.1 287.2
342(6) 0.02778 282.0 289.0
325(6) 0.02778 282.0 291.9
329(6) 0.02778 281.9 296.0
315(6) 0.02778 281.9 301.1
316(6) 0.02778 281.8 306.2
304(6) 0.02778 281.7 309.9
311(6) 0.02778 281.7 310.6
295(5) 0.0400 281.6 308.0
287(5) 0.0400 281.5 303.3
285(5) 0.0400 281.5 298.1
288(5) 0.0400 281.4 293.5
284(5) 0.0400 281.3 290.1
272(5) 0.0400 281.2 288.0
275(5) 0.0400 281.2 286.8
284(5) 0.0400 281.1 286.4
284(5) 0.0400 281.0 286.2
288(5) 0.0400 280.9 286.3
280(5) 0.0400 280.8 286.5
282(5) 0.0400 280.8 286.5
273(5) 0.0400 280.7 286.4
276(5) 0.0400 280.6 286.3
279(5) 0.0400 280.5 286.2
282(5) 0.0400 280.4 286.2
283(5) 0.0400 280.3 286.4
285(5) 0.0400 280.2 286.8
284(5) 0.0400 280.1 287.5
292(6) 0.02778 280.0 288.7
279(5) 0.0400 279.9 290.9
284(5) 0.0400 279.8 294.7
290(5) 0.0400 279.7 300.9
295(5) 0.0400 279.6 310.3
303(6) 0.02778 279.5 323.2
323(6) 0.02778 279.4 338.7
351(6) 0.02778 279.3 354.4
367(6) 0.02778 279.2 367.0
353(6) 0.02778 279.1 374.4
362(6) 0.02778 279.0 376.7
370(6) 0.02778 278.9 374.6
358(6) 0.02778 278.7 366.9
339(6) 0.02778 278.6 353.7
337(6) 0.02778 278.5 338.1
318(6) 0.02778 278.4 323.9
326(6) 0.02778 278.3 313.1
318(6) 0.02778 278.1 306.5
299(5) 0.0400 278.0 303.4
312(6) 0.02778 277.9 302.8
318(6) 0.02778 277.8 303.1
312(6) 0.02778 277.6 303.2
304(6) 0.02778 277.5 302.6
304(6) 0.02778 277.4 301.1
291(5) 0.0400 277.2 299.1
295(5) 0.0400 277.1 297.3
286(5) 0.0400 277.0 296.1
286(5) 0.0400 276.8 295.7
291(5) 0.0400 276.7 296.2
289(5) 0.0400 276.6 297.4
286(5) 0.0400 276.4 299.5
295(5) 0.0400 276.3 302.7
303(6) 0.02778 276.1 307.7
309(6) 0.02778 276.0 315.8
302(5) 0.0400 275.8 329.0
327(6) 0.02778 275.7 350.3
359(6) 0.02778 275.5 383.0
413(6) 0.02778 275.4 430.2
460(7) 0.02041 275.2 492.3
562(7) 0.02041 275.1 565.4
639(8) 0.01563 274.9 640.4
716(8) 0.01563 274.8 703.4
743(9) 0.01235 274.6 736.3
756(9) 0.01235 274.5 729.1
718(8) 0.01563 274.3 694.7
679(8) 0.01563 274.2 660.8
654(8) 0.01563 274.0 648.2
657(8) 0.01563 273.8 663.2
698(8) 0.01563 273.7 698.7
749(9) 0.01235 273.5 735.8
785(9) 0.01235 273.3 750.9
776(9) 0.01235 273.2 737.2
746(9) 0.01235 273.0 718.0
753(9) 0.01235 272.8 727.8
792(9) 0.01235 272.7 791.2
929(10) 0.01000 272.5 913.7
1116(11) 0.00826 272.3 1075.3
1291(11) 0.00826 272.2 1226.5
1376(12) 0.00694 272.0 1296.1
1317(11) 0.00826 271.8 1237.3
1134(11) 0.00826 271.6 1075.8
928(10) 0.01000 271.5 879.0
730(9) 0.01235 271.3 701.2
591(8) 0.01563 271.1 569.1
518(7) 0.02041 270.9 486.9
477(7) 0.02041 270.8 443.7
462(7) 0.02041 270.6 423.6
434(7) 0.02041 270.4 412.8
411(6) 0.02778 270.2 403.2
386(6) 0.02778 270.0 391.0
379(6) 0.02778 269.9 375.3
356(6) 0.02778 269.7 358.1
348(6) 0.02778 269.5 342.3
338(6) 0.02778 269.3 330.2
338(6) 0.02778 269.1 323.6
346(6) 0.02778 268.9 322.8
358(6) 0.02778 268.7 326.9
354(6) 0.02778 268.6 333.6
359(6) 0.02778 268.4 339.5
366(6) 0.02778 268.2 341.1
347(6) 0.02778 268.0 337.2
332(6) 0.02778 267.8 330.2
333(6) 0.02778 267.6 323.3
319(6) 0.02778 267.4 319.2
318(6) 0.02778 267.2 318.5
333(6) 0.02778 267.0 320.1
331(6) 0.02778 266.8 321.0
349(6) 0.02778 266.7 318.3
354(6) 0.02778 266.5 311.5
352(6) 0.02778 266.3 302.9
349(6) 0.02778 266.1 294.8
343(6) 0.02778 265.9 288.4
324(6) 0.02778 265.7 283.9
306(6) 0.02778 265.5 281.0
297(5) 0.0400 265.3 279.2
285(5) 0.0400 265.1 278.2
279(5) 0.0400 264.9 277.9
279(6) 0.02778 264.7 278.3
274(5) 0.0400 264.5 279.2
270(5) 0.0400 264.3 280.0
280(5) 0.0400 264.1 280.2
277(5) 0.0400 263.9 279.7
278(5) 0.0400 263.7 278.9
274(6) 0.02778 263.5 278.6
278(5) 0.0400 263.3 279.3
280(6) 0.02778 263.1 280.9
289(5) 0.0400 262.9 282.9
279(6) 0.02778 262.7 284.1
284(5) 0.0400 262.5 284.0
277(5) 0.0400 262.3 282.9
275(5) 0.0400 262.1 281.9
269(5) 0.0400 261.9 282.3
270(5) 0.0400 261.7 284.4
274(5) 0.0400 261.5 287.7
275(5) 0.0400 261.3 290.9
288(5) 0.0400 261.1 292.2
303(6) 0.02778 260.9 290.9
301(5) 0.0400 260.7 287.6
325(6) 0.02778 260.5 283.6
335(6) 0.02778 260.3 280.2
348(6) 0.02778 260.1 278.5
340(6) 0.02778 259.9 279.2
332(6) 0.02778 259.7 282.5
310(6) 0.02778 259.5 287.7
302(5) 0.0400 259.3 293.6
291(5) 0.0400 259.1 298.0
279(5) 0.0400 258.9 299.1
273(5) 0.0400 258.7 296.6
266(5) 0.0400 258.5 291.6
267(5) 0.0400 258.3 285.7
267(5) 0.0400 258.1 280.4
264(5) 0.0400 257.9 276.7
265(5) 0.0400 257.7 275.0
265(5) 0.0400 257.5 275.9
264(5) 0.0400 257.3 279.7
272(5) 0.0400 257.1 287.5
285(5) 0.0400 256.9 300.1
298(5) 0.0400 256.7 318.3
340(6) 0.02778 256.5 340.9
374(6) 0.02778 256.3 365.5
397(6) 0.02778 256.1 387.3
412(6) 0.02778 255.9 402.7
425(7) 0.02041 255.7 408.9
417(6) 0.02778 255.5 405.2
394(6) 0.02778 255.3 392.0
373(6) 0.02778 255.1 373.4
354(6) 0.02778 254.9 355.5
329(6) 0.02778 254.7 342.8
336(6) 0.02778 254.5 337.5
338(6) 0.02778 254.3 340.0
344(6) 0.02778 254.1 349.5
366(6) 0.02778 253.9 363.9
370(6) 0.02778 253.8 381.1
379(6) 0.02778 253.6 399.1
393(6) 0.02778 253.4 413.9
414(6) 0.02778 253.2 424.3
409(6) 0.02778 253.0 430.7
408(6) 0.02778 252.8 431.6
409(6) 0.02778 252.6 422.1
379(6) 0.02778 252.4 401.0
357(6) 0.02778 252.2 372.9
337(6) 0.02778 252.0 343.2
309(6) 0.02778 251.9 316.5
296(5) 0.0400 251.7 295.8
280(5) 0.0400 251.5 281.5
261(5) 0.0400 251.3 272.5
270(5) 0.0400 251.1 267.5
258(5) 0.0400 250.9 265.1
259(5) 0.0400 250.7 264.3
259(5) 0.0400 250.6 264.4
263(5) 0.0400 250.4 264.8
264(5) 0.0400 250.2 264.9
254(5) 0.0400 250.0 264.4
263(5) 0.0400 249.8 263.3
251(5) 0.0400 249.7 261.7
253(5) 0.0400 249.5 260.2
245(5) 0.0400 249.3 259.2
251(5) 0.0400 249.1 258.9
239(5) 0.0400 249.0 259.0
257(5) 0.0400 248.8 259.2
229(5) 0.0400 248.6 258.9
260(5) 0.0400 248.4 257.9
248(5) 0.0400 248.3 256.7
249(5) 0.0400 248.1 255.8
243(5) 0.0400 247.9 255.5
238(5) 0.0400 247.8 255.7
249(5) 0.0400 247.6 256.2
245(5) 0.0400 247.4 256.8
255(5) 0.0400 247.2 257.3
259(5) 0.0400 247.1 257.8
254(5) 0.0400 246.9 258.5
256(5) 0.0400 246.8 259.4
258(5) 0.0400 246.6 260.5
281(5) 0.0400 246.4 261.4
289(5) 0.0400 246.3 261.4
302(5) 0.0400 246.1 260.0
325(6) 0.02778 245.9 257.6
332(6) 0.02778 245.8 254.9
329(6) 0.02778 245.6 252.6
305(5) 0.0400 245.5 251.0
294(6) 0.02778 245.3 250.0
274(5) 0.0400 245.2 249.8
263(5) 0.0400 245.0 250.1
260(5) 0.0400 244.9 251.2
249(5) 0.0400 244.7 252.8
246(5) 0.0400 244.6 255.0
245(5) 0.0400 244.4 257.3
255(5) 0.0400 244.3 258.9
255(5) 0.0400 244.1 259.5
250(5) 0.0400 244.0 259.2
258(5) 0.0400 243.8 258.7
251(5) 0.0400 243.7 258.3
261(5) 0.0400 243.5 257.5
249(5) 0.0400 243.4 256.0
258(5) 0.0400 243.3 254.0
236(5) 0.0400 243.1 252.1
249(5) 0.0400 243.0 250.5
249(5) 0.0400 242.9 249.5
255(5) 0.0400 242.7 249.0
266(5) 0.0400 242.6 248.6
277(5) 0.0400 242.4 248.3
270(5) 0.0400 242.3 248.1
264(5) 0.0400 242.2 247.9
266(5) 0.0400 242.1 247.8
260(5) 0.0400 241.9 247.9
260(5) 0.0400 241.8 248.2
243(5) 0.0400 241.7 248.7
263(5) 0.0400 241.6 249.5
260(5) 0.0400 241.4 250.7
268(5) 0.0400 241.3 252.5
251(5) 0.0400 241.2 255.2
274(5) 0.0400 241.1 259.4
266(5) 0.0400 240.9 265.5
287(5) 0.0400 240.8 274.1
304(6) 0.02778 240.7 285.7
318(6) 0.02778 240.6 300.5
347(6) 0.02778 240.5 318.3
367(6) 0.02778 240.4 338.6
377(6) 0.02778 240.3 363.1
397(6) 0.02778 240.2 395.2
423(7) 0.02041 240.0 435.8
459(7) 0.02041 239.9 477.1
461(7) 0.02041 239.8 502.8
479(7) 0.02041 239.7 495.9
442(7) 0.02041 239.6 458.1
388(6) 0.02778 239.5 407.0
337(6) 0.02778 239.4 358.8
315(6) 0.02778 239.3 321.5
284(5) 0.0400 239.2 296.9
274(5) 0.0400 239.1 283.0
278(5) 0.0400 239.0 276.7
271(5) 0.0400 238.9 275.0
266(5) 0.0400 238.9 275.2
274(5) 0.0400 238.8 275.6
284(5) 0.0400 238.7 276.5
285(5) 0.0400 238.6 278.9
285(5) 0.0400 238.5 284.0
290(5) 0.0400 238.4 291.3
308(6) 0.02778 238.3 299.2
299(5) 0.0400 238.2 306.5
319(6) 0.02778 238.2 314.2
322(6) 0.02778 238.1 326.7
342(6) 0.02778 238.0 348.1
358(6) 0.02778 237.9 378.2
377(6) 0.02778 237.8 410.8
412(6) 0.02778 237.8 432.4
408(6) 0.02778 237.7 429.2
392(6) 0.02778 237.6 402.1
352(6) 0.02778 237.5 365.3
324(6) 0.02778 237.5 331.5
306(6) 0.02778 237.4 306.7
281(5) 0.0400 237.3 291.1
276(5) 0.0400 237.3 281.9
264(5) 0.0400 237.2 275.9
264(5) 0.0400 237.1 271.9
251(5) 0.0400 237.1 269.7
252(5) 0.0400 237.0 268.8
259(5) 0.0400 237.0 267.8
265(5) 0.0400 236.9 265.3
257(5) 0.0400 236.8 261.4
254(5) 0.0400 236.8 257.4
244(5) 0.0400 236.7 254.3
254(5) 0.0400 236.7 252.8
261(5) 0.0400 236.6 252.7
266(5) 0.0400 236.6 253.4
268(5) 0.0400 236.5 254.3
273(5) 0.0400 236.5 254.7
275(5) 0.0400 236.4 254.9
264(5) 0.0400 236.4 255.9
266(5) 0.0400 236.3 258.6
269(5) 0.0400 236.3 263.5
287(5) 0.0400 236.2 271.2
282(5) 0.0400 236.2 281.7
294(5) 0.0400 236.2 295.3
301(5) 0.0400 236.1 311.5
325(6) 0.02778 236.1 326.9
330(6) 0.02778 236.0 335.4
319(6) 0.02778 236.0 332.9
304(6) 0.02778 236.0 323.4
289(5) 0.0400 235.9 315.3
302(6) 0.02778 235.9 314.4
305(6) 0.02778 235.9 321.6
310(6) 0.02778 235.9 333.0
310(6) 0.02778 235.8 340.1
310(6) 0.02778 235.8 335.3
296(5) 0.0400 235.8 319.2
292(5) 0.0400 235.8 299.0
274(5) 0.0400 235.7 280.9
268(5) 0.0400 235.7 268.0
272(5) 0.0400 235.7 260.8
270(5) 0.0400 235.7 258.3
275(5) 0.0400 235.6 259.2
275(5) 0.0400 235.6 261.4
273(5) 0.0400 235.6 262.8
265(5) 0.0400 235.6 261.9
262(5) 0.0400 235.6 258.9
254(5) 0.0400 235.6 255.3
235(5) 0.0400 235.6 252.4
247(5) 0.0400 235.5 250.6
245(5) 0.0400 235.5 250.0
241(5) 0.0400 235.5 249.9
244(5) 0.0400 235.5 250.0
244(5) 0.0400 235.5 250.5
241(5) 0.0400 235.5 252.1
251(5) 0.0400 235.5 255.8
256(5) 0.0400 235.5 263.0
265(5) 0.0400 235.5 275.4
290(5) 0.0400 235.5 294.2
303(6) 0.02778 235.5 319.3
330(6) 0.02778 235.5 347.7
364(6) 0.02778 235.5 372.3
377(6) 0.02778 235.5 385.2
399(6) 0.02778 235.5 386.1
392(6) 0.02778 235.5 380.5
390(6) 0.02778 235.5 371.6
375(6) 0.02778 235.5 361.5
363(6) 0.02778 235.5 355.2
358(6) 0.02778 235.6 355.5
339(6) 0.02778 235.6 359.5
346(6) 0.02778 235.6 359.5
320(6) 0.02778 235.6 347.7
326(6) 0.02778 235.6 326.3
299(5) 0.0400 235.6 302.7
270(5) 0.0400 235.6 282.8
266(5) 0.0400 235.6 268.9
254(5) 0.0400 235.7 261.4
256(5) 0.0400 235.7 259.2
251(5) 0.0400 235.7 260.7
254(5) 0.0400 235.7 264.1
257(5) 0.0400 235.7 267.3
254(5) 0.0400 235.8 267.8
250(5) 0.0400 235.8 264.7
247(5) 0.0400 235.8 259.4
248(5) 0.0400 235.8 254.2
249(5) 0.0400 235.8 250.2
242(5) 0.0400 235.9 248.1
246(5) 0.0400 235.9 247.8
247(5) 0.0400 235.9 249.2
248(5) 0.0400 236.0 251.8
260(5) 0.0400 236.0 255.2
263(5) 0.0400 236.0 258.6
271(5) 0.0400 236.0 260.9
281(5) 0.0400 236.1 261.0
276(5) 0.0400 236.1 258.7
272(5) 0.0400 236.1 255.5
271(5) 0.0400 236.2 253.2
266(5) 0.0400 236.2 252.5
267(5) 0.0400 236.2 253.2
263(5) 0.0400 236.3 254.5
258(5) 0.0400 236.3 254.8
251(5) 0.0400 236.3 253.3
245(5) 0.0400 236.4 250.8
239(5) 0.0400 236.4 248.4
250(5) 0.0400 236.5 246.7
253(5) 0.0400 236.5 245.7
245(5) 0.0400 236.5 245.2
244(5) 0.0400 236.6 244.7
244(5) 0.0400 236.6 244.1
249(5) 0.0400 236.7 243.6
247(5) 0.0400 236.7 243.4
255(5) 0.0400 236.7 243.7
261(5) 0.0400 236.8 244.3
251(5) 0.0400 236.8 245.0
260(5) 0.0400 236.9 245.7
260(5) 0.0400 236.9 246.3
262(5) 0.0400 237.0 247.0
262(5) 0.0400 237.0 247.6
258(5) 0.0400 237.1 249.0
266(5) 0.0400 237.1 252.2
255(5) 0.0400 237.2 258.1
256(5) 0.0400 237.2 267.3
264(5) 0.0400 237.3 279.1
274(5) 0.0400 237.3 290.7
280(5) 0.0400 237.4 297.4
279(5) 0.0400 237.4 295.0
267(5) 0.0400 237.5 285.3
264(5) 0.0400 237.5 273.5
260(5) 0.0400 237.6 263.5
254(5) 0.0400 237.6 256.6
266(5) 0.0400 237.7 252.7
254(5) 0.0400 237.7 250.9
254(5) 0.0400 237.8 249.6
256(5) 0.0400 237.8 248.2
245(5) 0.0400 237.9 246.7
256(5) 0.0400 237.9 245.3
261(5) 0.0400 238.0 244.3
258(5) 0.0400 238.0 243.7
261(5) 0.0400 238.1 243.5
263(5) 0.0400 238.1 243.4
265(5) 0.0400 238.2 243.6
253(5) 0.0400 238.3 243.9
254(5) 0.0400 238.3 244.4
264(5) 0.0400 238.4 245.2
260(5) 0.0400 238.4 246.5
250(5) 0.0400 238.5 248.5
254(5) 0.0400 238.5 251.6
257(5) 0.0400 238.6 255.8
252(5) 0.0400 238.7 260.9
259(5) 0.0400 238.7 265.9
267(5) 0.0400 238.8 269.5
267(5) 0.0400 238.8 271.5
268(5) 0.0400 238.9 272.9
271(5) 0.0400 238.9 274.6
287(5) 0.0400 239.0 276.7
283(5) 0.0400 239.1 279.4
284(5) 0.0400 239.1 281.9
298(5) 0.0400 239.2 283.0
287(5) 0.0400 239.2 283.2
293(5) 0.0400 239.3 285.6
287(5) 0.0400 239.4 294.5
307(6) 0.02778 239.4 313.9
329(6) 0.02778 239.5 346.8
371(6) 0.02778 239.5 392.7
423(7) 0.02041 239.6 445.1
489(7) 0.02041 239.7 488.8
504(7) 0.02041 239.7 503.9
492(7) 0.02041 239.8 487.7
452(7) 0.02041 239.8 462.4
443(7) 0.02041 239.9 451.4
462(7) 0.02041 240.0 465.5
520(7) 0.02041 240.0 500.5
553(7) 0.02041 240.1 536.7
573(8) 0.01563 240.1 544.7
541(7) 0.02041 240.2 510.8
465(7) 0.02041 240.3 452.0
402(6) 0.02778 240.3 391.7
355(6) 0.02778 240.4 343.3
302(5) 0.0400 240.4 311.0
286(5) 0.0400 240.5 293.0
285(5) 0.0400 240.6 284.8
280(5) 0.0400 240.6 281.2
261(5) 0.0400 240.7 278.1
257(5) 0.0400 240.7 273.6
256(5) 0.0400 240.8 268.7
267(5) 0.0400 240.8 264.9
259(5) 0.0400 240.9 263.1
258(5) 0.0400 241.0 263.3
264(5) 0.0400 241.0 264.8
268(5) 0.0400 241.1 266.2
256(5) 0.0400 241.1 266.0
261(5) 0.0400 241.2 264.3
266(5) 0.0400 241.3 262.7
261(5) 0.0400 241.3 262.2
259(5) 0.0400 241.4 263.1
247(5) 0.0400 241.4 264.4
242(5) 0.0400 241.5 264.4
233(5) 0.0400 241.6 262.4
237(5) 0.0400 241.6 259.0
247(5) 0.0400 241.7 255.6
245(5) 0.0400 241.7 252.8
246(5) 0.0400 241.8 250.8
237(5) 0.0400 241.8 249.6
242(5) 0.0400 241.9 249.2
240(5) 0.0400 241.9 249.3
248(5) 0.0400 242.0 249.9
247(5) 0.0400 242.1 250.9
240(5) 0.0400 242.1 252.2
246(5) 0.0400 242.2 253.8
237(5) 0.0400 242.2 256.1
249(5) 0.0400 242.3 259.6
252(5) 0.0400 242.3 264.9
246(5) 0.0400 242.4 272.0
263(5) 0.0400 242.4 280.1
273(5) 0.0400 242.5 286.7
278(5) 0.0400 242.5 288.4
276(5) 0.0400 242.6 284.8
279(5) 0.0400 242.7 279.1
270(5) 0.0400 242.7 274.5
269(5) 0.0400 242.8 271.7
278(5) 0.0400 242.8 269.6
266(5) 0.0400 242.9 267.1
267(5) 0.0400 242.9 264.0
259(5) 0.0400 243.0 260.7
254(5) 0.0400 243.0 257.5
252(5) 0.0400 243.1 254.8
253(5) 0.0400 243.1 252.9
250(5) 0.0400 243.2 251.7
249(5) 0.0400 243.2 251.1
241(5) 0.0400 243.3 250.7
247(5) 0.0400 243.3 250.4
235(5) 0.0400 243.4 249.9
240(5) 0.0400 243.4 249.4
248(5) 0.0400 243.4 249.0
241(5) 0.0400 243.5 248.8
239(5) 0.0400 243.5 248.8
240(5) 0.0400 243.6 249.2
241(5) 0.0400 243.6 249.9
258(5) 0.0400 243.7 251.2
249(5) 0.0400 243.7 253.5
257(5) 0.0400 243.8 257.2
269(5) 0.0400 243.8 263.0
269(5) 0.0400 243.9 270.7
279(5) 0.0400 243.9 279.8
279(5) 0.0400 243.9 288.4
282(5) 0.0400 244.0 294.1
284(5) 0.0400 244.0 295.4
290(5) 0.0400 244.1 292.6
269(5) 0.0400 244.1 288.3
271(5) 0.0400 244.1 284.4
270(5) 0.0400 244.2 280.9
273(5) 0.0400 244.2 278.1
269(5) 0.0400 244.3 277.4
277(5) 0.0400 244.3 279.7
266(5) 0.0400 244.3 285.3
267(5) 0.0400 244.4 293.7
281(5) 0.0400 244.4 303.4
283(5) 0.0400 244.4 312.9
294(5) 0.0400 244.5 322.9
316(6) 0.02778 244.5 335.2
340(6) 0.02778 244.6 349.7
370(6) 0.02778 244.6 362.3
400(6) 0.02778 244.6 366.8
414(6) 0.02778 244.7 359.3
395(6) 0.02778 244.7 342.1
370(6) 0.02778 244.7 321.2
336(6) 0.02778 244.8 301.5
312(6) 0.02778 244.8 286.6
295(5) 0.0400 244.8 277.6
271(5) 0.0400 244.9 274.3
273(5) 0.0400 244.9 274.7
255(5) 0.0400 244.9 276.4
267(5) 0.0400 244.9 276.7
266(5) 0.0400 245.0 274.6
273(5) 0.0400 245.0 271.8
261(5) 0.0400 245.0 270.1
276(5) 0.0400 245.1 270.3
276(5) 0.0400 245.1 272.0
277(5) 0.0400 245.1 275.2
276(5) 0.0400 245.1 279.1
270(5) 0.0400 245.2 282.7
277(5) 0.0400 245.2 285.3
280(5) 0.0400 245.2 288.0
277(5) 0.0400 245.2 291.1
279(5) 0.0400 245.3 292.6
282(5) 0.0400 245.3 290.1
288(5) 0.0400 245.3 283.4
297(5) 0.0400 245.3 274.5
305(6) 0.02778 245.4 266.3
296(5) 0.0400 245.4 259.9
322(6) 0.02778 245.4 255.6
335(6) 0.02778 245.4 253.0
363(6) 0.02778 245.5 251.5
345(6) 0.02778 245.5 250.6
337(6) 0.02778 245.5 250.1
324(6) 0.02778 245.5 249.7
288(5) 0.0400 245.5 249.5
280(5) 0.0400 245.6 249.3
267(5) 0.0400 245.6 249.2
264(5) 0.0400 245.6 249.2
254(5) 0.0400 245.6 249.3
254(5) 0.0400 245.6 249.4
251(5) 0.0400 245.6 249.8
254(5) 0.0400 245.7 250.4
246(5) 0.0400 245.7 251.3
252(5) 0.0400 245.7 252.4
260(5) 0.0400 245.7 253.6
247(5) 0.0400 245.7 254.4
254(5) 0.0400 245.7 254.4
244(5) 0.0400 245.7 253.7
248(5) 0.0400 245.8 252.9
261(5) 0.0400 245.8 252.5
254(5) 0.0400 245.8 252.8
258(5) 0.0400 245.8 254.0
264(5) 0.0400 245.8 256.4
278(5) 0.0400 245.8 259.9
283(5) 0.0400 245.8 264.1
281(5) 0.0400 245.8 268.1
276(5) 0.0400 245.9 270.0
277(5) 0.0400 245.9 269.0
270(5) 0.0400 245.9 266.3
266(5) 0.0400 245.9 263.3
257(5) 0.0400 245.9 260.8
256(5) 0.0400 245.9 258.6
260(5) 0.0400 245.9 256.9
251(5) 0.0400 245.9 255.7
261(5) 0.0400 245.9 255.0
250(5) 0.0400 245.9 254.8
255(5) 0.0400 245.9 255.1
252(5) 0.0400 245.9 255.8
260(5) 0.0400 246.0 257.1
262(5) 0.0400 246.0 259.0
260(5) 0.0400 246.0 261.5
254(5) 0.0400 246.0 264.9
260(5) 0.0400 246.0 269.1
272(5) 0.0400 246.0 274.1
283(5) 0.0400 246.0 280.9
299(5) 0.0400 246.0 291.9
322(6) 0.02778 246.0 310.0
359(6) 0.02778 246.0 337.0
392(6) 0.02778 246.0 370.8
417(6) 0.02778 246.0 403.2
431(7) 0.02041 246.0 419.3
412(6) 0.02778 246.0 409.8
392(6) 0.02778 246.0 383.4
344(6) 0.02778 246.0 354.5
330(6) 0.02778 246.0 332.6
315(6) 0.02778 246.0 323.2
336(6) 0.02778 246.0 329.3
347(6) 0.02778 246.0 352.7
391(6) 0.02778 246.0 393.5
454(7) 0.02041 246.0 447.0
510(7) 0.02041 246.0 500.4
528(7) 0.02041 246.0 531.7
532(7) 0.02041 246.0 528.1
519(7) 0.02041 246.0 505.0
489(7) 0.02041 246.0 486.5
480(7) 0.02041 246.0 482.1
471(7) 0.02041 246.0 483.7
469(7) 0.02041 246.0 472.8
427(7) 0.02041 246.0 442.6
376(6) 0.02778 246.0 404.9
339(6) 0.02778 246.0 371.6
318(6) 0.02778 246.0 349.6
322(6) 0.02778 246.0 342.5
330(6) 0.02778 246.0 350.9
354(6) 0.02778 246.0 372.8
392(6) 0.02778 246.0 403.0
405(6) 0.02778 246.0 432.1
440(7) 0.02041 246.0 448.8
434(7) 0.02041 246.0 452.5
437(7) 0.02041 246.0 449.3
440(7) 0.02041 246.0 437.3
412(6) 0.02778 246.0 413.2
399(6) 0.02778 246.0 385.1
384(6) 0.02778 246.0 363.8
374(6) 0.02778 246.0 352.8
365(6) 0.02778 246.0 349.0
351(6) 0.02778 246.0 344.4
332(6) 0.02778 246.0 333.9
309(6) 0.02778 245.9 319.4
299(5) 0.0400 245.9 303.9
299(5) 0.0400 245.9 290.0
286(5) 0.0400 245.9 279.3
288(5) 0.0400 245.9 272.2
283(5) 0.0400 245.9 267.7
292(5) 0.0400 245.9 264.9
279(5) 0.0400 245.9 263.2
289(5) 0.0400 245.9 262.0
283(5) 0.0400 245.9 261.4
284(5) 0.0400 245.9 261.7
269(5) 0.0400 245.9 263.6
274(5) 0.0400 245.9 267.8
281(5) 0.0400 245.9 274.4
283(5) 0.0400 245.9 282.8
298(5) 0.0400 245.9 290.4
299(5) 0.0400 245.9 293.6
285(5) 0.0400 245.9 290.3
277(5) 0.0400 245.9 282.9
277(5) 0.0400 245.9 275.1
265(5) 0.0400 245.9 269.0
248(5) 0.0400 245.9 264.8
256(5) 0.0400 245.9 261.9
259(5) 0.0400 245.9 259.6
253(5) 0.0400 245.9 257.9
254(5) 0.0400 245.9 256.5
254(5) 0.0400 245.8 255.3
262(5) 0.0400 245.8 254.1
255(5) 0.0400 245.8 253.3
254(5) 0.0400 245.8 252.8
256(5) 0.0400 245.8 252.8
261(5) 0.0400 245.8 253.2
247(5) 0.0400 245.8 254.2
255(5) 0.0400 245.8 255.8
245(5) 0.0400 245.8 258.0
254(5) 0.0400 245.8 260.4
247(5) 0.0400 245.8 262.1
253(5) 0.0400 245.8 262.7
261(5) 0.0400 245.8 262.6
252(5) 0.0400 245.8 262.3
254(5) 0.0400 245.8 262.0
258(5) 0.0400 245.8 261.4
249(5) 0.0400 245.8 260.4
258(5) 0.0400 245.8 259.7
260(5) 0.0400 245.8 259.5
265(5) 0.0400 245.8 260.1
255(5) 0.0400 245.8 262.2
263(5) 0.0400 245.8 266.8
280(5) 0.0400 245.8 274.7
290(5) 0.0400 245.8 286.8
310(6) 0.02778 245.8 303.1
326(6) 0.02778 245.8 320.7
338(6) 0.02778 245.8 334.1
340(6) 0.02778 245.8 338.7
339(6) 0.02778 245.8 336.2
341(6) 0.02778 245.8 331.0
320(6) 0.02778 245.8 325.8
319(6) 0.02778 245.8 323.2
325(6) 0.02778 245.8 323.4
324(6) 0.02778 245.8 323.4
323(6) 0.02778 245.8 318.0
298(5) 0.0400 245.8 306.3
283(5) 0.0400 245.8 292.5
276(5) 0.0400 245.8 280.6
263(5) 0.0400 245.8 272.2
258(5) 0.0400 245.8 267.5
259(5) 0.0400 245.9 265.6
261(5) 0.0400 245.9 265.3
261(5) 0.0400 245.9 266.1
255(5) 0.0400 245.9 267.7
264(5) 0.0400 245.9 269.6
261(5) 0.0400 245.9 270.4
247(5) 0.0400 245.9 269.6
255(5) 0.0400 245.9 267.4
242(5) 0.0400 245.9 264.3
239(5) 0.0400 245.9 260.8
249(5) 0.0400 245.9 257.6
250(5) 0.0400 245.9 255.2
250(5) 0.0400 245.9 253.6
262(5) 0.0400 245.9 252.8
248(5) 0.0400 246.0 252.7
241(5) 0.0400 246.0 253.4
251(5) 0.0400 246.0 255.2
257(5) 0.0400 246.0 258.0
261(5) 0.0400 246.0 261.8
263(5) 0.0400 246.0 265.7
267(5) 0.0400 246.0 268.4
282(5) 0.0400 246.0 268.1
275(5) 0.0400 246.0 265.8
263(5) 0.0400 246.1 263.4
267(5) 0.0400 246.1 262.1
270(5) 0.0400 246.1 261.9
268(5) 0.0400 246.1 262.0
266(5) 0.0400 246.1 261.5
257(5) 0.0400 246.1 260.0
258(5) 0.0400 246.1 258.0
263(5) 0.0400 246.2 255.9
260(5) 0.0400 246.2 254.4
253(5) 0.0400 246.2 253.5
252(5) 0.0400 246.2 253.0
258(5) 0.0400 246.2 252.8
247(5) 0.0400 246.2 252.8
253(5) 0.0400 246.3 253.3
258(5) 0.0400 246.3 254.4
256(5) 0.0400 246.3 256.0
252(5) 0.0400 246.3 257.9
259(5) 0.0400 246.3 259.6
250(5) 0.0400 246.3 260.6
257(5) 0.0400 246.4 261.0
272(5) 0.0400 246.4 262.0
269(5) 0.0400 246.4 264.6
273(5) 0.0400 246.4 269.4
280(5) 0.0400 246.5 276.4
289(5) 0.0400 246.5 284.8
285(5) 0.0400 246.5 291.5
284(5) 0.0400 246.5 292.7
284(5) 0.0400 246.5 287.6
270(5) 0.0400 246.6 279.6
265(5) 0.0400 246.6 272.5
264(5) 0.0400 246.6 268.1
266(5) 0.0400 246.6 267.2
254(5) 0.0400 246.7 270.4
267(5) 0.0400 246.7 278.1
267(5) 0.0400 246.7 290.0
269(5) 0.0400 246.8 304.5
277(5) 0.0400 246.8 317.2
280(6) 0.02778 246.8 321.2
281(5) 0.0400 246.8 313.6
270(5) 0.0400 246.9 299.6
275(5) 0.0400 246.9 285.5
266(5) 0.0400 246.9 274.4
256(5) 0.0400 247.0 267.1
253(5) 0.0400 247.0 262.8
252(5) 0.0400 247.0 260.7
256(5) 0.0400 247.1 259.9
261(5) 0.0400 247.1 260.0
260(5) 0.0400 247.1 260.6
268(5) 0.0400 247.2 261.7
264(5) 0.0400 247.2 263.7
271(5) 0.0400 247.2 266.9
284(5) 0.0400 247.3 272.0
304(6) 0.02778 247.3 280.2
325(6) 0.02778 247.3 292.6
342(6) 0.02778 247.4 309.4
364(6) 0.02778 247.4 329.8
378(6) 0.02778 247.4 351.0
371(6) 0.02778 247.5 367.1
357(6) 0.02778 247.5 372.3
358(6) 0.02778 247.5 370.1
358(6) 0.02778 247.6 371.1
349(6) 0.02778 247.6 384.5
397(6) 0.02778 247.7 413.6
428(7) 0.02041 247.7 456.5
479(7) 0.02041 247.7 508.5
514(7) 0.02041 247.8 561.5
556(7) 0.02041 247.8 594.0
557(7) 0.02041 247.9 580.5
519(7) 0.02041 247.9 525.9
467(7) 0.02041 248.0 458.8
406(6) 0.02778 248.0 399.5
368(6) 0.02778 248.0 353.8
335(6) 0.02778 248.1 321.6
314(6) 0.02778 248.1 300.3
300(5) 0.0400 248.2 287.0
293(5) 0.0400 248.2 278.9
294(5) 0.0400 248.3 274.2
313(6) 0.02778 248.3 272.2
312(6) 0.02778 248.4 272.3
325(6) 0.02778 248.4 274.5
334(6) 0.02778 248.4 278.7
326(6) 0.02778 248.5 283.8
309(6) 0.02778 248.5 287.8
299(5) 0.0400 248.6 288.3
286(5) 0.0400 248.6 285.1
279(5) 0.0400 248.7 280.3
283(5) 0.0400 248.7 275.3
269(5) 0.0400 248.8 271.2
253(5) 0.0400 248.8 268.7
270(5) 0.0400 248.9 267.6
274(5) 0.0400 248.9 267.6
258(5) 0.0400 249.0 268.4
271(5) 0.0400 249.0 270.1
268(5) 0.0400 249.1 271.9
269(5) 0.0400 249.1 272.3
265(5) 0.0400 249.2 270.8
253(5) 0.0400 249.2 268.3
256(5) 0.0400 249.3 266.5
263(5) 0.0400 249.4 266.4
275(5) 0.0400 249.4 268.6
270(5) 0.0400 249.5 273.2
280(5) 0.0400 249.5 279.7
294(5) 0.0400 249.6 286.6
285(5) 0.0400 249.6 291.3
290(5) 0.0400 249.7 292.2
289(5) 0.0400 249.7 289.8
293(5) 0.0400 249.8 284.9
274(5) 0.0400 249.8 279.3
270(5) 0.0400 249.9 275.2
268(5) 0.0400 250.0 274.1
272(5) 0.0400 250.0 276.8
278(5) 0.0400 250.1 283.4
287(6) 0.02778 250.1 292.9
308(6) 0.02778 250.2 302.4
291(5) 0.0400 250.2 306.8
300(5) 0.0400 250.3 302.7
301(5) 0.0400 250.4 292.7
294(5) 0.0400 250.4 281.7
290(5) 0.0400 250.5 272.5
280(5) 0.0400 250.5 266.0
279(5) 0.0400 250.6 262.1
275(5) 0.0400 250.7 260.1
276(5) 0.0400 250.7 259.4
271(5) 0.0400 250.8 259.5
266(5) 0.0400 250.8 260.1
269(5) 0.0400 250.9 260.9
260(5) 0.0400 251.0 261.5
260(5) 0.0400 251.0 261.5
264(5) 0.0400 251.1 261.0
280(5) 0.0400 251.1 260.4
269(5) 0.0400 251.2 260.1
261(5) 0.0400 251.3 259.7
271(5) 0.0400 251.3 259.1
255(5) 0.0400 251.4 258.3
261(5) 0.0400 251.5 257.5
269(5) 0.0400 251.5 256.8
258(5) 0.0400 251.6 256.5
259(5) 0.0400 251.6 256.3
255(5) 0.0400 251.7 256.3
261(5) 0.0400 251.8 256.5
263(5) 0.0400 251.8 256.7
260(5) 0.0400 251.9 257.1
259(5) 0.0400 252.0 257.5
263(5) 0.0400 252.0 258.1
260(5) 0.0400 252.1 258.9
262(5) 0.0400 252.2 260.0
262(5) 0.0400 252.2 261.8
262(5) 0.0400 252.3 264.6
268(5) 0.0400 252.3 269.1
268(5) 0.0400 252.4 275.8
278(5) 0.0400 252.5 284.8
278(5) 0.0400 252.5 295.2
269(5) 0.0400 252.6 304.7
284(5) 0.0400 252.7 310.2
291(5) 0.0400 252.7 310.7
298(5) 0.0400 252.8 307.0
298(6) 0.02778 252.9 302.0
306(5) 0.0400 252.9 298.7
308(6) 0.02778 253.0 298.0
315(6) 0.02778 253.0 298.7
312(6) 0.02778 253.1 299.9
301(5) 0.0400 253.2 302.3
313(6) 0.02778 253.2 306.9
319(6) 0.02778 253.3 314.7
323(6) 0.02778 253.4 325.9
325(6) 0.02778 253.4 339.3
340(6) 0.02778 253.5 353.3
370(6) 0.02778 253.6 367.0
379(6) 0.02778 253.6 376.8
368(6) 0.02778 253.7 377.4
358(6) 0.02778 253.8 368.9
359(6) 0.02778 253.8 356.6
353(6) 0.02778 253.9 343.3
320(6) 0.02778 253.9 330.2
311(6) 0.02778 254.0 318.2
309(6) 0.02778 254.1 309.2
294(5) 0.0400 254.1 304.2
305(6) 0.02778 254.2 302.8
304(6) 0.02778 254.3 303.0
294(5) 0.0400 254.3 303.4
303(5) 0.0400 254.4 305.1
310(6) 0.02778 254.5 309.8
302(5) 0.0400 254.5 317.2
309(6) 0.02778 254.6 324.4
321(5) 0.0400 254.6 327.5
306(6) 0.02778 254.7 324.9
295(5) 0.0400 254.8 317.2
294(5) 0.0400 254.8 306.1
283(5) 0.0400 254.9 294.5
284(5) 0.0400 255.0 284.9
276(5) 0.0400 255.0 277.9
268(5) 0.0400 255.1 273.2
269(5) 0.0400 255.1 270.5
274(5) 0.0400 255.2 269.4
272(5) 0.0400 255.3 269.8
282(6) 0.02778 255.3 271.7
284(5) 0.0400 255.4 275.6
286(6) 0.02778 255.4 282.1
297(5) 0.0400 255.5 291.3
319(6) 0.02778 255.6 302.7
339(6) 0.02778 255.6 313.4
347(6) 0.02778 255.7 318.8
337(6) 0.02778 255.7 315.5
323(5) 0.0400 255.8 305.9
310(6) 0.02778 255.9 295.1
292(5) 0.0400 255.9 286.4
282(5) 0.0400 256.0 280.9
278(5) 0.0400 256.0 278.6
278(5) 0.0400 256.1 278.9
282(5) 0.0400 256.1 281.4
285(6) 0.02778 256.2 286.3
287(5) 0.0400 256.3 294.4
306(6) 0.02778 256.3 305.8
306(6) 0.02778 256.4 318.7
315(6) 0.02778 256.4 328.6
319(6) 0.02778 256.5 329.4
309(6) 0.02778 256.5 320.3
303(6) 0.02778 256.6 306.5
299(5) 0.0400 256.7 293.0
282(5) 0.0400 256.7 282.4
274(5) 0.0400 256.8 275.0
269(5) 0.0400 256.8 270.3
259(5) 0.0400 256.9 267.6
254(5) 0.0400 256.9 266.2
259(5) 0.0400 257.0 265.6
257(5) 0.0400 257.0 265.7
262(5) 0.0400 257.1 266.1
266(5) 0.0400 257.1 266.8
263(5) 0.0400 257.2 267.3
264(5) 0.0400 257.2 267.4
262(5) 0.0400 257.3 267.1
264(5) 0.0400 257.3 266.8
249(5) 0.0400 257.4 266.9
259(5) 0.0400 257.4 267.9
271(5) 0.0400 257.5 269.8
266(5) 0.0400 257.5 272.4
283(6) 0.02778 257.6 275.2
284(5) 0.0400 257.6 277.1
286(5) 0.0400 257.7 277.3
291(6) 0.02778 257.7 276.2
271(5) 0.0400 257.8 274.1
261(5) 0.0400 257.8 271.6
268(5) 0.0400 257.9 269.3
265(5) 0.0400 257.9 267.6
263(5) 0.0400 258.0 266.5
266(5) 0.0400 258.0 266.1
262(5) 0.0400 258.0 266.2
268(5) 0.0400 258.1 266.6
268(5) 0.0400 258.1 267.2
264(5) 0.0400 258.2 267.7
276(5) 0.0400 258.2 267.9
263(5) 0.0400 258.3 268.0
272(5) 0.0400 258.3 268.2
280(5) 0.0400 258.3 268.9
277(5) 0.0400 258.4 270.1
283(6) 0.02778 258.4 272.0
299(5) 0.0400 258.5 274.9
312(6) 0.02778 258.5 278.7
314(6) 0.02778 258.6 283.5
312(6) 0.02778 258.6 289.3
320(6) 0.02778 258.6 296.3
331(5) 0.0400 258.7 305.1
330(6) 0.02778 258.7 316.6
324(6) 0.02778 258.7 331.8
344(6) 0.02778 258.8 350.0
374(6) 0.02778 258.8 369.4
388(6) 0.02778 258.9 386.0
400(6) 0.02778 258.9 393.5
390(6) 0.02778 258.9 388.2
392(6) 0.02778 259.0 375.4
371(6) 0.02778 259.0 363.6
378(6) 0.02778 259.0 358.7
379(6) 0.02778 259.1 362.8
392(7) 0.02041 259.1 374.4
407(6) 0.02778 259.1 388.2
412(6) 0.02778 259.2 395.9
404(7) 0.02041 259.2 391.3
386(6) 0.02778 259.2 375.7
365(6) 0.02778 259.2 355.4
347(6) 0.02778 259.3 335.7
325(5) 0.0400 259.3 319.6
308(6) 0.02778 259.3 308.3
297(5) 0.0400 259.4 302.1
296(5) 0.0400 259.4 300.2
290(6) 0.02778 259.4 301.6
288(5) 0.0400 259.4 304.1
291(5) 0.0400 259.5 305.3
298(6) 0.02778 259.5 303.7
286(5) 0.0400 259.5 299.9
279(6) 0.02778 259.6 295.9
295(5) 0.0400 259.6 293.9
289(5) 0.0400 259.6 295.2
290(6) 0.02778 259.6 300.7
300(5) 0.0400 259.6 310.5
324(6) 0.02778 259.7 324.0
338(6) 0.02778 259.7 338.9
360(6) 0.02778 259.7 350.9
351(6) 0.02778 259.7 354.9
347(6) 0.02778 259.8 350.0
336(6) 0.02778 259.8 341.2
325(6) 0.02778 259.8 334.4
325(6) 0.02778 259.8 332.2
326(6) 0.02778 259.8 334.7
324(6) 0.02778 259.9 339.0
338(6) 0.02778 259.9 342.3
337(6) 0.02778 259.9 344.4
342(6) 0.02778 259.9 345.7
349(6) 0.02778 259.9 344.6
348(6) 0.02778 259.9 339.3
332(6) 0.02778 260.0 331.0
312(6) 0.02778 260.0 323.6
320(6) 0.02778 260.0 320.0
321(6) 0.02778 260.0 322.0
335(6) 0.02778 260.0 330.6
350(6) 0.02778 260.0 346.2
397(7) 0.02041 260.1 369.3
434(7) 0.02041 260.1 400.0
461(7) 0.02041 260.1 435.2
477(7) 0.02041 260.1 467.1
489(7) 0.02041 260.1 485.2
472(7) 0.02041 260.1 483.2
437(7) 0.02041 260.1 461.2
402(6) 0.02778 260.1 426.2
374(6) 0.02778 260.2 388.3
349(6) 0.02778 260.2 355.0
323(6) 0.02778 260.2 329.4
302(5) 0.0400 260.2 311.8
293(5) 0.0400 260.2 300.9
295(5) 0.0400 260.2 295.1
295(5) 0.0400 260.2 293.1
303(6) 0.02778 260.2 294.0
301(5) 0.0400 260.2 297.6
304(6) 0.02778 260.2 303.9
308(6) 0.02778 260.2 313.0
333(6) 0.02778 260.2 323.4
340(6) 0.02778 260.3 332.1
333(6) 0.02778 260.3 334.6
324(6) 0.02778 260.3 329.2
324(6) 0.02778 260.3 319.0
310(6) 0.02778 260.3 307.7
296(5) 0.0400 260.3 297.5
285(5) 0.0400 260.3 289.0
287(5) 0.0400 260.3 282.6
281(6) 0.02778 260.3 277.9
277(5) 0.0400 260.3 274.9
264(5) 0.0400 260.3 272.9
272(6) 0.02778 260.3 271.8
263(5) 0.0400 260.3 271.0
269(5) 0.0400 260.3 270.3
262(5) 0.0400 260.3 269.6
263(5) 0.0400 260.3 269.0
263(5) 0.0400 260.3 268.5
266(5) 0.0400 260.3 268.3
265(5) 0.0400 260.3 268.5
264(5) 0.0400 260.3 269.0
274(5) 0.0400 260.3 270.1
278(5) 0.0400 260.3 271.8
273(5) 0.0400 260.3 274.3
272(5) 0.0400 260.3 277.6
282(5) 0.0400 260.3 281.6
291(5) 0.0400 260.3 286.1
296(5) 0.0400 260.3 290.2
298(5) 0.0400 260.3 292.5
294(5) 0.0400 260.3 292.2
309(6) 0.02778 260.3 290.1
305(6) 0.02778 260.3 288.0
299(5) 0.0400 260.3 287.4
298(6) 0.02778 260.3 288.3
296(5) 0.0400 260.3 290.5
302(5) 0.0400 260.3 292.8
294(6) 0.02778 260.3 293.7
306(6) 0.02778 260.3 292.7
289(5) 0.0400 260.3 290.3
283(6) 0.02778 260.3 287.5
283(5) 0.0400 260.3 284.8
282(6) 0.02778 260.3 282.0
280(5) 0.0400 260.3 279.2
268(5) 0.0400 260.3 276.6
278(5) 0.0400 260.3 274.7
272(5) 0.0400 260.3 273.8
276(5) 0.0400 260.3 273.9
284(6) 0.02778 260.2 275.3
282(5) 0.0400 260.2 278.4
289(6) 0.02778 260.2 283.3
300(5) 0.0400 260.2 290.5
299(5) 0.0400 260.2 299.9
301(6) 0.02778 260.2 310.4
323(5) 0.0400 260.2 319.5
322(6) 0.02778 260.2 323.8
321(5) 0.0400 260.2 321.5
309(6) 0.02778 260.2 313.8
304(6) 0.02778 260.2 304.0
285(5) 0.0400 260.2 294.6
286(5) 0.0400 260.2 286.9
274(6) 0.02778 260.2 281.2
273(5) 0.0400 260.2 277.1
272(5) 0.0400 260.2 274.0
264(5) 0.0400 260.2 271.6
261(5) 0.0400 260.2 269.8
254(5) 0.0400 260.2 268.5
261(5) 0.0400 260.2 267.6
265(5) 0.0400 260.1 267.0
266(5) 0.0400 260.1 266.6
265(5) 0.0400 260.1 266.2
262(5) 0.0400 260.1 266.0
253(5) 0.0400 260.1 265.8
257(5) 0.0400 260.1 265.8
271(5) 0.0400 260.1 266.0
264(5) 0.0400 260.1 266.5
266(5) 0.0400 260.1 267.3
260(5) 0.0400 260.1 268.5
267(5) 0.0400 260.1 270.0
264(5) 0.0400 260.1 271.3
263(5) 0.0400 260.1 272.1
264(5) 0.0400 260.1 272.0
271(5) 0.0400 260.1 271.1
259(5) 0.0400 260.1 269.9
251(5) 0.0400 260.1 268.8
265(5) 0.0400 260.1 268.1
266(5) 0.0400 260.1 267.8
264(5) 0.0400 260.1 268.0
262(5) 0.0400 260.1 268.4
272(5) 0.0400 260.1 268.6
262(5) 0.0400 260.0 268.5
261(5) 0.0400 260.0 268.0
261(5) 0.0400 260.0 267.3
265(5) 0.0400 260.0 266.6
277(5) 0.0400 260.0 266.1
275(5) 0.0400 260.0 265.8
290(5) 0.0400 260.0 265.7
291(5) 0.0400 260.0 265.8
286(5) 0.0400 260.0 266.1
290(5) 0.0400 260.0 266.7
299(5) 0.0400 260.0 267.5
287(5) 0.0400 260.0 268.6
294(5) 0.0400 260.0 270.2
289(5) 0.0400 260.0 272.2
287(5) 0.0400 260.0 274.8
294(5) 0.0400 260.0 278.0
294(5) 0.0400 260.0 281.8
294(5) 0.0400 260.0 286.2
301(5) 0.0400 260.0 291.1
306(6) 0.02778 260.0 295.3
313(6) 0.02778 260.0 297.7
306(6) 0.02778 260.0 297.4
295(5) 0.0400 260.0 295.1
295(6) 0.02778 260.0 292.7
284(5) 0.0400 260.0 291.6
283(5) 0.0400 260.0 292.6
292(5) 0.0400 260.0 295.8
290(5) 0.0400 260.0 300.5
297(5) 0.0400 260.0 305.1
299(5) 0.0400 260.0 307.3
305(6) 0.02778 260.1 305.8
302(5) 0.0400 260.1 301.0
288(5) 0.0400 260.1 294.7
286(5) 0.0400 260.1 288.5
276(5) 0.0400 260.1 283.3
275(5) 0.0400 260.1 279.5
275(5) 0.0400 260.1 277.0
267(5) 0.0400 260.1 275.7
272(5) 0.0400 260.1 275.3
276(5) 0.0400 260.1 275.6
281(5) 0.0400 260.1 276.5
275(5) 0.0400 260.1 278.2
278(5) 0.0400 260.1 280.7
280(5) 0.0400 260.1 284.0
293(5) 0.0400 260.1 288.2
295(5) 0.0400 260.2 292.9
315(6) 0.02778 260.2 297.6
318(6) 0.02778 260.2 302.0
330(6) 0.02778 260.2 306.1
335(6) 0.02778 260.2 310.7
330(6) 0.02778 260.2 317.1
323(6) 0.02778 260.2 326.2
331(6) 0.02778 260.2 339.1
344(6) 0.02778 260.2 357.0
352(6) 0.02778 260.3 379.9
387(6) 0.02778 260.3 406.9
417(6) 0.02778 260.3 434.6
428(7) 0.02041 260.3 457.3
458(7) 0.02041 260.3 467.7
454(7) 0.02041 260.3 462.5
431(7) 0.02041 260.3 445.5
428(7) 0.02041 260.4 423.3
403(6) 0.02778 260.4 400.7
371(6) 0.02778 260.4 380.0
337(6) 0.02778 260.4 362.3
340(6) 0.02778 260.4 348.6
323(6) 0.02778 260.4 339.5
312(6) 0.02778 260.5 335.3
319(6) 0.02778 260.5 336.4
322(6) 0.02778 260.5 343.5
345(6) 0.02778 260.5 357.5
361(6) 0.02778 260.5 379.8
404(6) 0.02778 260.6 411.4
437(7) 0.02041 260.6 452.5
494(7) 0.02041 260.6 500.8
570(8) 0.01563 260.6 550.7
612(8) 0.01563 260.7 593.7
643(8) 0.01563 260.7 623.8
674(8) 0.01563 260.7 642.9
697(8) 0.01563 260.7 656.1
679(8) 0.01563 260.8 664.6
670(8) 0.01563 260.8 662.1
652(8) 0.01563 260.8 640.4
609(8) 0.01563 260.8 599.6
565(8) 0.01563 260.9 548.6
526(7) 0.02041 260.9 497.1
469(7) 0.02041 260.9 451.2
437(7) 0.02041 261.0 413.4
403(6) 0.02778 261.0 383.7
380(6) 0.02778 261.0 361.4
348(6) 0.02778 261.0 345.0
333(6) 0.02778 261.1 333.5
322(6) 0.02778 261.1 326.1
318(6) 0.02778 261.1 322.1
322(6) 0.02778 261.2 320.5
319(6) 0.02778 261.2 320.2
313(6) 0.02778 261.2 320.2
311(6) 0.02778 261.3 319.6
314(6) 0.02778 261.3 319.0
324(6) 0.02778 261.3 319.0
330(6) 0.02778 261.4 320.1
324(6) 0.02778 261.4 321.6
331(6) 0.02778 261.5 322.4
337(6) 0.02778 261.5 320.8
327(6) 0.02778 261.5 316.6
320(6) 0.02778 261.6 310.6
313(6) 0.02778 261.6 304.3
310(6) 0.02778 261.7 298.8
308(6) 0.02778 261.7 294.7
301(5) 0.0400 261.7 292.0
293(5) 0.0400 261.8 290.8
287(5) 0.0400 261.8 290.6
284(5) 0.0400 261.9 291.0
289(5) 0.0400 261.9 291.6
286(5) 0.0400 262.0 292.3
282(5) 0.0400 262.0 293.8
282(5) 0.0400 262.1 296.5
302(5) 0.0400 262.1 301.1
298(5) 0.0400 262.1 308.1
315(6) 0.02778 262.2 317.8
330(6) 0.02778 262.2 330.0
344(6) 0.02778 262.3 344.2
361(6) 0.02778 262.3 359.7
370(6) 0.02778 262.4 375.7
384(6) 0.02778 262.4 390.8
384(6) 0.02778 262.5 401.9
392(6) 0.02778 262.5 405.0
384(6) 0.02778 262.6 397.9
363(6) 0.02778 262.7 382.7
343(6) 0.02778 262.7 363.6
320(6) 0.02778 262.8 344.7
317(6) 0.02778 262.8 328.3
300(5) 0.0400 262.9 315.4
293(5) 0.0400 262.9 306.3
290(5) 0.0400 263.0 300.5
276(5) 0.0400 263.0 297.1
283(5) 0.0400 263.1 295.4
280(5) 0.0400 263.2 294.4
285(5) 0.0400 263.2 293.5
278(5) 0.0400 263.3 292.2
284(5) 0.0400 263.3 290.4
279(5) 0.0400 263.4 288.2
278(5) 0.0400 263.5 285.8
282(5) 0.0400 263.5 283.3
275(5) 0.0400 263.6 280.9
277(5) 0.0400 263.7 278.8
274(5) 0.0400 263.7 277.1
265(5) 0.0400 263.8 275.9
274(5) 0.0400 263.9 275.3
284(5) 0.0400 263.9 275.2
281(5) 0.0400 264.0 275.6
279(5) 0.0400 264.1 276.7
272(5) 0.0400 264.1 278.5
268(5) 0.0400 264.2 280.9
277(5) 0.0400 264.3 283.7
280(5) 0.0400 264.3 286.7
277(5) 0.0400 264.4 289.2
280(5) 0.0400 264.5 290.6
285(5) 0.0400 264.6 290.5
269(5) 0.0400 264.6 288.7
277(5) 0.0400 264.7 286.1
273(5) 0.0400 264.8 283.1
271(5) 0.0400 264.9 280.2
268(5) 0.0400 264.9 277.8
264(5) 0.0400 265.0 276.0
274(5) 0.0400 265.1 274.7
264(5) 0.0400 265.2 273.8
262(5) 0.0400 265.2 273.3
271(5) 0.0400 265.3 273.1
272(5) 0.0400 265.4 273.2
276(5) 0.0400 265.5 273.5
269(5) 0.0400 265.6 274.0
277(5) 0.0400 265.7 274.8
284(5) 0.0400 265.7 275.9
299(5) 0.0400 265.8 277.3
310(6) 0.02778 265.9 279.1
291(5) 0.0400 266.0 281.4
308(6) 0.02778 266.1 284.1
302(5) 0.0400 266.2 287.5
306(6) 0.02778 266.3 291.5
319(6) 0.02778 266.3 296.2
314(6) 0.02778 266.4 301.9
323(6) 0.02778 266.5 308.5
329(6) 0.02778 266.6 315.5
344(6) 0.02778 266.7 322.0
342(6) 0.02778 266.8 326.6
337(6) 0.02778 266.9 328.3
327(6) 0.02778 267.0 326.9
331(6) 0.02778 267.1 323.2
328(6) 0.02778 267.2 318.4
316(6) 0.02778 267.3 313.3
311(6) 0.02778 267.4 308.7
309(6) 0.02778 267.5 304.9
304(6) 0.02778 267.6 302.1
298(5) 0.0400 267.7 300.3
304(6) 0.02778 267.8 299.4
292(5) 0.0400 267.9 299.4
297(5) 0.0400 268.0 300.5
308(6) 0.02778 268.1 303.1
321(6) 0.02778 268.2 307.2
330(6) 0.02778 268.3 312.5
340(6) 0.02778 268.4 318.6
348(6) 0.02778 268.5 324.6
352(6) 0.02778 268.6 329.7
349(6) 0.02778 268.7 333.2
356(6) 0.02778 268.8 335.2
354(6) 0.02778 268.9 335.6
360(6) 0.02778 269.0 335.0
347(6) 0.02778 269.2 334.2
352(6) 0.02778 269.3 333.7
337(6) 0.02778 269.4 333.5
329(6) 0.02778 269.5 333.3
325(6) 0.02778 269.6 332.3
323(5) 0.0400 269.7 329.9
328(6) 0.02778 269.8 325.6
311(6) 0.02778 270.0 320.1
308(6) 0.02778 270.1 314.0
306(6) 0.02778 270.2 308.1
297(5) 0.0400 270.3 302.9
298(5) 0.0400 270.4 298.7
305(6) 0.02778 270.6 295.6
305(6) 0.02778 270.7 293.8
293(5) 0.0400 270.8 293.1
298(5) 0.0400 270.9 293.1
292(5) 0.0400 271.1 293.6
299(5) 0.0400 271.2 294.3
292(5) 0.0400 271.3 295.0
296(5) 0.0400 271.4 295.8
300(5) 0.0400 271.6 296.8
309(6) 0.02778 271.7 298.4
310(6) 0.02778 271.8 300.5
303(6) 0.02778 272.0 303.0
309(6) 0.02778 272.1 305.6
314(6) 0.02778 272.2 307.8
319(6) 0.02778 272.4 309.2
313(6) 0.02778 272.5 309.8
306(6) 0.02778 272.6 310.0
308(6) 0.02778 272.8 310.2
306(6) 0.02778 272.9 311.0
313(6) 0.02778 273.1 312.4
313(6) 0.02778 273.2 314.4
313(6) 0.02778 273.4 316.9
325(6) 0.02778 273.5 319.4
318(6) 0.02778 273.6 321.6
329(6) 0.02778 273.8 323.0
326(6) 0.02778 273.9 323.5
327(6) 0.02778 274.1 323.3
326(6) 0.02778 274.2 323.0
323(6) 0.02778 274.4 323.3
334(6) 0.02778 274.5 324.4
339(6) 0.02778 274.7 326.8
336(6) 0.02778 274.8 330.4
331(6) 0.02778 275.0 335.1
338(6) 0.02778 275.1 340.2
350(6) 0.02778 275.3 344.9
344(6) 0.02778 275.5 348.5
367(6) 0.02778 275.6 350.6
359(6) 0.02778 275.8 351.3
367(6) 0.02778 275.9 350.8
371(6) 0.02778 276.1 348.8
349(6) 0.02778 276.3 345.0
351(6) 0.02778 276.4 339.4
350(6) 0.02778 276.6 332.6
342(6) 0.02778 276.8 325.4
325(6) 0.02778 276.9 318.6
317(6) 0.02778 277.1 312.5
306(6) 0.02778 277.3 307.3
306(6) 0.02778 277.4 302.9
304(6) 0.02778 277.6 299.3
301(5) 0.0400 277.8 296.3
287(5) 0.0400 278.0 293.8
299(5) 0.0400 278.1 291.6
287(5) 0.0400 278.3 289.9
287(5) 0.0400 278.5 288.5
287(5) 0.0400 278.7 287.4
291(5) 0.0400 278.9 286.6
280(5) 0.0400 279.0 286.0
291(5) 0.0400 279.2 285.5
286(5) 0.0400 279.4 285.1
285(5) 0.0400 279.6 284.9
287(5) 0.0400 279.8 284.8
291(5) 0.0400 280.0 284.8
293(5) 0.0400 280.2 284.8
298(5) 0.0400 280.3 284.9
294(5) 0.0400 280.5 285.0
275(5) 0.0400 280.7 285.2
276(5) 0.0400 280.9 285.4
283(5) 0.0400 281.1 285.6
291(5) 0.0400 281.3 285.9
289(6) 0.02778 281.5 286.3
287(5) 0.0400 281.7 286.7
284(5) 0.0400 281.9 287.3
286(5) 0.0400 282.1 287.9
289(5) 0.0400 282.3 288.6
290(5) 0.0400 282.5 289.6
288(5) 0.0400 282.7 290.7
285(5) 0.0400 282.9 292.0
285(5) 0.0400 283.1 293.5
284(5) 0.0400 283.3 295.1
287(5) 0.0400 283.5 296.7
298(5) 0.0400 283.7 298.2
294(5) 0.0400 284.0 299.2
298(5) 0.0400 284.2 299.6
287(5) 0.0400 284.4 299.4
299(5) 0.0400 284.6 298.8
294(5) 0.0400 284.8 297.8
302(5) 0.0400 285.0 296.8
298(5) 0.0400 285.2 295.8
304(6) 0.02778 285.5 295.0
285(5) 0.0400 285.7 294.5
294(5) 0.0400 285.9 294.2
303(6) 0.02778 286.1 294.2
297(5) 0.0400 286.3 294.5
299(5) 0.0400 286.6 294.9
297(5) 0.0400 286.8 295.6
298(5) 0.0400 287.0 296.5
294(5) 0.0400 287.2 297.6
290(5) 0.0400 287.5 298.9
304(6) 0.02778 287.7 300.4
291(5) 0.0400 287.9 301.9
301(5) 0.0400 288.2 303.5
299(5) 0.0400 288.4 304.9
303(6) 0.02778 288.6 306.1
294(5) 0.0400 288.9 306.9
301(5) 0.0400 289.1 307.2
296(5) 0.0400 289.3 307.2
299(5) 0.0400 289.6 307.1
299(5) 0.0400 289.8 306.9
302(5) 0.0400 290.0 306.9
305(6) 0.02778 290.3 307.2
304(6) 0.02778 290.5 307.9
296(5) 0.0400 290.7 309.1
296(5) 0.0400 291.0 310.8
300(5) 0.0400 291.2 312.7
317(6) 0.02778 291.5 314.7
311(6) 0.02778 291.7 316.5
317(6) 0.02778 291.9 317.8
319(6) 0.02778 292.2 318.3
317(6) 0.02778 292.4 318.0
310(6) 0.02778 292.7 317.0
319(6) 0.02778 292.9 315.5
315(6) 0.02778 293.2 313.9
310(6) 0.02778 293.4 312.4
324(6) 0.02778 293.7 311.0
307(6) 0.02778 293.9 310.0
308(6) 0.02778 294.1 309.5
306(6) 0.02778 294.4 309.3
305(6) 0.02778 294.6 309.7
295(5) 0.0400 294.9 310.5
307(6) 0.02778 295.1 311.8
305(6) 0.02778 295.4 313.5
315(6) 0.02778 295.6 315.8
315(6) 0.02778 295.9 318.6
313(6) 0.02778 296.1 322.1
310(6) 0.02778 296.4 326.4
323(6) 0.02778 296.6 331.6
331(6) 0.02778 296.9 337.8
347(6) 0.02778 297.1 345.0
343(6) 0.02778 297.4 353.1
352(6) 0.02778 297.6 361.9
368(6) 0.02778 297.9 370.9
382(6) 0.02778 298.1 379.5
387(6) 0.02778 298.3 386.9
383(6) 0.02778 298.6 391.9
392(7) 0.02041 298.8 393.9
377(6) 0.02778 299.1 392.5
365(6) 0.02778 299.3 388.1
369(6) 0.02778 299.6 381.5
359(6) 0.02778 299.8 373.7
365(6) 0.02778 300.1 365.7
341(6) 0.02778 300.3 358.2
334(6) 0.02778 300.5 351.9
334(6) 0.02778 300.8 347.1
335(6) 0.02778 301.0 344.0
346(6) 0.02778 301.3 342.7
335(6) 0.02778 301.5 343.2
346(6) 0.02778 301.7 345.2
355(6) 0.02778 302.0 348.7
355(6) 0.02778 302.2 353.2
365(6) 0.02778 302.5 358.4
368(6) 0.02778 302.7 363.9
374(6) 0.02778 302.9 369.0
387(6) 0.02778 303.2 373.2
374(6) 0.02778 303.4 376.0
383(6) 0.02778 303.6 377.0
370(6) 0.02778 303.8 376.2
380(6) 0.02778 304.1 373.6
370(6) 0.02778 304.3 369.5
369(6) 0.02778 304.5 364.3
361(6) 0.02778 304.7 358.5
357(6) 0.02778 305.0 352.5
331(6) 0.02778 305.2 346.8
336(6) 0.02778 305.4 341.7
330(6) 0.02778 305.6 337.2
341(6) 0.02778 305.8 333.4
332(6) 0.02778 306.0 330.3
333(6) 0.02778 306.2 327.9
324(6) 0.02778 306.4 325.9
318(6) 0.02778 306.6 324.3
339(6) 0.02778 306.8 323.1
315(6) 0.02778 307.0 322.1
335(6) 0.02778 307.2 321.4
326(6) 0.02778 307.4 321.0
326(6) 0.02778 307.6 320.8
317(6) 0.02778 307.8 320.8
325(6) 0.02778 308.0 321.1
324(6) 0.02778 308.2 321.8
326(6) 0.02778 308.4 322.8
336(6) 0.02778 308.6 324.3
327(6) 0.02778 308.7 326.3
336(6) 0.02778 308.9 328.8
330(6) 0.02778 309.1 332.0
347(6) 0.02778 309.3 335.7
337(6) 0.02778 309.4 340.1
343(6) 0.02778 309.6 345.0
348(6) 0.02778 309.7 350.3
365(6) 0.02778 309.9 355.7
370(6) 0.02778 310.1 360.9
373(6) 0.02778 310.2 365.5
383(6) 0.02778 310.4 369.1
367(6) 0.02778 310.5 371.2
383(6) 0.02778 310.6 371.5
380(6) 0.02778 310.8 370.2
374(6) 0.02778 310.9 367.3
368(6) 0.02778 311.1 363.5
358(6) 0.02778 311.2 359.0
344(6) 0.02778 311.3 354.3
335(6) 0.02778 311.4 349.9
343(6) 0.02778 311.5 345.8
337(6) 0.02778 311.7 342.4
332(6) 0.02778 311.8 339.7
329(6) 0.02778 311.9 337.8
346(6) 0.02778 312.0 336.6
357(6) 0.02778 312.1 336.3
358(6) 0.02778 312.2 336.6
372(6) 0.02778 312.3 337.7
371(6) 0.02778 312.4 339.4
385(6) 0.02778 312.5 341.8
396(6) 0.02778 312.5 344.7
384(7) 0.02041 312.6 348.2
385(6) 0.02778 312.7 352.2
405(6) 0.02778 312.8 356.4
419(6) 0.02778 312.8 360.8
412(6) 0.02778 312.9 364.9
410(6) 0.02778 313.0 368.4
404(6) 0.02778 313.0 371.0
381(6) 0.02778 313.1 372.2
373(6) 0.02778 313.1 372.0
375(6) 0.02778 313.2 370.4
360(6) 0.02778 313.2 367.6
365(6) 0.02778 313.3 364.2
354(6) 0.02778 313.3 360.4
343(6) 0.02778 313.4 356.5
338(6) 0.02778 313.4 353.0
335(6) 0.02778 313.4 349.9
328(6) 0.02778 313.5 347.3
334(6) 0.02778 313.5 345.4
326(6) 0.02778 313.5 343.9
323(6) 0.02778 313.5 343.0
328(6) 0.02778 313.5 342.4
329(6) 0.02778 313.6 342.0
320(6) 0.02778 313.6 341.7
332(6) 0.02778 313.6 341.3
324(6) 0.02778 313.6 340.9
324(6) 0.02778 313.6 340.3
325(6) 0.02778 313.6 339.7
327(6) 0.02778 313.6 339.1
307(6) 0.02778 313.6 338.6
316(6) 0.02778 313.6 338.1
318(6) 0.02778 313.6 337.7
323(6) 0.02778 313.6 337.6
317(6) 0.02778 313.6 337.6
318(6) 0.02778 313.6 338.0
333(6) 0.02778 313.7 338.6
332(6) 0.02778 313.7 339.5
337(6) 0.02778 313.7 340.7
319(6) 0.02778 313.7 342.2
340(6) 0.02778 313.7 343.8
346(6) 0.02778 313.7 345.5
331(6) 0.02778 313.7 347.3
339(6) 0.02778 313.7 349.0
325(6) 0.02778 313.7 350.8
354(6) 0.02778 313.7 352.5
349(6) 0.02778 313.7 354.3
356(6) 0.02778 313.8 356.1
339(6) 0.02778 313.8 358.0
352(6) 0.02778 313.8 360.0
365(6) 0.02778 313.9 361.8
356(6) 0.02778 313.9 363.4
358(7) 0.02041 314.0 364.6
369(6) 0.02778 314.0 365.1
363(6) 0.02778 314.1 364.8
359(6) 0.02778 314.1 363.7
360(6) 0.02778 314.2 361.7
360(6) 0.02778 314.3 359.0
368(6) 0.02778 314.4 355.8
369(6) 0.02778 314.5 352.3
370(6) 0.02778 314.6 348.8
367(6) 0.02778 314.7 345.3
358(7) 0.02041 314.9 342.1
364(7) 0.02041 315.0 339.3
364(7) 0.02041 315.2 336.8
346(7) 0.02041 315.3 334.8
342(7) 0.02041 315.5 333.2
341(7) 0.02041 315.7 332.0
334(6) 0.02778 315.9 331.2
340(7) 0.02041 316.2 330.8
338(7) 0.02041 316.4 330.7
335(6) 0.02778 316.7 330.9
335(6) 0.02778 317.0 331.2
333(6) 0.02778 317.3 331.8
337(6) 0.02778 317.6 332.4
331(6) 0.02778 317.9 333.2
328(6) 0.02778 318.3 333.9
337(6) 0.02778 318.7 334.7
333(6) 0.02778 319.1 335.5
335(6) 0.02778 319.6 336.3
330(6) 0.02778 320.0 337.0
326(6) 0.02778 320.6 337.6
333(6) 0.02778 321.1 338.0
338(6) 0.02778 321.6 338.4
326(6) 0.02778 322.2 338.6
314(6) 0.02778 322.9 338.7
328(6) 0.02778 323.5 338.7
325(7) 0.02041 324.2 338.7
334(7) 0.02041 325.0 338.8
345(7) 0.02041 325.7 338.8
336(7) 0.02041 326.5 338.9
354(7) 0.02041 327.4 339.2
346(7) 0.02041 328.3 339.6
348(7) 0.02041 329.2 340.1
358(7) 0.02041 330.2 340.8
353(7) 0.02041 331.3 341.7
341(7) 0.02041 332.4 342.8
348(7) 0.02041 333.5 344.0
351(7) 0.02041 334.7 345.4
345(7) 0.02041 335.9 347.0
352(7) 0.02041 337.3 348.8
351(7) 0.02041 338.6 350.8
341(7) . . .
338(7) . . .
352(7) . . .
353(7) . . .
337(7) . . .
342(7) . . .
344(7) . . .
333(7) . . .
323(7) . . .
340(7) . . .
327(7) . . .
333(7) . . .
312(7) . . .
327(7) . . .
327(7) . . .
315(7) . . .
309(7) . . .
307(7) . . .
285(7) . . .
299(7) . . .
301(7) . . .
290(7) . . .
282(7) . . .
279(7) . . .
278(7) . . .
276(7) . . .
266(7) . . .
269(7) . . .
262(7) . . .
261(7) . . .
257(7) . . .
248(6) . . .
246(6) . . .
237(6) . . .
236(6) . . .
231(7) . . .
222(7) . . .
233(7) . . .
230(7) . . .
223(7) . . .
214(7) . . .
212(7) . . .
213(7) . . .
208(6) . . .
205(6) . . .
195(6) . . .
203(6) . . .
189(6) . . .
200(6) . . .
184(6) . . .
185(6) . . .
174(6) . . .
177(6) . . .
173(6) . . .
172(6) . . .
162(6) . . .
173(6) . . .
163(6) . . .
161(6) . . .
150(5) . . .
143(6) . . .
127(6) . . .
142(6) . . .
135(6) . . .
128(6) . . .
122(6) . . .
133(6) . . .
132(6) . . .
131(6) . . .
117(5) . . .
116(5) . . .
125(6) . . .
125(6) . . .
118(5) . . .
116(5) . . .
122(6) . . .
122(6) . . .
122(6) . . .
122(6) . . .
114(5) . . .
124(6) . . .
116(5) . . .
124(6) . . .
118(5) . . .
115(5) . . .
117(6) . . .
113(6) . . .
108(6) . . .
112(6) . . .
102(6) . . .
112(6) . . .
111(6) . . .
96(6) . . .
120(6) . . .
117(6) . . .
104(6) . . .
106(6) . . .
109(6) . . .
105(6) . . .
113(6) . . .
96(6) . . .
105(6) . . .
107(6) . . .
109(6) . . .
105(6) . . .
108(6) . . .
108(6) . . .
88(5) . . .
111(6) . . .
109(6) . . .
102(7) . . .
99(7) . . .
98(7) . . .
113(8) . . .
104(7) . . .
108(7) . . .
111(7) . . .
99(7) . . .
97(7) . . .
94(7) . . .
103(7) . . .
100(7) . . .
96(7) . . .
96(7) . . .
107(7) . . .
97(7) . . .
99(7) . . .
98(7) . . .
100(7) . . .
89(7) . . .
107(7) . . .
100(7) . . .
99(7) . . .
107(7) . . .
102(7) . . .
102(10) . . .
101(10) . . .
99(10) . . .
93(10) . . .
97(10) . . .
98(10) . . .
111(11) . . .
96(10) . . .
99(10) . . .
109(10) . . .
108(10) . . .
106(10) . . .
110(10) . . .
84(9) . . .
103(10) . . .
122(11) . . .
116(11) . . .
93(10) . . .
103(10) . . .
91(10) . . .
116(11) . . .
111(11) . . .
95(10) . . .
117(11) . . .
